Manufacturing and workshop practices have become important in the industrial envi-
ronment to produce products for the service of mankind. The knowledge of manufacturing
practices is highly essential for all engineers and technocrats for familiarizing themselves
with modern concepts of manufacturing technologies. The basic need is to provide theoreti-
cal and practical knowledge of manufacturing processes and workshop technology to all the
engineering students. Therefore, an attempt has been made through this book to present
both the theoretical and practical knowledge of these subjects. Considering the general
needs of engineering students in the country and the fact that they hardly get any exposure
to hand tools, equipments, machines and manufacturing setups, a basic course in manufac-
turing science remains a core subject for all the branches of engineering. This book covers
most of the syllabus of manufacturing processes/technology, workshop technology and work-
shop practices for engineering diploma and degree classes prescribed by different universi-
ties and state technical boards. While preparing the manuscript of this book, the examina-
tion requirements of the engineering students have also been kept in mind. The book is
written in very simple language so that even an average student can easily grasp the subject
matter. Some comparisons have been given in tabular form and the stress has been given
on figures for better understanding of tools, equipments, machines and manufacturing set-
ups used in various manufacturing shops. The contents include exposure to bench work and
fitting, smithy and forging, sheet metal work, wood and wood working, casting, welding and
machine shop practices. At the end of each chapter, a number of questions have been
provided for testing the student’s understanding about the concept of the subject. The whole
text has been organized in twenty six chapters.
The first chapter presents the brief introduction of the subject with modern concepts
of manufacturing technology needed for the competitive industrial environment. Chapter 2
provides the necessary details of plant and shop layouts. General industrial safety measures
to be followed in various manufacturing shops are described in detail in chapter 3.
Chapters 4–8 provide necessary details regarding fundamentals of ferrous materials,
non-ferrous materials, melting furnaces, properties and testing of engineering materials and
heat treatment of metals and alloys.
Chapters 9–13 describe various tools, equipments and processes used in various shops
such as carpentry, pattern making, mold and core making, foundry shop. Special casting
methods and casting defects are also explained at length.
Chapters 14–16 provide basic knowledge of mechanical working of metals. Fundamental
concepts related to forging work and other mechanical working processes (hot and cold
working) have been discussed at length with neat sketches.
Chapter 17 provides necessary details of various welding and allied joining processes
such as gas welding, arc welding, resistance welding, solid state welding, thermochemical
welding, brazing and soldering.
Chapters 18–19 describe sheet metal and fitting work in detail. Various kinds of hand
tools and equipments used in sheet metal and fitting shops have been described using neat
Chapters 20–24 provide construction and operational details of various machine tools
namely lathe, drilling machine, shaper, planer, slotter, and milling machine with the help
of neat diagrams.
Chapter 25 deals with technique of manufacturing of products with powder metallurgy.
The last chapter of the book discusses the basic concepts of quality control and inspection
techniques used in manufacturing industries.
The author strongly believes that the book would serve not only as a text book for the
students of engineering curriculum but would also provide reference material to engineers
working in manufacturing industries.
Although every care has been taken to check misprints and mistakes, yet it is difficult
to claim perfection. Any errors, omissions and suggestions for improvement of this volume
will be thankfully acknowledged and included in the next edition.
On completion of the book ‘Introduction to Basic Manufacturing
Processes and Workshop Technology’, foremost I acknowledge the grace
of God; and the blessing of my father late Sh. Sada Ram, my mother Smt.
Sona Devi, my respected teacher Prof. G.S. Sekhon and my elders. I wish to
acknowledge my sincere thanks to Sh. Shailendra Kumar, lecturer in Hindu
College of Engineering, Sonepat, Haryana for assisting me at various stages
during preparation of the manuscript. I also acknowledge the students and
colleagues whose association has given me the experience of teaching this
and related subjects and hence the manuscript of this book could be possible.
I am very happy to record my sense of gratitude to my wife Promilla, daugh-
ter Swati and son Ravi Kant for their patience, understanding and moral
support without which it would have not been possible for me to complete
Finally, I am thankful to our publisher, New Age International (P) Ltd.
Publishers for bringing out the book in a record time and such a nice format.
Manufacturing is the backbone of any industrialized nation. Manufacturing and technical staff
in industry must know the various manufacturing processes, materials being processed, tools
and equipments for manufacturing different components or products with optimal process
plan using proper precautions and specified safety rules to avoid accidents. Beside above, all
kinds of the future engineers must know the basic requirements of workshop activities in
term of man, machine, material, methods, money and other infrastructure facilities needed
to be positioned properly for optimal shop layouts or plant layout and other support services
effectively adjusted or located in the industry or plant within a well planned manufacturing
The complete understanding of basic manufacturing processes and workshop technology
is highly difficult for any one to claim expertise over it. The study deals with several aspects
of workshops practices also for imparting the basic working knowledge of the different
engineering materials, tools, equipments, manufacturing processes, basic concepts of electro-
mechanical controls of machine tools, production criteria’s, characteristics and uses of various
testing instruments and measuring or inspecting devices for checking components or products
manufactured in various manufacturing shops in an industrial environment. It also describes
and demonstrates the use of different hand tools (measuring, marking, holding and supporting
tools, cutting etc.), equipments, machinery and various methods of manufacturing that facilitate
shaping or forming the different existing raw materials into suitable usable forms. It deals
with the study of industrial environment which involves the practical knowledge in the area
of ferrous and non ferrous materials, their properties and uses. It should provide the knowledge
of basic workshop processes namely bench work and fitting, sheet metal, carpentry, pattern
making, mould making, foundry, smithy, forging, metal working and heat treatment, welding,
fastening, machine shop, surface finishing and coatings, assembling inspection and quality
control. It emphasizes on basic knowledge regarding composition, properties and uses of
different raw materials, various production processes, replacement of or improvement over
a large number of old processes, new and compact designs, better accuracy in dimensions,
quicker methods of production, better surface finishes, more alternatives to the existing
materials and tooling systems, automatic and numerical control systems, higher mechanization
and greater output.
2 Introduction to Basic Manufacturing Processes and Workshop Technology
1.2 SCOPE OF STUDY
Today’s competitive manufacturing era of high industrial development and research, is being
called the age of mechanization, automation and computer integrated manufacturing. Due to
new researches in the manufacturing field, the advancement has come to this extent that
every different aspect of this technology has become a full-fledged fundamental and advanced
study in itself. This has led to introduction of optimized design and manufacturing of new
products. New developments in manufacturing areas are deciding to transfer more skill to the
machines for considerably reduction of manual labor. The scope of the subject of workshop
technology and manufacturing practices is a extremely wide as it specifies the need of greater
care for man, machine, material and other equipments involving higher initial investment by
using proper safety rule and precautions. The through and deep knowledge in the course of
study of this important subject is therefore becoming essential for all kinds of engineers to
have sound foundation in their profession. Therefore the course of study of this subject
provides a good theoretical background and a sound practical knowledge to the engineering
students and workshop staff. One should also be aware of the following terms for better
understanding of the scope of the study
1.3 MANUFACTURING ENGINEERING
Manufacturing is derived from the Latin word manufactus, means made by hand. In modern
context it involves making products from raw material by using various processes, by making
use of hand tools, machinery or even computers. It is therefore a study of the processes
required to make parts and to assemble them in machines. Process Engineering, in its
application to engineering industries, shows how the different problems related to development
of various machines may be solved by a study of physical, chemical and other laws governing
the manufacturing process. The study of manufacturing reveals those parameters which can
be most efficiently being influenced to increase production and raise its accuracy. Advance
manufacturing engineering involves the following concepts—
1. Process planning.
2. Process sheets.
3. Route sheets.
5. Cutting tools, machine tools (traditional, numerical control (NC), and computerized
numerical control (CNC).
6. Jigs and Fixtures.
7. Dies and Moulds.
8. Manufacturing Information Generation.
9. CNC part programs.
10. Robot programmers.
11. Flexible Manufacturing Systems (FMS), Group Technology (GT) and Computer
integrated manufacturing (CIM).
1.4 PRODUCTION PROCESS
It is the process followed in a plant for converting semi- finished products or raw materials
into finished products or raw materials into finished products. The art of converting raw
material into finished goods with application of different types of tools, equipments, machine
tools, manufacturing set ups and manufacturing processes, is known as production. Generally
there are three basic types of production system that are given as under.
1. Job production
2. Batch production
3. Mass production
Job production comprises of an operator or group of operators to work upon a single job
and complete it before proceeding to the next similar or different job. The production
requirement in the job production system is extremely low. It requires fixed type of layout
for developing same products.
Manufacturing of products (less in number say 200 to 800) with variety of similar parts
with very little variation in size and shape is called batch production. Whenever the production
of batch is over, the same manufacturing facility is used for production of other batch product
or items. The batch may be for once or of periodical type or of repeated kinds after some
irregular interval. Such manufacturing concepts are leading to GT and FMS technology.
Manufacturing of products in this case requires process or functional layout.
Where as mass production involves production of large number of identical products (say
more than 50000) that needs line layout type of plant layout which is highly rigid type and
involves automation and huge amount of investment in special purpose machines to increase
1.5 PROCESS PLANNING
Process planning consists of selection of means of production (machine-tools, cutting tools,
presses, jigs, fixtures, measuring tools etc.), establishing the efficient sequence of operation,
determination of changes in form, dimension or finish of the machine tools in addition to the
specification of the actions of the operator. It includes the calculation of the machining time,
as well as the required skill of the operator. It also establishes an efficient sequence of
manufacturing steps for minimizing material handling which ensures that the work will be
done at the minimum cost and at maximum productivity. The basic concepts of process
planning are generally concerned with the machining only. Although these concepts may also
be extended to other processes such as casting, forging, sheet metal forming, assembling and
heat treatment as well.
1.6 MANUFACTURING PROCESS
Manufacturing process is that part of the production process which is directly concerned
with the change of form or dimensions of the part being produced. It does not include the
transportation, handling or storage of parts, as they are not directly concerned with the
changes into the form or dimensions of the part produced.
1.7 CLASSIFICATION OF MANUFACTURING PROCESSES
For producing of products materials are needed. It is therefore important to know the
characteristics of the available engineering materials. Raw materials used manufacturing of
products, tools, machines and equipments in factories or industries are extracted from ores.
The ores are suitably converted the metal into a molten form by reducing or refining processes
4 Introduction to Basic Manufacturing Processes and Workshop Technology
in foundries. This molten metal is poured into moulds for providing commercial castings,
called ingots. Such ingots are then processed in rolling mills to obtain market form of
material supply in form of bloom, billets, slabs and rods. These forms of material supply are
further subjected to various manufacturing processes for getting usable metal products of
different shapes and sizes in various manufacturing shops. All these processes used in
manufacturing concern for changing the ingots into usable products may be classified into six
major groups as primary shaping processes, secondary machining processes, metal forming
processes, joining processes, surface finishing processes and processes effecting change in
properties. These are discussed as under.
1.7.1 Primary Shaping Processes
Primary shaping processes are manufacturing of a product from an amorphous material.
Some processes produces finish products or articles into its usual form whereas others do not,
and require further working to finish component to the desired shape and size. Castings need
re-melting of scrap and defective ingots in cupola or in some other melting furnace and then
pouring of the molten metal into sand or metallic moulds to obtain the castings. Thus the
intricate shapes can be manufactured. Typical examples of the products that are produced by
casting process are machine beds, automobile engines, carburetors, flywheels etc. The parts
produced through these processes may or may not require to under go further operations.
Some of the important primary shaping processes is:
(1) Casting, (2) Powder metallurgy, (3) Plastic technology, (4) Gas cutting, (5) Bending and
1.7.2. Secondary or Machining Processes
As large number of components require further processing after the primary processes. These
components are subjected to one or more number of machining operations in machine shops,
to obtain the desired shape and dimensional accuracy on flat and cylindrical jobs. Thus, the
jobs undergoing these operations are the roughly finished products received through primary
shaping processes. The process of removing the undesired or unwanted material from the
workpiece or job or component to produce a required shape using a cutting tool is known as
machining. This can be done by a manual process or by using a machine called machine tool
(traditional machines namely lathe, milling machine, drilling, shaper, planner, slotter). In
many cases these operations are performed on rods, bars and flat surfaces in machine shops.
These secondary processes are mainly required for achieving dimensional accuracy and a very
high degree of surface finish. The secondary processes require the use of one or more
machine tools, various single or multi-point cutting tools (cutters), job holding devices, marking
and measuring instruments, testing devices and gauges etc. for getting desired dimensional
control and required degree of surface finish on the workpieces. The example of parts produced
by machining processes includes hand tools machine tools instruments, automobile parts,
nuts, bolts and gears etc. Lot of material is wasted as scrap in the secondary or machining
process. Some of the common secondary or machining processes are—
(1) Turning, (2) Threading, (3) Knurling, (4) Milling, (5) Drilling, (6) Boring, (7) Planning,
(8) Shaping, (9) Slotting, (10) Sawing, (11) Broaching, (12) Hobbing, (13) Grinding, (14) Gear
cutting, (15) Thread cutting and (16) Unconventional machining processes namely machining
with Numerical Control (NC) machines tools or Computer Numerical Control (CNC) machines
tools using ECM, LBM, AJM, USM setups etc.
1.7.3 Metal Forming Processes
Forming processes encompasses a wide variety of techniques, which make use of suitable
force, pressure or stresses, like compression, tension and shear or their combination to cause
a permanent deformation of the raw material to impart required shape. These processes are
also known as mechanical working processes and are mainly classified into two major categories
i.e., hot working processes and cold working processes. In these processes, no material is
removed; however it is deformed and displaced using suitable stresses like compression,
tension, and shear or combined stresses to cause plastic deformation of the materials to
produce required shapes. Such processes lead to production of directly usable articles which
include kitchen utensils, rods, wires, rails, cold drink bottle caps, collapsible tubes etc. Some
of the important metal forming processes are:
Hot working Processes
(1) Forging, (2) Rolling, (3) Hot spinning, (4) Extrusion, (5) Hot drawing and (6) Hot spinning.
Cold working processes
(1) Cold forging, (2) Cold rolling, (3) Cold heading, (4) Cold drawing, (5) Wire drawing,
(6) Stretch forming, (7) Sheet metal working processes such as piercing, punching, lancing,
notching, coining, squeezing, deep drawing, bending etc.
1.7.4 Joining Processes
Many products observed in day-to-day life, are commonly made by putting many parts together
may be in subassembly. For example, the ball pen consists of a body, refill, barrel, cap, and
refill operating mechanism. All these parts are put together to form the product as a pen.
More than 800 parts are put together to make various subassemblies and final assembly of
car or aero-plane. A complete machine tool may also require to assemble more than 100 parts
in various sub assemble or final assembly. The process of putting the parts together to form
the product, which performs the desired function, is called assembly. An assemblage of parts
may require some parts to be joined together using various joining processes. But assembly
should not be confused with the joining process. Most of the products cannot be manufactured
as single unit they are manufactured as different components using one or more of the above
manufacturing processes, and these components are assembled to get the desired product.
Joining processes are widely used in fabrication and assembly work. In these process two or
more pieces of metal parts are joined together to produce desired shape and size of the
product. The joining processes are carried out by fusing, pressing, rubbing, riveting, screwing
or any other means of assembling. These processes are used for assembling metal parts and
in general fabrication work. Such requirements usually occur when several pieces are to be
joined together to fabricate a desired structure of products. These processes are used developing
steam or water-tight joints. Temporary, semi-permanent or permanent type of fastening to
make a good joint is generally created by these processes. Temporary joining of components
can be achieved by use of nuts, screws and bolts. Adhesives are also used to make temporary
joints. Some of the important and common joining processes are:
(1) Welding (plastic or fusion), (2) Brazing, (3) Soldering, (4) Riveting, (5) Screwing,
(6) Press fitting, (7) Sintering, (8) Adhesive bonding, (9) Shrink fitting, (10) Explosive welding,
(11) Diffusion welding, (12) Keys and cotters joints, (13) Coupling and (14) Nut and bolt joints.
1.7.5 Surface Finishing Processes
Surface finishing processes are utilized for imparting intended surface finish on the surface
of a job. By imparting a surface finishing process, dimension of part is not changed functionally;
6 Introduction to Basic Manufacturing Processes and Workshop Technology
either a very negligible amount of material is removed from the certain material is added to
the surface of the job. These processes should not be misunderstood as metal removing
processes in any case as they are primarily intended to provide a good surface finish or a
decorative or protective coating on to the metal surface. Surface cleaning process also called
as a surface finishing process. Some of the commonly used surface finishing processes are:
(1) Honing, (2) Lapping, (3) Super finishing, (4) Belt grinding, (5) Polishing, (6) Tumbling,
(7) Organic finishes, (8) Sanding, (9) deburring, (10) Electroplating, (11) Buffing, (12) Metal
spraying, (13) Painting, (14) Inorganic coating, (15)Anodizing, (16) Sheradising, (17) Parkerizing,
(18) Galvanizing, (19) Plastic coating, (20) Metallic coating, (21)Anodizing and (22) Sand blasting.
1.7.6 Processes Effecting Change in Properties
Processes effecting change in properties are generally employed to provide certain specific
properties to the metal work pieces for making them suitable for particular operations or use.
Some important material properties like hardening, softening and grain refinement are needed
to jobs and hence are imparted by heat treatment. Heat treatments affect the physical
properties and also make a marked change in the internal structure of the metal. Similarly
the metal forming processes effect on the physical properties of work pieces Similarly shot
peening process, imparts fatigue resistance to work pieces. A few such commonly used processes
are given as under:
(1) Annealing, (2) Normalising, (3) Hardening, (4) Case hardening, (5) Flame hardening,
(6) Tempering, (7) Shot peeing, (8) Grain refining and (9) Age hardening.
In addition, some allied manufacturing activities are also required to produce the finished
product such as measurement and assembly.
1.8. PRODUCT SIMPLIFICATION AND STANDARDISATION
The technique of simplification and standardization of product is closely inter-related that
leads to higher efficiency in production, better quality and reduced production cost. Simplification
is a process of determining limited number of grades, types and sizes of a components or
products or parts in order to achieve better quality control, minimize waste, simplify production
and, thus, reduce cost of production. By eliminating unnecessary varieties, sizes and designs,
simplification leads to manufacture identical components or products for interchangeability
and maintenance purposes of assembly of parts. Standardization is the important step towards
interchangeable manufacture, increased output and higher economy. The technique of
standardization comprises of determining optimal manufacturing processes, identifying the
best possible engineering material, and allied techniques for the manufacture of a product and
adhering to them very strictly so long as the better standards for all these are not identified.
Thus definite standards are set up for a specified product with respect to its quality, required
equipment, machinery, labor, material, process of manufacture and the cost of production.
The identified standard with time for a specified product should never be taken as final for
ever because improvement is always possible. It must accommodate the outcome of all the
new researches in the manufacturing areas in order to keep pace with increasing global
competition. Improvements over the existing standards in all respects should always be
welcomed. The different standards prevailing in different industries may be of the types of
managerial, design, manufacturing and technical needs. Managerial standards are applicable
to administrative functions within industry. These include the company policy, accounting
procedures, personnel policies, performance evaluation, control of expenditures, safety aspects,
security procedures and regulations, etc. where as design, manufacturing and technical standards
are needed for manufacturing concepts of the industry. These include design and manufacturing
techniques, practices, materials and parts, supplies, methods of testing, drafting method,
abbreviations and symbols, specifications and nomenclature, etc.
1.9 INSPECTION AND QUALITY CONTROL
A product is manufactured to perform desired functions. It must have a specified dimension
such as length, width, height, diameter and surface smoothness to perform or accomplish its
intended function. It means that each product requires a defined size, shape and other
characteristics as per the design specifications. For manufacturing the product to the specified
size, the dimensions should be measured and checked during and after the manufacturing
process. It involves measuring the size, smoothness and other features, in addition to their
checking. These activities are called measurement and inspection respectively.
In the era of globalization, every industry must pay sufficient attention towards maintaining
quality because it is another important requirement or function of a production unit. If a
manufacturing concern wants to survive for longer time and to maintain its reputation among
the users, it should under all condition apply enough efforts not only to keep up the standard
of quality of its products once established but to improve upon the same from time to time.
For this, every manufacturing concern must maintain a full-fledged inspection and quality
control department which inspects the product at different stages of its production. Vigilant
inspection of raw materials and products depends upon the entire process of standardization.
The production unit of manufacturing concern must produce identical products. However a
minor variation may be allowed to a predetermined amount in their finished dimensions of
the products. The two extremities of dimensions of the product are called limits. All the parts
of which the finished dimensions lie within these limits are acceptable parts. This facilitates
easy and quicker production, easy inspection, requires less skill on the part of worker and
accommodates a slight inaccuracy in the machine as well, resulting in an over all reduction
in the production cost of the part.
1.10 MECHANIZATION AND AUTOMATION
Mechanization means something is done or operated by machinery and not by hand.
Mechanization of the manufacturing means is milestone oriented trend towards minimizing
the human efforts to the extent of its possibility, by adopting mechanical and electrical means
or methods for automating the different manufacturing processes. Such a trend may be in the
area of automating and mechanizing the processes of material handling, loading and unloading
of components, actual operations performed on the job or transportation, etc. But, no feedback
is provided by the process, operation or machinery. Extension of mechanization of the production
process is termed as automation and it is controlled by a closed loop system in which feedback
is provided by the sensors. It controls the operations of different machines automatically. The
automatic control may be applied for some operations or for all the operations of a machine
or group of machines. Accordingly the machine will be known as semi-automatic or fully
automatic. The term was identified shortly after the World War II at the Ford Motor Company
to describe the automatic handling of materials and parts between the process operations.
The word ‘automation’ is derived from the Greek word automatos meaning self-acting.
Automation can also be defined as the process of following a predetermined sequence of
operations with little or no human intervention, using specialized equipment and devices that
8 Introduction to Basic Manufacturing Processes and Workshop Technology
perform and control the manufacturing process. Automation is a word that has many meanings
in the industry today. Automatic machines of all kinds existed long before the term automation
was conceived. But, it should be noted that all automatic machines do not come under the
category of automation. Automation is a technology concerned with the application mechanical,
electronic, and computer based systems to operate and control production.
Every machine should involve some automation, may be to a lesser degree or to a higher
extent to which is mainly governed by economic considerations. Automation means a system
in which many or all of the processes in the production, movement, and inspection of parts
and material are performed under control by the self-operating devices called controllers. This
implies that the essential elements of automation comprise of mechanization, sensing, feedback,
and control devices. The reasons why one should go for automation are:
1. Increased productivity
2. Reduced cost of labor and dependence on labor shortages
3. Improved quality
4. Reduced in-process inventory
5. Reduced manufacturing time
6. Reduced dependence on operator skills
7. Increased safety or reduced risk of humans.
Automation can be classified into three categories, viz.
1. Fixed automation
2. Programmable automation
3. Flexible automation.
1.10.1 Fixed Automation
It is also known as hard automation which is utilized to produce a standardized product such
as gears, nuts and bolts, etc. Even though the operating conditions can be changed, fixed
automation is used for very large quantity production of one or few marginally different
components. Highly specialized tools, devices, equipment, special purpose machine tools, are
utilized to produce a product or a component of a product very efficiently and at high production
rates with as low unit costs as possible relative to other alternative methods of manufacturing.
1.10.2 Programmable Automation
In programmable automation, one can change the design of the product or even change the
product by changing the program. Such technique is highly useful for the low quantity
production of large number of different components. The equipments used for the manufacturing
are designed to be flexible or programmable. The production normally carried out in batches.
1.10.3 Flexible Automation
There is a third category possible between fixed automation and programmable automation
that is called flexible automation using Computer Aided Design (CAD) and Computer Aided
Manufacturing (CAD/CAM) activities. This is also called as flexible manufacturing system
(FMS). It allows producing different products on the same equipment in any order or mix. One
important example of programmable automation, in discrete manufacturing, is numerical
control. Robot is another example of programmable automation. Robot being integral part of
FMS and Computer Integrated Manufacturing (CIM) system can do a large number of
manufacturing tasks for replacing the human labor.
In the present globalized manufacturing scenario, the advancements of hardware and
software concepts using the mechatronics for fast mechanization and automation of
manufacturing processes have become essential to be incorporated in the manufacturing
1.11 COMPUTER AIDED MANUFACTURING (CAM)
The computer aided manufacturing implies manufacturing itself, aided or controlled by
computers. In a wider sense, it denotes all the activities in the manufacturing environment
like use of computers in inventory control, project management, material requirement planning,
data acquisition, testing and quality control. Improved reliability in view of the better
manufacturing methods and controls at the manufacturing stage, the products thus
manufactured as well as of the manufacturing system would be highly reliable. Since most
of the components of a CAM system would include integrated diagnostics and monitoring
facilities, they would require less maintenance compared to the conventional manufacturing
methods. Because of the Computer Numerical Control (CNC) machines used in production
and the part programs being made by the stored geometry from the design stage, the scrap
level would be reduced to the minimum possible and almost no rework would be necessary.
Since all the information and controlling functions are attempted with the help of the computer,
a better management control on the manufacturing activity is possible. All the above advantages
when properly translated, would mean a lower total cost and consequently, higher final
earnings. Therefore any manufacturing activity in a production unit (job shop production or
mass scale manufacture) can get the benefits of Computer Aided Manufacturing. However,
better results can be obtained when the design and manufacturing activities are properly
integrated. Also, when there is a large variety of products or minor changes required in the
existing production programme, CAM can easily manage the necessary changes or alterations.
Following are the main advantages of using CAM.
1. Greater design freedom
Any changes that are required in design can be incorporated at any design stage without
worrying about any delays, since there would hardly be any in an integrated CAM environment.
2. Increased productivity
In view of the fact that the total manufacturing activity is completely organized through
the computer, it would be possible to increase the productivity of the plant.
3. Greater operating flexibility
CAM enhances the flexibility in manufacturing methods and changing of product lines.
4. Shorter lead time
Lead times in manufacturing would be greatly reduced.
The integration of CAD and CAM systems is called Computer Integrated Manufacturing
(CIM) system. The role of computer in manufacturing may be in two major groups namely
computer monitoring and control of the manufacturing process and manufacturing support
applications, which deal essentially with the preparations for act of manufacturing and post
manufacture operations. Computers are used in controlling machine tools and other material
10 Introduction to Basic Manufacturing Processes and Workshop Technology
1.12 KINDS OF PRODUCTION SYSTEMS
The choice of production type dictates the machine requirements, organizational system to
a large extent, layout planning and inventory subsystems. Three main types of production are
job, batch and flow or process production. The simplest way is to classify based on production
and processes by lot size, namely single unit production, small lot production, moderate lot
production, large lot production, and continuous production. The second classification comprises
three categories, namely small size production of a large variety of products, medium-scale
production of a limited range of products, and a large-scale production of a small variety of
products. Obviously, this method is related to the number of product types and production lot
sizes, and is an effective means of analyzing modern production management. The third
classification is related to the size of the production system expressed through the number
of employees or the amount of fixed assets involved, namely small production unit employing
less than 30 employees, medium-small having 30 to 300 employees, medium with 301 to 2,000
employees and large with 2001 to 15,000 employees, and a giant corporation employing more
than 15,000 employees
Job shop production deals the manufacture of very small lots, often of single jobs. This
may be required in special situations for the purpose of proving a design, making prototypes,
in tool making or for special purpose applications. In view of the very small lot, no special
purpose machines or tooling can be economically justified. Hence, the manufacturing has to
be carried on with the general purpose machines and tooling, which is a very lengthy and
often an error prone process.
1.13 MANUFACTURING SYSTEM
Manufacturing basically implies making of goods or articles and providing services to meet
the needs of mankind. It creates value by useful application of physical and mental-labor in
the process. It is a chain of interrelated activities of production process and other support
services activities of an manufacturing environment such as order processing, product design,
design and manufacturing of tools, die, mould, jigs, fixtures and gauges, selection of material,
planning, managing and maintaining control of the processes, production, and reliable quality
of processed product in a systematic and sequential manner with proper coordination,
cooperation and integration of the whole manufacturing system that will lead to economical
production and effective marketing of proposed product in the minimum possible time. It is,
therefore, evident that manufacturing today is not a one man activity as it was in the initial
stages, wherein all the physical and mental inputs were applied by a single craftsman. These
days it has become totally a team work which consists of several components interacting
together in a dynamic manner. This entire domain of manufacturing is known as Manufacturing
System, which takes the required inputs and delivers the products for the customer. It is,
therefore, evident that manufacturing today is not a one man activity as it was in the
preliminary stages, wherein all the physical and mental inputs were provided by a single
workman. Today it is a team work which consists of several components interacting together
in a dynamic manner to provide the required physical and mental inputs at appropriate stages
to impart desired results. This entire domain of manufacturing is known as Manufacturing
System, which takes the required inputs and delivers the products for the customer.
Manufacturing system requires a large number of activities, few independent and rests
mostly interrelated. The manufacturing activities in a manufacturing system jointly contribute
towards economic and qualitatively acceptable production of desired articles in minimum
possible time. As per the need of the customer, the products are identified and their demands
are determined roughly for market forecast by considering present and future competition.
Products that may render the desired service over its expected life satisfactorily as per
requirement of customers are identified in terms of their demand, conceived and developed
for securing orders by the sales department. Once the product design activity is over and the
design finalized from all angles, functional, aesthetic, material selection, safety, economy, etc.,
it is followed by preparation of production drawings of the product assembly and its components
including a bill of materials. This is the stage where a make or buy decision has to be taken
in order to decide as to which components are to be bought from outside and which are to
be manufactured within the concern. It is followed by process planning i.e. selection of the
best process and an its parameters, design of jigs, fixtures and dies, selection of tooling,
programming of tool path as per need, for the components to be produced in-house. An
important activity in process planning within the organization is also to involve latest research
and development findings, through which the old processes are improved and new one’s are
developed in order to ensure better quality and economic production. The interaction of
different manufacturing activities in a manufacturing system can also be further enhanced by
the use of computer and hence leading CIM. The real manufacturing or production activity
is carried out on the shop. The layout of the shop floor has a significant influence on the tools
required to be coordinated in order to an economical and high quality production of various
components. It should be such that it ensures timely movement of raw materials, dies
moulds, jigs and fixtures and finished components, adequate safety to men, material and
machinery, enables timely inspection and quality control and minimizes handling time for
material and parts, etc. During actual manufacturing a lot of different activities are called
management function. Various engineers play an important role in the organizational function
of a manufacturing concern. They are required to ensure proper movement of the material,
tools and parts as per their specialized jobs in industry.
1.14 PRODUCT DEVELOPMENT
A product development has to go through the following concepts of product engineering which
are given as under.
1. Product specifications
2. Conceptual design
3. Ergonomics and aesthetics
5. Detailed design
6. Prototype development
9. Design for manufacture
10. Design for assembly
Now let us consider the manufacturing environment of a given product. How does the
product idea originate. Market forces determine the need for a product. Expertise on the part
12 Introduction to Basic Manufacturing Processes and Workshop Technology
of the company estimates the likely demand and probable profitability and decides on the best
mode of designing and manufacturing the desired product.
Traditionally, after the design of the product, the part prints are released for production.
The production engineering section first considers the feasibility of production of the product.
Having ascertained its feasibility, process planning is done so that the product can be
manufactured at the lowest possible cost. Any redesign that is needed for improving the
producibility of the product without compromising on its functionality would have to be done
at this stage. Having decided on the process plan for manufacture, the necessary actions are
undertaken for its implementation. These are making of the tooling required, acquiring of
new equipment or tools, procurement of the raw materials, releasing of the detailed operational
instructions to the shop floor, etc. The conventional methods of manufacturing are generally
inefficient and dependent on operator skills. These methods consume more time, have high
costs, and give poor accuracy.
Product design is an activity which needs to be well organized and take into account all
influences that are likely to be responsible for the success of the product under development.
A product here means a single component which is functional in itself like a wrench or an
assembly of a large number of components all of which will contribute to the functioning of
the part such as an automobile engine. The complexity of the design process certainly increases
with the number and diversity of components present in the final part. Since there are such
a large number of influencing factors, it is impossible to specify a design procedure for each
component. Here we are interested in developing some common guidelines and steps that are
needed to proceed for a successful product design and manufacture.
From the above discussion it can inferred that products can be manufactured by more
than one processes. Therefore several alternatives for manufacturing products are available.
The selection of a suitable process is depended upon the factors including volume of production,
properties of the components, technical viability of process, economy involved and desired
quality. Based upon the volume of product the manufacturing activity can be identified in
terms of job shop production, batch production and mass production
1.15 COMPUTERS IN MANUFACTURING INDUSTRIES
Factors governing increased productivity, more accuracy, greater flexibility of shapes, and
reduced manufacturing costs are forcing the manufacturing concerns to use computers in
design, manufacturing and other allied functions of industrial activities. With an increase in
the need for quality manufacturing along with the factors such as short lead time and short
product lives and increasing consumer awareness as regards the quality of the product, it is
becoming increasingly important for the manufacturers to initiate steps to achieve all these.
The developments in microelectronics in the recent past have made higher computational
ability available at a low cost. Therefore, it becomes imperative that manufacturing takes
advantage of the availability of low cost and also using yet more powerful computers. Computers
have been in use in manufacturing industries since 1960. Initially they were in use only in
supportive functions such as inventory control purchase accounting, etc. In to day’s time,
computer applications have progressed considerably in all areas of design and manufacturing
involving CAD and CAM. This however needs to be emphasized that all the benefits of CAD
and CAM can be achieved only if these two important functions are effectively interfaced. This
interfacing is known as CAD/CAM. It involves the flow of information in both the directions.
With the result the parts and assemblies are designed keeping in view the limitations and
capabilities of the processes and materials. Consequently, newer and superior products can be
produced more quickly and at lower costs.
Today, computers are not only used in manufacturing but they play also an important
role in all manufacturing related activities such as business or financial management, factory
level production management, CIM technologies, CAD, feature and solid modelling, and
CAM, manufacturing information, manufacturing system. The important sub-activities of
industrial environment have been identified to support with the use of computer in the
manufacturing industries. These are given as under:
1. Business or Financial Management
2. Sales and Marketing
3. Purchase Order Control
2. Factory Level Production management
2. Production Management
3. Manufacturing production scheduling (MPS)
4. Material requirement planning (MRP)
5. Just in time (JIT)
6. Bill of Materials
7. Capacity Planning
8. Inventory Control.
3. CIM Technologies
1. Computer Networks
2. System Design and Analysis
3. Distributed Processing
4. Database Management Manufacturing
5. Modelling and Simulation
6. Expert Systems
7. Quality Engineering.
4. Computer Aided Design (CAD)
This area is also known Feature and Solid Modelling
1. Variational and Parametric
3. Computer Graphics
4. Graphic Standards
14 Introduction to Basic Manufacturing Processes and Workshop Technology
5. Inter-graphics exchange specification (IGES)
6. Data exchange file (DXF)
7. Manufacturing Robot Programming
8. Design Analyses Tools
10. Finite element modelling (FEM)
11. Finite element analysis (FEA)
14. Test and Analysis
15. Design Tools Mechanical
16. Hydraulic, Electronics, etc.
5. Computer Aided Manufacturing (CAM)
This involves activities related to manufacturing information and manufacturing system
which are given as under—
2. Process Planning
3. Production Planning
4. Computer numerical control (CNC) part Programming
5. Robot Programming
6. Coordinate measuring machine (CMM) Programming.
1. Production Activity
4. Material Handling
6. Production Control
10. Capacity Planning
11. Quality Control.
One of the most important components for getting various benefits associated with
computer applications in manufacturing is the common databases associated with all aspects
of manufacturing. In fact, all the modules in the CAM would actually be sharing the database
created in any module. Any module would be able to modify the data as required for that
particular application. This approach reduces the work involved in maintaining the product
database and at the same time includes the latest modifications for any aspect related to
manufacturing. In contrast to the common database approach, it is possible that sometimes
individual modules in the production aspects may be taken from different vendors. In this
case care need to be taken that information is properly transmitted between the modules and
the data updating in all the modules takes place properly and at the right time. Some of above
mentioned manufacturing activities are controlled by computers. These activities are commonly
identified using the following terms.
1. Computer Aided Design (CAD)
2. Computer Aided Engineering (CAE)
3. Computer Aided Design And Drafting (CADD)
4. Computer Aided Process Planning (CAPP)
5. Computer Aided Tool Design (CATD)
6. Computer Aided Manufacturing (CAM)
7. Computer Aided Numerical Control (NC) Part Programming
8. Computer Aided Scheduling
9. Computer Aided Material Requirement Planning, etc.
10. Flexible Manufacturing System (FMS)
11. Group Technology (GT)
12. Computer aided Testing (CAT).
1. How do you classify the manufacturing processes?
2. Distinguish between ‘primary’ and ‘secondary’ processes?
3. Discuss primary shaping processes. Give also a brief account of the primary shaping processes.
4. Explain the secondary or machining processes. Give also a brief account of these processes.
5. Describe and name the types of joining processes, surface finishing operations and the
processes employed for changing the properties of manufactured components.
6. Write a short note on assembly process.
7. Write short notes on:
(a) Simplification, (b) Standardization, (c) Inspection and quality control, (d) Interchangeability,
(e) Mechanization, (f) Automation, (g) Mechatronics.
8. What do you understand from the terms Manufacturing, Process plan, Maintenance?
9. Explain the term ‘Manufacturing System’. What all it encompasses and how an integrated
approach is made for making an economical and competitive product? Describe how the use
of computers helps in increasing manufacturing efficiency.
10. Explain the terms CAD, CAM, NC, CAD/CAM, MRP, FMS and CIM?
11. Write a short note on Group Technology?
12. Explain the influence exerted by the computers on the manufacturing scene?
13. Briefly explain the conventional process of the product cycle in the conventional manufacturing
16 Introduction to Basic Manufacturing Processes and Workshop Technology
14. What are the functions that get benefited by the use of computers in design and manufacturing
15. Briefly explain the various automation aspects used in manufacturing activities.
16. Write down the advantages which can be gained by the adoption of CAD?
17. Describe the advantages which can be gained by the adoption of CAM?
18. Write down the advantages which can be gained by the adoption of FMS?
19. Write down the advantages which can be gained by the adoption of manufacturing production
20. Write down the advantages which can be gained by the adoption of Material Requirement
21. Explain the main advantages which can be gained by the adoption of CIM?
PLANT AND SHOP LAYOUT
In a manufacturing organization, a job to be manufactured spends most of the time in moving
and waiting. For reduction of this moving and waiting time of jobs/parts, it is necessary to
have proper layout and proper scheduling procedure. Plant layout specifies the position of the
overall arrangement of the various facilities such as equipments, material, manpower, materials
handling, service facilities, and passage required to facilitate efficient operation of production system
of the plant within the area of the site selected previously. Shop layout in manufacturing plant
also forms an integral part of factory planning or plant layout. Plant layout begins with the
design the position of the factory building and goes up to the location and movement of a work
table of the machine. All the manufacturing facilities such as equipments, raw materials,
machinery, tools, fixtures, workers, etc. are given a proper place in each shop of the
manufacturing plant. Plant layout of an industrial organization plays an important role in
scientific management and is defined as :
“Plant layout is such a systematic and efficient functional arrangement of
various departments, machines, tools, equipment and other supports services of an
industrial organization that will facilitate the smooth processing of the proposed
or undertaken product in the most effective, most efficient and most economical
manner in the minimum possible time”
Plant layout of an industrial organization comprises of all the aspects connected with the
industrial enterprise, viz., grounds, buildings, machinery, equipment, departments, methods
of manufacturing, factory services, material handling, flow of production, working conditions,
hygiene, labor and shipment of goods, etc. It does not necessarily mean planning a new
enterprise only. However, it also involves minor improvements, here and there, in the existing
layout, expansion of the exiting plant, re-layout of the existing plant and layout of a new
proposed plant. In a best possible plant layout, material handling and transportation is minimized
and efficiently controlled. Bottlenecks and points of congestions are eliminated so that the
raw material and semi-finished goods move fast from one work station to another. Work
stations are designed suitably to facilitate the smooth processing of the proposed or undertaken
product in the most effective, most efficient and most economical manner in the minimum
possible time. Optimal spaces are allocated to production centers and service centers. The
primary goal of plant layout is to maximize profits by setting up the best possible arrangements
of all plant facilities to the maximum advantage of reducing the cost of production of the
18 Introduction to Basic Manufacturing Processes and Workshop Technology
2.2. OBJECTIVES OF GOOD PLANT LAYOUT
Good plant layout comprises of best possible arrangement of the buildings, men, machine and
materials for processing a under taken product. The main objectives of a good plant layout
involves minimum material movement, smooth flow of the product in the plant, full utilization
of the space of the plant, provide adequate safety and satisfaction to the plant workers, evolve
sufficient flexibility in the arrangement of the above factors so as to suit the minor future
changes, if any and facilitates an effective supervision. It helps to integrate all the above
factors in such a way that the best compromise and coordination among them is achieved.
The movements of workers and manufacturing staffs within the plant are minimized. Waiting
time of the semi-finished and finished products should be reduced to the minimum. Working
conditions as far as possible should be safer and better for the satisfaction of the workers.
There should be an increased flexibility for changes in product design and for future expansion.
There should be full utilization of whole space of the shop and plant layout. The work
methods and reduced production cycle times should be improved and the plant maintenance
must be simpler. There should be increased productivity and better product quality with
reduced capital cost. A good layout facilitates materials to move through the plant at the
desired speed with the minimum possible cost.
2.3. IMPORTANT FACTORS FOR INSTALLATION OF A PLANT
The important factors while planning for installation of plant include availability of space,
power, water, raw material, good climatic conditions, good means of communication, ancillaries,
low local taxes and similar other economic considerations, marketing facilities for the planned
product, space for process disposal and skilled and unskilled labor locally. One has to keep in
mind the possibilities of utilization and sale of the process wastes and by-products of the
planned industry. Decision of manufacturing new product, financial and other aids, facilities
for expansion presence of related industries, local by laws and securities, hospitality are also
important factors which one must keep in mind for location of an enterprise. After finalizing
the size and location of the plant, the next step is to design the inner layout of the plant to
plan out the sequence of different shops and their locations accordingly to specifications of
material and product, manufacturing processes, type of production, material handling facilities,
system and facilities for storing, inter-dependability of one shop over the other, links among
various shops, service facilities and lighting and ventilation. Next, the internal arrangement
of the above mentioned infracturctral facilities of different shops are identified. This
identification is termed as shop layout. The main factors namely size and type of equipment,
number of machines to be installed, floor area required for working on each machine, power
requirements for the machines, requirements of factory services, sequence of operations to
be followed, visibility to all the machines for proper supervision and control, type of drive
used, safe working conditions, provision of stores within the shop, i.e. for tools, instruments,
finished parts and consumable materials, etc. affects the layout of the plant. A good plant
layout should meet the following basic requirement:
1. Integration of manufacturing centre facilities in terms of man, machine and material.
2. Movements of production personnel and material handling should be minimized.
3. Smooth and continuous flow of production or manufacturing work with least possible
bottlenecks and congestion points.
4. Floor space utilization should be optimum as for as possible.
Plant and Shop Layout 19
5. Working place should be free from pollution and safe working conditions should
prevail in each shop of the plant.
6. The handling of raw material, semi finished and finished product should be should
be tackled optimally and effectively
7. Plant layout and shop layouts must be flexible to facilitate changes in production
8. There should be better working environment in term of proper light, ventilation
and other amenities such as drinking water and toilets for welfare for the
2.4. MERITS OF A GOOD PLANT LAYOUT
The main advantages of a good plant layout involve effectively and economical utilization
of entire floor space of the plant, increased rate of production, reduced men and machine
hours per unit of production, reduced material handling, minimal production delays, effective
utilization of men, machinery, material and other factory support services, reduced overall
production time, elimination of large amount of paper work, significant reduction in the
indirect expenses, considerable reduction in inventory work for material, promote effective
supervision, facilitate easy flow of men, tools and material, promote flexibility in arrangement
to suit the future changes, promotes better planning and effective control, facilitates better
and easier maintenance of plant and machinery, provides safer and healthier working conditions
thereby improving the morale of the workmen, provides the material as well as psychological
satisfaction to the workers and enhance overall efficiency of the plant. The major merits of
a good plant layout are given as under:
1. Reduced men and machine hours per unit of production,
2. Effectively and economical utilization of entire floor space of the plant,
3. Work flow is smooth and continuous
4. Work in process inventory is less
5. Production control is better
6. Manufacturing time is less
7. Relatively less floor area is required
8. Material handling is less.
2.5. TYPES OF LAYOUTS
The fulfilling the objectives of a good layout as per yearly product requirement and product
types, the layouts are classified into four major categories namely fixed or position layout,
line or product layout, process or functional layout and combination or group layout. Each
kind of layouts is explained with respective merit, demerits and application as under.
2.5.1 Fixed or Position Layout
Fixed or position layout is also known as project layout. A typical fixed layout is shown in Fig.
2.1. In this type of layout the major part of an assembly or material remains at a fixed
position. All its accessories, auxiliary material, machinery, equipment needed, tools required
and the labor are brought to the fixed site to work. Thus, the product by virtue of its bulk
20 Introduction to Basic Manufacturing Processes and Workshop Technology
or weight remains at one location. Therefore the location of the major assembly, semi
assembly component and material is not disturbed till the product is ready for dispatch. This
layout is suitable when one or a few pieces of an item are to be manufactured and material
forming or treating operation requires only tools or simple machines. This layout is highly
preferable when the cost of moving the major piece of material is high and the responsibility
of product quality by one skilled workman or group of skilled workers is expected. This type
of layout is mainly adopted for extremely large items manufactured in very small quantity
such as ships, aero planes, boilers, reactors etc. It main merit of this layout is the minimum
movement of men, material, and tooling during manufacturing process. This layout is high
flexible as the type of product and the related processes can be easily changed without any
change in the layout. The merit and demerit of this type of layout is given as under.
Fig. 2.1 Typical project layout
Its main merits are—
1. Layout is highly flexible for varieties of products having intermittent demand as the
type of product and the related processes can be easily altered without any change
in the layout.
2. There is a minimum movement of men, material, and tooling during manufacturing
3. The material is drastically reduced.
4. Highly skilled operators are required to complete the work at one point and
responsibility for quality is fixed on one person or the assembly crew.
5. Every personnel of manufacturing team is responsible for quality work for
manufacturing the product.
The major demerits of this layout are
1. The cost of equipment handling is very high.
2. Labors and equipments are difficult to utilize fully.
3. It is limited to large items only.
This type of layout is mostly adopted for extremely large items manufactured in very
small quantity such as ships, aero planes, aircraft, locomotive, ship assembly shops, shipyards,
boilers, reactors etc.
2.5.2. Process or Functional Layout
A typical process or functional layout is shown in Fig. 2.2. In this type of layout arrangements
of similar machines, production facilities and manufacturing operations are grouped together
Plant and Shop Layout 21
according to their functions. Machine tools of one kind are positioned together so that all the
similar operations are performed always at the same place e.g. all the lathes may be grouped
together for all kinds of turning and threading operations, all drilling machines in one area
for carrying out drilling work, all tapping machines in one area for carrying out tapping work,
all milling machines in one area for carrying out milling work all buffing and polishing
machines at one place for carrying out surface finishing work, and so on. This type of layout
is normally preferred for the industries involved in job order type of production and
manufacturing and/or maintenance activities of non- repetitive type. This layout needs not to
have to be changed every time of the product or component changes. Also the breakdown of
any machine does not affect the production. This type of layout is highly suitable for batch
Shaping Milling Drilling
Fig. 2.2 Typical functional layout
The major merits of this layout are :
1. There exists a wide flexibility regarding allotment of work to equipment and workers.
2. There is a better utilization of the available equipment.
3. Comparatively less numbers of machines are needed in this layout and hence thus
reducing capital investment.
4. There is an improved product quality, because the supervisors and workers attend
to one type of machines and operations.
5. Varieties of jobs coming as different job orders thus make the work more interesting
for the workers.
6. Workers in one section are not affected by the nature of the operations carried out
in another section. For example, a lathe operator is not affected by the rays of the
welding as the two sections are quite separate.
22 Introduction to Basic Manufacturing Processes and Workshop Technology
The major demerits of this layout are :
1. This layout requires more space in comparison to line or product layout for the
same amount of production.
2. Production control becomes relatively difficult in this layout.
3. Raw material has to travel more which increases material handling and the associated
4. This layout requires more efficient co-ordination and inspections.
5. Increased material handling cost due to more movement of process raw material to
6. More material in process remains in queue for further operations.
7. Requires large in-process inventory.
8. Completion of same product takes more time.
1. This layout is used for batch or moderate production.
2. It specify path for group technology.
2.5.3.Line or Product Layout
A typical line or product layout is shown in Fig. 2.3. This layout implies that various operations
on raw material are performed in a sequence and the machines are placed along the product
flow line, i.e., machines are arranged in the sequence in which the raw material will be
operated upon. In this type of layout all the machines are placed in a line according to the
sequence of operations, i.e., each following machine or section is arranged to perform the
next operation to that performed by its preceding machine or section. In this layout raw
material starts from one end of production lines and moves from one machine to next along
a sequential path. Line layout is advantages in the continuous- production system where the
number of end products is small and the parts are highly standardized and interchangeable.
It is suitable for products having steady demand. This layout may have operational sequence
namely forging, turning, drilling, milling, grinding and inspection before the product is sent
to the finished goods store for packing and shipment. This layout is used for mass production
and ensures smooth flow of materials and reduced material handling. Breakdown of any
machine in the line in this layout may result in even stoppage of production.
Shaping Milling Drilling Inspection Dispatch
Fig. 2.3 Typical line layout
Its main merits are—
1. It involves smooth and continuous work flow.
2. It may require less skilled workers
3. It helps in reducing inventory.
4. Production time is reduced in this layout.
Plant and Shop Layout 23
5. Better coordination, simple production planning and control are achieved in this
6. For the same amount of production, less space requirements for this layout.
7. Overall processing time of product is very less.
8. This layout involves automatic material handling, lesser material movements and
hence leads to minimum possible cost of manufacturing.
The major demerits of this layout as compared with process layout are—
1. It is very difficult to increase production beyond the capacities of the production
2. When single inspector has to look after many machines, inspection becomes difficult
3. This layout is very less flexible for product change.
4. The rate or pace rate of working depends upon the output rate of the slowest
machine and hence leading to excessive idle time for other machines if the production
line is not adequately balanced.
5. Machines being put up along the line, more machines of each type have to be
installed for keeping a few as stand by, because if on machine in the line fails, it
may lead to shut down of the complete production line. That is why the line or
product layout involves heavy capital investments.
It is used in assembly work.
Fig. 2.4 shows a typical combination type of layout for manufacturing different sizes of crank
shafts. It is also known as group layout. A combination of process and product layouts
combines the advantages of both types of layouts. Most of the manufacturing sections are
arranged in process layout with manufacturing lines occurring here and there scattered
wherever the conditions permit. These days, the most of manufacturing industries have
adopted this kind of layout. In this type of layout, a set of machinery or equipment is grouped
together in a section, and so on, so that each set or group of machines or equipment is used
to perform similar operation s to produce a family of components. A combination layout is
Fig. 2.4 Typical combination layout
24 Introduction to Basic Manufacturing Processes and Workshop Technology
possible where an item is being made in different types and sizes. In such cases, machinery
and manufacturing equipments are arranged in a process layout but a group of number of
similar machines is then arranged in a sequence to manufacture various types and sizes of
products. In this layout, it is noted that, no matter the product varies in size and type, the
sequence of operations remain same or similar. This layout is suitable when similar activities
are performed together thereby avoiding wasteful time in changing from one unrelated activity
to the next. It focuses on avoiding unnecessary duplication of an effort. It is preferable for
storing and retrieving information changing related to recurring problems thereby reducing
the search tin understanding information and eliminating the need to solve the problem
again. It is also useful when a number of items are produced in same sequence but none of
the items are to be produced in bulk and thus no item justifies for an individual and independent
production line. There are some merits, demerits and application of this layout which are
given as under :
The merits of this type of layout are:
1. Reduction in cost of machine set-up time and material handling of metals.
2. Elimination of excess work-in-process inventory which subsequently allows the
reduction in lot size.
3. Simplification of production planning functions, etc.
The major demerits of this layout are :
1. Change of the existing layout is time consuming and costly.
2. Inclusion of new components in the existing component requires thorough analysis.
3. Change of input component mix may likely to change complete layout structure.
4. Change of batch size may change number of machines.
Manufacturing circular metal saws, hacksaw, wooden saw, files and crank shaft.
2.6 Comparison of Line or Product Layout and Process or Functional Layout
Comparison of line or product layout and process or functional layout is given in Table 2.1.
Table 2.1 Comparison of Line or Product Layout and Process or Functional Layout
S.No. Line or Product Layout Process or Functional Layout
1. In line or product layout, similar machines
are arranged according to the sequence of
operations required for manufacturing the
2. It leads to transfer lines.
3. It is meant for mass production and
extremely less job variety
4. Work flow is smooth in this layout
5. Job movement is very less.
6. Full automation in material handling is
possible in this layout.
In process or functional layout, similar
machines are arranged in one location for
manufacturing the product.
It leads to group technology.
It is meant for moderate production and more
Work flow is not smooth in this layout
Job movement is comparatively more.
Automation in material handling is not
effective in this layout.
Plant and Shop Layout 25
7. Machine utilization is poor in this layout.
8. Capital investment required is more in this
9. Inventory requirement is less.
10. Breakdown of one machine affects greatly in
11. Production planning and control is easy.
12. Quality of product is not so good.
13. Work flexibility is very less in this layout
14. Space required for same amount of
production is less.
15. Time taken in completion of product is less.
16. Less skilled workers are required
17. Monotony in working is more because jobs
are repetitive in nature in this layout.
18. It is used in mass production or assembly
1. What do you understand by the term plant layout?
2. Name and explain different factors responsible for selection of the site for installation of a
new plant layout.
3. What are the major objectives of plant layout?
4. What are the common advantages of a good plant layout?
5. Explain the various kinds of plant layout and the situations in which each type is used.
6. Compare process layout and product layout.
7. List out the equipments required for a sheet metal shop, carpentry shop, foundry shop,
smithy and forging shop. Draw also the layouts of the above shops.
8. Prepare a layout for fitting shop and machine shop.
Machinery utilization is better in this layout.
Capital investment required is comparatively
less in this layout.
Inventory requirement is comparatively
Breakdown of one machine does not affect so
much in this layout.
Production planning and control is
Quality of product quality is better
Work flexibility is more in this layout
Space required for same amount of production
is comparatively more.
Time taken in completion of product is more.
More skilled workers are required.
Monotony in working is less because jobs are
non-repetitive in this layout.
It is used in job order production or
maintenance work of non-repetitive type.
Industrial Safety 27
by safety measures. Every industrial personnel are required to contribute the efforts towards
safety. For ensuring industrial safety, the first factory act in India was passed by the Governor
General of India on 23rd Sept., 1948. It was further amended in 1950, 1951, 1954 and 1976,
which came into force on 26th November, 1976.
3.2 SAFETY CONCEPTS
In all kinds of industries, each shop supervisor is generally assigned the responsibility of
safety in his shop regarding the men, machines and materials. Every supervisor in each shop
ensures to the top executives in respect of all kinds of the safety matters. He is supposed to
incorporate all new safety measures needed in the shop from time to time. With the growth
in the size of the industry and depending upon the hazardousness of industrial processes, a
full fledged safety department should be created under the intensive supervision through a
safety manager. The safety manager may be given a line position or staff position depending
upon the working conditions in the industry. Sometimes the responsibility for safety rests on
a safety committee formed by the top executives of the organization. A safety committee may
consist of executives, supervisors, and shop floor workers. Thus the lower level employees get
a channel of communication on safety matters direct to executive level. It is a matter of fact
that those organizations which made safety committees had lower record of accidents than
those without safety committees. Safety committees always motivate all the industrial
employees for developing safety consciousness. It acts also as a policy making body on safety
matters. To enhance the efficiency of the safety committee, some safety problem may be
assigned to safety staff for identifying and implementing safety rules and publicizing them. Its
members should be asked to go on the shop floor and watch what is being done there till date
about the safety measures. It should be asked to report periodically as what improvements
have been made and what more can be done for safety aspects in near future for avoiding
any mis-happening in the plant. Safety committee often organizes safety programs to make
industrial persons sufficiently alert for overall safety within the plant. A safety program tends
to discover when, where and why accidents occur. It always aims at reducing accidents and
the losses associated with them. It begins with the assumption that more work-connected
accidents can be prevented. It does not have an end rather it is a continuous process to
achieve adequate safety. It involves providing, safety equipments and special training to
employees. It consists of support by top management, appointing a safety officer, engineering
a safe plant, processes and operations, educating all industrial employees to work safely,
studying and analyzing the accidents to prevent their occurrence in future, holding safety
contests, safety weeks etc., and awarding incentives or special prizes to departments which
enforces the safety rules and having least number of accidents.
A safety programme should always include engineering safety at the design and equipment
installation stage, education of employees in safe practices, concerns the attitude of employees
and management. It should motivate all the industrial employees in accident prevention and
safety consciousness. It must provide all safety instructions and training essential for the
employees to think, act and work safely so that the number of accidents can be minimized.
Safety education must give knowledge about safe and unsafe mechanical conditions and
personal practices. Safety training must involve induction and orientation of new recruits to
safety rules and practices, explaining safety function, during their initial job training through
efforts made by the first level supervisors. Formulating employee’s safety committees, holding
of employee’s safety meeting, display of charts, posters, film etc. are very much essential in
each industry for stressing the need to act safely. It educates employees to develop their
28 Introduction to Basic Manufacturing Processes and Workshop Technology
safety consciousness. An industrial worker will usually accept the use of a safety measure if
he is convinced of its necessity. Therefore, suitable measures must be adopted to increase the
awareness of a need for safety in the environment of work. Such measures are required in
an industrial organization to develop safety consciousness among workers or other employees.
There should be sufficient display of safety posters and films from time to time to remind
industrial workers to particular hazards/accidents, providing simple and convenient safety
devices, providing time to the worker for setting, removing and replacing any necessary
safety devices. All industrial personnel should be asked from the first day to start working
to adopt safety measures because an unskilled worker should be familiar fully to work safely.
A safety committee should manage regular safety programmes that may hold safety
competitions. Award and prizes are also to be given to the winners for imparting due respect
and recognition to safe workers and create in employees a feeling of pride in safe work. It
should elaborate on the safety theme until all the employees are safety conscious. It must
hold regular safety meetings and stimulates the safety ideas in industrial workers for being
more safety conscious. It must ask the shop supervisor to display all the safety aspects near
the work centre. It should also mail safety information and sufficient literature pertaining to
safety for reading at homes of all the industrial employees. It must welcome all safety
suggestions. It must mark categorically all accident areas. It must conduct safety training
lectures periodically for providing wide publicity to safety aspects for everything including
men, machines and materials
3.3 PLANNING FOR INDUSTRIAL SAFETY
Mis-happening of a large number of fire hazards, accidents, industrial disasters etc., can be
reduced to the minimum possible extent through careful safety planning within an industrial
organization. All these unwanted events can be prevented by effective planning for safety.
Safety consideration includes proper layout of buildings and equipment, such as providing
adequate ventilation, sufficient working area to the operator, clear pathways for movement
of materials and parts, provision for adequate personnel facilities- viz., canteens, lunch rooms,
dispensary, fire fighting services, etc. Careful planning in advance for optimized and safe
layout of design and manufacturing activities for industry ensures industrial safety in the
manufacturing and inventory areas. Incorporating safety considerations well in time are
helpful for the establishment of a new plant as well as an existing plant needing major
alterations. Such considerations lead to adequate safety to men, machine and equipments,
reduction in operational time and increase in production. Several codes and standards for
industrial safety, health and hygiene, fire prevention, etc. have been prescribed by government
and other safety agencies and they should be fully taken care of at the planning and
implementation stages of a plant. A number of important features should be considered and
suitably incorporated planning the layout of a new plant and its buildings for safety. Hoists
and conveyors are commonly used in industries for raising, lowering and transporting loads
for limited distances. A high degree of safety is needed while these equipments are in operation.
During operations of these equipments, one should keep in mind the following important
Material handling and its storage are very common functions in a plant. Material handling
when performed manually the chances of injuries are greater. Therefore the following points
should be taken care for carrying out such tasks. All material handling equipments such as
conveyers, automotive guided vehicles, robots, cranes should carry proper guards for its gears
and other dangerous moving parts to prevent access from these parts during operation. All
Industrial Safety 29
hoisting devices must be equipped with limit switches for preventing loads block from over
traveling accidentally. Hoisting equipment especially cranes, should only be operated by properly
trained personnel for avoiding all sorts of mishaps or accidents. While operating a crane, the
operator should be entirely guided by standard signal and both operator and his signaler
should be thoroughly trained. Proper protections against fire and explosion hazards are
required when gasoline operated crains are being used. Where manual loading is done on
conveyors which run along a vertical path, either partially or totally, safe load sign should be
prominently displayed on all loading stations. Sufficient lighting, ventilation, drainage, escape
ways and guarding should be provided for conveyors which run in pits, tunnels and similar
other enclosures. Riding on a conveyor should always be prohibited. All the persons working
on or around the conveyor must wear tight cloths and safety shoes. All rotating, reciprocating
and projecting parts of machinery and equipments such as sprockets, gears, etc., should be
adequately protected by proper guarding. An effective lubrication schedule should be worked
out and implemented. All inspection should be carried out regularly and worn out parts, if
any, should be replaced immediately.
The workers should be properly trained to adopt safe working habits and proper supervision
should be done while these operations are being carried out manually. Industrial personnel
and unskilled workers should be adequately trained for adopting safe working habits in the
proper ways of lifting and setting down the objects. They should be told to be careful from
pinches and shear points and to grasp the articles firmly when lifting or setting down. Objects
which are wet or dirty or have slippery surfaces, such as greasy or oily and wet articles should
be completely wiped off dry before handling them. The hands should also be kept free of oil
and grease. For preventing hand injuries the handlers should be made to wear protective
clothing like leather hand gloves, sleeves, etc. The worker handling materials should always
wear foot in order to prevent foot injuries. If an object is to be lifted and carried to some
distance it should be ensured that the pathway is not slippery and there are no obstructions
on the passage or way. The unskilled industrial workers should be properly trained for
keeping correct positions of their feet, positions of back and knees, holding the object close
to the body while lifting and carrying, correct and firm grip, position of chin and application
of body weight in lifting and setting down by hand. This will help to prevent muscle strains
and back injuries. When a gang or team of workers is used to carry a heavy load form one
place to another the supervisor should ensure the use of proper tools and direct the work
himself to ensure proper synchronization in the lifting, walking and setting down actions of
all the workers involved. While transporting material by trucks, the truck should be operated
at safe limit speed as specified and special care should be taken at blind corners and doorways.
During storing material, it should be ensured that the electrical panels and installations and
fire extinguishers and hoses are kept clear and have free accessibility. Also the pathways,
entries and exits should always be kept clear for movement. The use of racks and bins
enables more storage capacity, easy movement of material from one place to another and
ensures better safety in an industrial organization
3.3.1 Objectives of Industrial Safety
The objectives of industrial safety are as follows:
1. Industrial safety is needed to check all the possible chances of accidents for preventing
loss of life and permanent disability of any industrial employee, any damage to
machine and material as it leads to the loss to the whole establishment.
2. It is needed to eliminate accidents causing work stoppage and production loss.
30 Introduction to Basic Manufacturing Processes and Workshop Technology
3. It is needed to prevent accidents in industry by reducing any hazard to minimum.
4. It is needed to reduce workman’s compensation, insurance rate and all the cost of
5. It is required to educate all members regarding the safety principles to avoid accidents
6. It is needed to achieve better morale of the industrial employees.
7. It is required to have better human relations within the industry.
8. It is needed to increase production means to a higher standard of living.
3.4 ACCIDENTS AND THEIR TYPES
The accidents are the mishaps leading injury to man, machines or tools and equipment and
may cause injury and result either death or temporary disablement or permanent disablement
of the industrial employees. A survey was conducted in 1952 in America which specified that
approximately ten thousands industrial persons were killed in accidents and more than lakhs
were injured in a year. The accidents are unwanted events or mishaps that result in some
sort of injury to men, material, machines, tools, equipment and semi or finished product
hence, a loss to the whole establishment. The total cost of these accidents was more than
crores of dollars. An industrial accident may be defined as an event, detrimental to the health
of man, suddenly occurring and originating from external sources, and which is associated
with the performance of a paid job, accompanied by an injury, followed by disability or even
death. An accident may happen to any employee under certain circumstances. The said injury
or loss may be minor or major in nature and accordingly the accident is termed as non-
reportable or reportable kind. It should, however, be understood that no hard and line of
demarcation can be laid between these two aspects and their identification varies with the
place of application. For example a small burn or cut oft body will be reportable accident in
a workshop whereas the same, can be treated by first aid and does not involve any appreciable
loss of time, not be considered a reportable accident. Few industries determine the accidents
by the extent to which it leads to the disablement of the victim and number of hours or days
he is to remain absent from duty on account of the problem. There are others which take
into consideration various factors like machine, tools, materials, cost of medicines, loss of
production and compensation to be given to the worker who meets with the accident. An
accident can be very costly to the injured employee as well as to the employer of the
manufacturing concern. Some direct or indirect costs are associated with accidents in
industries. The direct costs involve payment of compensation and overheads uncompensated
wage losses of the injured employees, cost of medical care and hospitalization. Whereas
indirect costs of an accident comprise of costs of damage of machines, materials and plant
equipments, costs of wages paid for time lost by workers not injured, costs of wages paid to
the victim, costs of investigating agency involving recording and reporting of accidents and
its causes, costs of deputing new employee for replacement of the injured employee, cost of
decreased production by the substituting victim, cost of delays in production due to accident,
cost of reduced efficiency of the victim when he joins the manufacturing concern after getting
recovered and cost of lowered production due to reduced morale of employees. An accident
is an unexpected event which is likely to cause, an injury. Proper diagnosis of causes of mis-
happening and corrective measures of the same always helps in preventing future accidents.
Accidents in industries put a heavy burden on society also. All direct and indirect cost to the
management will ultimately have to be met by the consumers in terms of increased cost of
Industrial Safety 31
product. Also, the financial burden of disabled persons and their dependents have to be born
by society. Thus every citizen in a nation has to bear a proportion of the cost of accidents.
Every care and prevention therefore should be evolved adopted to prevent accidents to the
maximum possible extents. Accidents do not just happen but they are caused because of
failure to follow the needed safety precautions and safety rules. If someone is honest with
himself, he cannot think of a single accident that could not have been prevented by care.
There are various types of common accidents needing due attention to prevent them which
are as follows:
1. Near Accident
An accident with no damage or injury is called near accident.
An accident with very less damage is called trivial.
3. Minor Accident
It is an accident with damage and injury more than trivial.
4. Serious Accident
An accident with heavy damage and lot of injury is called serious accident.
It is an accident with very heavy damage. There may be loss of lives also.
3.4.1 Effect of Accidents
The adverse effects of the accident are given as under—
(A) Effect on the owner of factory
(i) Direct cost of an accident
1. Cost of the compensation paid to the workers.
2. Cost of the money paid for treatment.
3. Cost of the monetary value of damaged tools, equipments and materials.
(ii) Indirect cost of an accident
1. Cost of the lost time of injured worker.
2. Cost of the time lost by other employees.
3. Cost of the delays in production.
4. Cost of the time lost by supervisors, safety engineers etc.
5. Cost of the lowered production due to substitute worker.
(B) Effect on worker
1. The industrial workers may get temporary or permanent disability.
2. If the industrial worker dies, his family loses the earner and the compensation
never equals to his earnings.
3. Accident also affects the morale of the employees working in the manufacturing
(C) Effect on society
Work connected with injuries put a considerable burden on society also as given as
32 Introduction to Basic Manufacturing Processes and Workshop Technology
1. Cost of accidents is included in the products, so the society has to pay more prices
for the industrial products.
2. If some industrial workers do not come under compensation act, the need for help
from society is much greater.
3. Loss of production hours may causes fewer products in market. So more prices if
demand is more than production.
3.5 CAUSES OF ACCIDEENTS
The accidents may take place due to human causes, environmental causes and mechanical
causes. These causes are discussed as under.
1. Accidents may occur while working on unsafe or dangerous equipments or machineries
possessing rotating, reciprocating and moving parts.
2. Accidents occur while operating machines without knowledge, without safety
precautions, without authority, without safety devices.
3. Accidents generally occur while operating or working at unsafe speed.
4. Accidents may occur while working for long duration of work, shift duty etc.
5. Accidents commonly occur during use of improper tools.
6. Accidents may occur while working with mental worries, ignorance, carelessness,
nervousness, dreaming etc.
7. Accidents occur because of not using personal protective devices.
1. Accidents may occur during working at improper temperature and humidity causes
fatigue to the workers so chances of accidents increases with workers having fatigue.
2. The presence of dust fumes and smoke in the working area may causes accidents.
3. Poor housekeeping, congestion, blocked exits, bad plant layout etc. may cause
4. Accidents occur due to inadequate illumination.
5. Improper ventilation in the plant may also leads to industrial accidents.
1. Continued use of old, poor maintained or unsafe equipment may result in accidents.
2. Accidents commonly occur due to use of unguarded or improper guarded machines
3. Unsafe processes, unsafe design and unsafe construction of building structure may
lead to accidents in the plant.
4. Accidents occur due to improper material handling system and improper plant
5. Accidents may occur due to not using of safety devices such as helmets, goggles,
gloves, masks etc.
Industrial Safety 33
However the other general causes of accidents in workshops are listed under:
1. Because of ignorance to work with equipments, hand tools, cutting tools and machine
2. Operating machine and equipments without knowledge.
3. Extra curiosity to work without knowing.
4. Due to poor working conditions.
5. Because of speedy work.
6. Improper method to work.
7. Due to use of improper tools.
8. Because of lack of discipline.
9. Uninterested in work.
10. Due to carelessness.
11. Due to over confidence.
12. Bad working environment.
13. Because of excessive over times duty by industrial workers.
14. Dangerous materials with which to work.
15. Lack of cleanliness.
16. Due to poor planning.
In a conducted survey, it was observed that most of the accidents, to the tune of 98%,
could be easily avoided provided due precautions and care were adopted well in time. It was
stressed that accidents do happen but are caused due to the failure of one element or the
other. The most unfortunate and most common factor in occurring accidents is the human
element which occurs due to non-observance of the safety measures or safety rules. The past
statistics also reflects that the causes of accidents as well as the nature of accidents depend
entirely on the extent to which safety measures are adopted and not the manufacturing
processes or operation. The common causes which lead to accidents may be improper acts by
industrial personnel which result in violation of safety rules and non -observance of safety
precautions, due to improper tools, machinery and equipments or their unsafe or improper
use due to unsafe working position and unsafe working conditions in manufacturing areas.
Some major factors namely technical, unsafe working conditions, mechanical, environment,
human cause, unsafe acts and other personal factors are most responsible for accidents.
Technical causes or unsafe conditions involves deficiencies in plant, equipment, tools, machinery,
materials handling system, general work environment etc. Mechanical causes involve unsafe
design and construction of tools and devices, cutting tools, machines tools and mechanical
equipments, hazardous arrangement such as piling, over-loading etc, improper guards a against
dangerous machine components, defective tool and equipments, improper material handling,
leaking valves of acid and poisonous gases, and use of untested boilers and pressure vessels.
Environmental factors indicate improper physical and atmospheric surrounding conditions of
work which indirectly promote the occurrence of accidents These factors include too low
temperature to cause shivering, too high temperature to cause headache and sweating, too
high a humidity (in textile industry) to cause discomfort, fatigue and drowsiness, inadequate
illumination causing eyestrain, glares, and shadows, presence of dust, fumes and smokes in
34 Introduction to Basic Manufacturing Processes and Workshop Technology
industries such as foundries, chemical , paper and sugarcane etc. Lack of adequate ventilation,
high speed of work because of huge work load, more number of working hours and over and
above them the tendency of the employer to insist for over time work, inadequate rest periods
in between works, noise, bad odor and flash coming from the nearby machinery, equipment
or processes, and poor housekeeping are also personal factors.
A large number of accidents can be avoided if proper safety measures and safety rules
are adopted in manufacturing areas. Some of the important causes of accidents involve
violation of safety rules, not using of safety devices, improper use of gadgets and machine
controls, non-development of safety working habits, ignorance of the operation of tools, machine
and equipments operation, unsafe working conditions, monotony and work-relating stresses,
wear and tear of the functional components, explosive and inflammable material etc.
3.6 COMMON SOURCES OF ACCIDENTS
A large number of revolving, rotating, reciprocating and moving parts of machinery can be
said as the sources of danger and require guarding for protection against accidents. Extensive
studies reveal that some characteristic groups of dangerous parts are acting as common
sources of accidents in workshops. Many such major sources are as under.
1. Revolving parts, viz. pulley, flywheels, worms, worm wheel, fan, gears, gear trains,
gear wheels etc.
2. Projecting fasteners of revolving parts; like bolts, screws, nuts, key heads, cotters
and pins etc.
3. Intermittent feed mechanisms, viz., tool feed of planer; table feed of a shaper, ram
feed of power presses and similar other applications.
4. Revolving shafts, spindles, bars, mandrels, chucks, followers and tools like drills,
taps, reamers, milling cutters, and boring tool etc.
5. Rotating worms and spirals enclosed in casings, such as in conveyors and revolving
cutting tool, like milling cutters, circular saw blade, saw band, circular shears and
grinding wheels, etc.
6. Reciprocating tools and dies of power presses, spring hammer, drop hammers, and
reciprocating presses, reciprocating knives and saw blade such bow saw, shearing
and perforating machines and the cutting and trimming machine and power hack-
7. Moving parts of various machines, like those of printing machines, paper-cutters
and trimmers, etc.
8. Revolving drums and cylinders without casing, such as concrete and other mixers,
tumblers and tumbling barrels, etc.
9. High speed rotating cages such as in hydro-extractors.
10. Revolving weights, such as in hydraulic accumulator or in slotting machines for
11. Nips between meshing racks and pinions of machine parts
12. Nips between reciprocating parts and fixed components, such as between shaper
table and the fixture mounted on it or a planer table and table reversing stops, etc.
13. Nips between crank handles for machine controls and fixed parts.
Industrial Safety 35
14. Projecting nips between various links and mechanisms, like cranks, connecting
rods, piston rods, rotating wheels and discs, etc.
15. Projecting sharp edge or nips of belt and chain drives; via belt, pulleys, chains
sprockets and belt fasteners, spiked cylinders etc.
16. Nips between revolving control handles and fixed parts traverse gear handles of
lathes, millers, etc.
17. Moving balance weights and dead weight, hydraulic accumulators, counter-balance
weight on large slotting machines, etc.
18. Revolving drums and cylinders uncased, tumblers in the foundry, mixers, varnish
19. Nips between fixed and moving parts such as buckets or hoppers of conveyors
against tipping bars, stops or parts of the framework.
20. Nips between revolving wheels or cylinders and pans or tables, sand mixers, crushing
and incorporating mills, mortar mills, leather carrying machines, etc.
21. Cutting edges of endless band cutting machines, wood working, and log cutting
metal find stone-cutting band saws, cloth-cutting band knives, etc.
22. Nips between gears and racks strips, roller drives, presses, planning machine drives,
3.7 PREVENTIVE MEASURES
Few safety measures commonly used in industries comprise of the proper safety guards for
reciprocating machine components such as drop hammers, presses, shaper, slotter, power
hacksaw, paper cutters etc., fencing of dangerous and rotating parts like revolving shafts,
incorporating safety devices such as safety valves, rigid construction of heavy items like
hoists, cranes etc, proper insulation of electric wire and earthing of electric appliances,
wearing appropriate safety shoe and other necessary items for, body protection, maintenance
cleanliness of shop floor, removal of metal chips with proper protection, avoiding fire hazard.
Safety while working safely in any shop is the safety of human being and the safety of
workshop machinery. Hence there is a great need for the study of the domain of industrial
safety for accidents prevention and good house keeping is the utmost. Safe working conditions
in any industry may help to minimize the number of accidents taking place, prevent premature
death of talented employee, prevent needless pain and suffering to industrial employees,
reduce damages to equipment and machinery, increase production and reduce production cost.
Good housekeeping implies keeping industry clean, look pleasant well illuminated and ventilated
so that accidents are minimized, total production and quality are improved and the employee
morale is boosted. Careless handling of heavy materials and components is a major source
of back and foot injuries. To avoid premature fatigue of transport workers, full use should be
made of mechanized materials handling equipment. Use mechanical means of conveyance to
ensure the safety of men engaged in material handling. The transport workers should not be
asked to lift more than the permissible load. Personal protective devices such as safe hard
hats, rubberized hats for protection against liquids /chemicals, ear protectors, face mask/face
shields, welding helmet, goggles of case-hardened and clear glass for protection against impact
should be used as per the need.
36 Introduction to Basic Manufacturing Processes and Workshop Technology
The good housekeeping has been borrowed from the maintenance of domestic properties
in the home or house and is now liberally applied to the maintenance of both cleanliness and
order in all kinds of business establishments, e.g., industries etc. Cleanliness is a condition
wherein buildings, work and rest areas, machinery, equipments and tools are kept free from
dirt, dust etc. Necessity of good housekeeping is essential in order to make and maintain a
clean and neat factory work in its surroundings. It makes work more pleasant, most satisfying
and motivate for all kind of employees to work. The advantages of good house keeping are
fewer accidents, increased life of building, machinery, tools, etc., improved employee morale,
increased production, better product quality, continuous cleaning reduces housekeeping costs,
no time is lost in searching for tools etc, material handling and transportation pick up speed,
inspection, maintenance and production control functions become easier, much floor space
otherwise occupied by unused raw material and tools. A good house keeping procedure involves
plan and project the housekeeping program carefully and completely.
3.8 COMMON SAFTY METHODS
The common methods of safety are as follows:
1. Safety by construction or design.
2. Safety by position.
3. Safety by using fixed guards.
4. Safety by using interlock guards.
5. Safety by using automatic guards.
6. Safety by using trip guards.
7. Safety by using distance guards.
8. Safety by workplace layout and proper working conditions.
9. Safety by proper material handling.
10. Safety by using personal protective devices.
Few of the above methods of safety are discussed as under.
3.8.1 Safety by Construction
Whenever the new tools, devices, equipments and machine are designed, they should be
ensured that all their dangerous parts are either enclosed in suitable housings or provided
with suitably designed safety guards in order to eliminate any chances of danger that could
occur due to exposure of the dangerous parts. A common example involve belt drive and
motor in a in drilling machine, lathe, milling or in other machines are enclosed, the back
gears and tumbler gears in a lathe are either enclosed or provided with cast iron guards or
covers. All control levers and handles of machines should be carefully located to ensure
adequate safety in their operation. Generally, lubricating points are provided on the outer
surface that the interior parts are not required to be opened every now and then.
3.8.2 Safety by Position
The main principle involved in the method for safety by position is to design the machine in
such a way that the dangerous parts are so located or placed that they are always beyond
reach of the operator. It is therefore always advisable that all the dangerous parts of the
machine should invariably be guarded or enclosed in the body or housing of the machines as
Industrial Safety 37
far the design conditions permit. If it is not possible suitable external fencings must be
3.8.3 Safety by Using Fixed Guards
Such fixed guards either form an integral part of the machine or are so tightly secured to
them that they are not easily removable. In all cases, fixed guards are developed to have a
robust and rigid construction and they should be so placed that any access to the dangerous
parts of the machine is totally prevented from all directions particularly in the running
condition of the machines. Fixed guards adjusted in position remain fixed and they are
neither moved nor detached. In some cases the fixed guards are provided at a distance from
the danger point. Such a provision will carry a remote feeding arrangement and, therefore,
the operator will not be required to go near the dangerous points.
3.8.4 Safety by Using Interlock Guards
An interlocking guard may be mechanical, electrical, pneumatic or some sort of a combination
of these. Such guards cannot be removed and the dangerous parts are not exposed until and
unless the machine is totally stopped. Similarly, the machine cannot be started to work unless
the guards return in position and protects the dangerous parts. It is essential that such
guards should always acquire their positions to guard the dangerous parts before the machine
can be started,. Such arrangements prevent the starting and operation of the machine in case
the interlocking device fails and remain closed in position until the dangerous part is completely
at rest. Scotch interlocking and control interlocking designs of these guards are common used
to protect accidents. The former interlocking consists of a solid metal piece, called scotch
connected to it which is so located that it remains between two moving parts of the machine.
This prevents the machine from starting so long as the same is not removed and the guard
brought in proper position for protection. The latter comprises of the movable portion of the
guard as connected to some starting device or mechanism of the machine viz., fast and loose
pulleys, clutch, starter of the motor or tile hydraulic valve, etc. This connection is made in
such a way that it will not allow the operation of the said device or mechanism until and
unless the guard is brought in protecting position, which automatically enables its removal
from that position from where it prevents the operation of the starting mechanism.
3.8.5 Safety by Using Automatic Guards
The main principle of an automatic guard is that its operation is actuated by some moving
part of the machine. Automatic guard and machine operation is so linked that the part will
automatically bring the guard in protecting position before the operation of the machine
starts. The design of this guard is of such a kind that it automatically forces the operator to
move away from the dangerous area of work before the operation starts. Such arrangement
of such guard does not permit the operator access to this area again until and unless the
machine stops. The use of such guard is largely favored for heavy and slow acting machines
like heavy power presses.
3.8.6 Safety by Using Distance Guards
Distance guard helps to fence the dangerous components of machine such as bars or rails and
position them at a suitable distance from the machine such that even operator by chance,
extends his hands over it, his fingers, clothes or any of the body does not reach within the
area of dangerous parts. For additional safety, some sort of tripping device should always be
incorporated to stop the machine rapidly in case of an accident.
38 Introduction to Basic Manufacturing Processes and Workshop Technology
3.8.7 Safety by Using Trip Guards
Trip guard in machine is comprised with tripping device which enables quick stopping or
reversal of the motion of machine as soon as the operator approaches within the reach of
dangerous parts. Tripping device and the trip guard works in close conjunction with each
other during problematic situations.
3.8.8 Safety by Workplace Layout and Proper Working Conditions
Some safety using workplace layout and proper working conditions are given as under:
1. A suitable layout and proper working conditions play an important role in preventing
accidents which would have otherwise occurred.
2. Moving path or passage ways should be clearly marked and never be obstructed.
3. Every employee should have enough space to move and operate the machine.
4. The floor condition must be of non-skid kind. It should act as a satisfactory plane
which can be easily cleaned.
5. Height of working rooms should be adequate for proper ventilation and lighting.
6. Fire walls should be used to separate various compartments.
7. Windows should have adequate size and should be in adequate numbers.
8. Illumination should be sufficient, continuous, uniform and free from glare.
9. Proper ventilation should be there in workplace.
10. Noise level should be proper if any. If it is high, use silencers to minimize the noise
3.9 TYPES OF SAFETY
The fo1lowing general types of safety are considered in the workshop
1. Safety of self.
2. Safety of job.
3. Safety of machines tools.
However there are general safety precautions to be adopted while working in any workshop
3.9.1 General Safety Precautions while Working in a Workshop
1. One should not leave the machine ON even after the power is OFF and until it has
stopped running completely. Someone else may not notice that the machine is still
in motion and be injured.
2. Operator should not talk to other industrial persons when he is operating a machine.
3. One should not oil, clean, adjust or repair any machine while it is running. Stop the
machine and lock the power switch in the OFF position.
4. One should not operate any machine unless authorized to do so by the authorize
person in the shop.
5. Always check that work and cutting tools on any machine are clamped securely
6. The floor should be kept clean and clear of metal chips or curls and waste pieces.
Industrial Safety 39
Put them in the container provided for such things. Scraps and chips or curls may
cut through a shoe and injure the foot.
7. Defective guards must be replaced or repaired immediately.
8. One should not operate any machinery when the supervisor or instructor is not in
9. All set screws should be of flush or recessed type. Projecting set screws are very
dangerous because they catch on sleeves or clothing.
10. One should not try to stop the machine with hands or body.
11. Only trained operator should operate machine or switches as far as possible.
12. Always take help for handling long or heavy pieces of material.
13. Always follow safe lifting practices
14. No one should run in the shop at work time.
15. Always keep your body and clothes away from moving machine parts. Get first aid
immediately for any injury.
16. Never talk to anyone while operating the machine, nor allow anyone to come near
you or the machine.
17. Stop the machine before making measurements or adjustments.
18. Operator should concentrate on the work and must not talk unnecessarily while
operating the machines.
19. Never wear necktie, loose sweater, wristwatch, bangles, rings, and loose fitting
clothing while working in workshop.
20. Always wear overcoat or apron.
21. Stop machines before attempting to clean it.
22. Make sure that all guards are in their place before starting to operate a machine.
23. Do not attempt to operate a machine until you have received operating instructions.
24. Be thoroughly familiar with the ‘stop’ button and any emergency stop buttons
provided on the machines.
25. Remove burrs, chips and other unwanted materials as soon as possible. They can
cause serious cuts.
26. Do not leave loose rags on machines.
27. Wash your hands thoroughly after working to remove oils, abrasive particles, cutting
28. Report all injuries to the foreman, howsoever small. Cuts and burns should be
29. Keep the work area clean.
30. Keep your mind on the job, be alert, and be ready for any emergency.
31. Always work in proper lighting.
32. On should not lean against the machines.
40 Introduction to Basic Manufacturing Processes and Workshop Technology
3.9.2 Safety Precautions while Working with Different Hand Tools
(A) Screw Drivers
1. When working on electrical equipment use only a screw driver with an approved
2. One should wear goggles when re-sharpening screw-driver tips.
3. Screws with burred heads are dangerous and must be replaced or the burrs removed
with file or an abrasive cloth.
4. One should use the correct tip of screw drivers while screwing. Too arrow or too
wide tip will damage the work.
1. One should not hammer a wrench to loosen a stubborn fastener, unless the tool has
been specially designed for such treatment.
2. Always pull on a wrench. One can have more control over the tool if pulling instead
of pushing and there is less chance of injury.
3. It is dangerous practice to lengthen the wrench handle for, additional leverage. Use
a larger wrench.
4. Choose a wrench that fit properly. A loose fitting wrench may slip and round off the
corners of the bolt head and nut.
5. When using wrenches clean grease or oil from the floor in the work area. This will
reduce the possibility of slipping and losing balance.
1. One should not operate the hammer unless its head is tightly fixed to the handle.
2. Place the hammer on the bench carefully. A falling hammer can cause serious foot
3. Never strike two hammers together. The faces are very hard and the blow might
cause a chip to break off.
4. Never hold the hammer too far on the handle when striking a blow.
5. Unless the blow is struck squarely, the hammer may glance of the work.
3.9.3 Safety Precautions while Working with Different Cutting Tools
1. One should always use a file card to clean the file. Never use your hand. The chips
may penetrate in hand and cause a painful infection.
2. One should not use a file without a handle.
3. Short burns formed in filling may cause serious cuts. Always use a piece of cloth
to wipe the surface being field.
4. Files are highly brittle and should never be used as a hammer otherwise the file
5. Never hammer on a file. It may shatter and chips fly in all directions.
1. One should always hold the chisel in such a manner that the hammer blow may not
miss the chisel to injure your hand.
Industrial Safety 41
2. Edges of metal cut with the chisel are often sharp and cause bad cuts.
3. Flying chips are dangerous. Wear transparent plastic safety goggles and use a
shield, when using a chisel, to protect yourself and those working near you.
4. Sharp edges of chisels are removed by grinding or filing.
5. Mushroomed head of the chisel should be removed by grinding.
1. One should not test the sharpness of the blade by a running a finger across the
2. One should not brush away the chips with your hand.
3. All hard blades can shatter and produce flying chips. Wear your toggles.
4. One should not be sure that the blade is properly tensioned.
5. Store the saw so that you will not accidentally reach into the teeth when you pick
6. If the blade breaks while you are on cutting stroke, your hand may strike the works
and cause an injury. Therefore saw operator should work carefully.
1. One should remove all bars from the reamed holes.
2. Never use your hands to remove chips and cutting fluids from the reamer and work.
One should use a piece of cotton waste.
(E) Taps and Dies
1. One should use a brush to clean away chips formed by hand threading. Never use
2. One should always wear goggles if the tap, die or threaded piece is to be cleaned
with compressed air.
3. Tap operator should also be careful that other person working in the area also
4. Handle broken taps as you would handle broken glass. They are sharp edges and
are dangerous to handle.
5. Wash you hands after using cutting fluid. Skin-rashes caused by some cutting fluids
can develop into a serious skin disorder if they are left on the skin for a long period.
6. Take care of any cuts immediately. Infection may occur when injuries are not
1. If the lathe is used for polishing make sure that the machine is protected from the
abrasive grains that fall from the polishing wheels during polishing. They can cause
rapid wear of the precision parts.
2. One should not rub fingers or hand across a piece that has just been polished by
3. Cuts and burns should always be treated immediately by using first aid facility.
4. One should remove all abrasive particles by washing them thoroughly after the
42 Introduction to Basic Manufacturing Processes and Workshop Technology
3.9.4 General Safety Precautions while Working in Machine Shop
The following safety precautions or guidelines are generally adopted for every metal cutting
or machining shop. They must be strictly followed for safety. Specific safety guidelines for
some of the machine process like lathe, drilling, shaping, planning slotting, grinding, milling,
and finishing operations are also described in the following sections.
1. One should use the correct tools and work holding devices recommended for the process.
2. One should hold the work piece and tool securely on the machine.
3. One should clamp the tool correctly. An overhanging tool may cause catastrophic
failure of the tool, work piece or the machine tool.
4. One should not try to remove chips from the machine with your hands.
5. Never use compressed air from mouth. Use brush.
6. One should not touch a job-piece with bare hands while doing inspection or removing
it from the machine. Use gloves always.
7. One should operate the machine at recommended operating conditions based on
work material and tool material combination and other cutting conditions specified.
8. One should use recommended coolant depending upon work-tool material combination.
9. During machining ductile materials, use chip breakers and chip guards.
10. One should re-sharp the tools immediately when it starts producing rough surfaces
on the job-piece or produces chatter.
11. One should not run the machines at speed higher than recommended. It may
produce vibrations and chatter and damage job-piece, tool, or both.
12. Provide sufficient approach and over travel distances wherever necessary.
13. In case of power failures, switch off the machine and retrieve tool from the workpiece.
14. One should wear goggles to protect eyes from flying chips.
15. Machines are governed by the old clinch garbage input, garbage output. The skill
of the operator is often the limiting factor for the machining operation.
16. Stop machine before attempting to clean, removing tool or workpiece.
3.9.5 General Safety Guidelines while Working on Grinding Machines
1. Grinding wheels badly worn or cracked should be replaced
2. The grinding wheel should be properly balanced while mounting.
3. One should ensure that no combustible or flammable materials are nearby that
could be ignited by sparks generated by grinding wheels during grinding operations.
4. One should allow the grinding wheel to reach full speed before stepping it into the
grinding position. Faulty wheels usually break at the start of an operation.
5. Always use the face of the grinding wheel that is meant for grinding.
6. One should slowly move job-pieces across the face of wheel in a uniform manner.
This will keep the wheel sound.
7. Grinding wheels should be checked properly timely for soundness. Suspend the
wheel on a string and tap it. If the wheel rings, it is probably sound.
8. One should not use a grinding wheel that has been dropped or dealt with a heavy
blow, even if there is no apparent damage.
Industrial Safety 43
9. Before using a new grinding wheel, let it run for a few seconds at the full speed to
check and make sure that it is perfectly balanced.
10. One should not operate the grinding wheel beyond its bursting speed.
11. Follow the manufacturer’s instructions for the correct use of the grinding wheels.
12. Always wear goggles during grinding or allied processes.
3.9.6 Safety Precautions while Working on Lathe Machine
1. One should always be sure that all guards are in place before running the machine.
2. Always clamp the work and tool properly with correct size of work and tool holding
3. Always keep the machine clear of tools.
4. Machine should be stopped before making measurements or adjustments.
5. Wear an apron or a properly fitted shop coat. Goggles should also be used.
6. One should remove necktie, wrist watch and jewellery while working.
7. One should not operate the lathe until he knows the proper procedure.
8. One should check the work frequently when it is being machined.
9. One should check the face-plate or chuck by hand to be sure that there is no danger
of the work striking any part of the lathe.
10. Stop the machine and remove chips with pliers. One should not remove the chips
3.9.7 Safety Precautions while Working in Casting shop
Similar to other manufacturing processes, the following safety precautions need to be taken
in the casting shop also.
1. One should use mask to avoid excessive inhalation of the dust, which may cause
serious problem to health.
2. Always wear protective clothes to keep safe from the heat radiating from the
3. All foundry men should wear protective clothes, glasses, shoes, and gloves while
handling molten metal for casting process.
4. One should be alert as severe burn injury can result from spillage of the molten
5. Always use proper ventilation to protect from molten metal fumes and gases that
evolve from the mould during pouring.
6. One should not touch hot moulds and castings.
7. Always use earplugs to safeguard against the heavy noise.
8. One should always keep clean the work area.
3.9.8 Safety Precautions while Working in Welding shop
(A) Gas welding
1. One should not use a leaking gas cylinder.
44 Introduction to Basic Manufacturing Processes and Workshop Technology
2. One should not handle oxygen cylinders, valves, regulators, hoses or fittings with
3. Welder should not mix the gases in one cylinder.
4. No one should transfer the gas from one cylinder to another.
5. One should clearly mention on the cylinders the type of gas in it (i.e. oxygen,
6. One should use nose masks where the local exhaust ventilation is not practicable.
Insist the safety officer to provide proper ventilation system.
7. Always avoid skin contact with fluxes, which contain fluorides. If they will penetrate
the skin, they produce severe irritation.
8. No one should weld the parts, which are coated with toxic material such as lead,
cadmium, zinc, mercury, or paint containing toxic before materials. Any such coatings
must be removed prior to welding.
9. Acetylene gas should not be brought in contact with the unalloyed copper directly
(except in torch) which may result in a violent explosion.
(B) Arc welding
1. One should use protective clothing and eye protection devices while performing arc
welding operation, otherwise radiation from electric arc will damage the retina of
eyes. One has to be sure that other people standing nearby also uses eye-protection
devices from ultraviolet rays.
2. Always use ear protection devices such as muffler because excessive noise caused
during the process of arc welding may cause temporary or permanent hearing loss.
3. Welder should keep clothing and gloves dry.
4. Always keep welding cables free of grease and oil.
5. One should prevent the non-insulated portion of the electrode holder from touching
the welding ground or job-piece when the current is on.
6. Always keep the body insulated from both the work and the metal electrode holder.
7. One should carry out the welding process by standing on the insulating material
like dry wood rather than on a grounded metal structure.
8. It is easier and safer to establish an arc on a clean surface than on a dirty or rusty
9. Always turn the welding machine off when it is not in use.
10. One should not change the polarity switch when the machine is under use. This will
burn the surface of the switch and the resulting arc can cause injury to the welder.
11. Always avoid using electrode holders with defective jaws or poor insulation.
3.10 FACTORY ACT REGULATIONS WITH REGARD TO SAFETY
The objective of avoiding loss of lives and other industrial losses through accidents lead to
follow the factory act regulation. For example Workman Compensation Act-1923 provides
employer’s liability for compensation. Compensation depend upon the condition that injury
must have resulted either in death or partial disablement of an employee for a period
Industrial Safety 45
acceding three days during employment and accident must have arisen out of and during
employment. Factory act 1948 defines various terms of factories like manufacturing process,
machinery, worker, power, prime mover etc. It lays down rules for fencing of machinery for
safeguard nearby work and machinery in motion. Now a days, Indian factory act of 1949 is
in force which presently also provides for a large number of regulations regarding safety for
health of workers which include cleanliness, ventilation and temperature controls, humidity,
protection against inhalation of dust and fumes, drinking water, overcrowding and proper
locations for spittoons etc.
This act also specify some important regulations with regard to the age of employees for
specific nature of jobs and also their respective permissible working hours in a day, week and
month in order to avoid excessive fatigue and ensure more safety. It also covers some
additional regulations regarding welfare of workers, their overtime duties, wages, first-aid
provisions and conditions of employment of young persons and women. All such provisions
collectively contribute to safe working conditions in the factories.
Beside above, various safety organizations in different parts of the world carry on regular
studies and research in causes of accidents and the methods of their prevention. These
organizations regularly issue their periodical bulletins in respect of their achievements regarding
safety. These bulletins can be referred frequently for keeping in touch with the latest techniques
and measures of safety. Few well known such organizations are Safety First Association of
India, National Safety Council of U.S.A, International Labor Office, Geneva, Factory
Department, Ministry of Labor, H.M.S.O., (U.K.), National Safety Council, Bombay, Industrial
Health Organization, Kanpur, All India Institute of Hygiene and Public Health, Calcutta.
Indian Council of Medical Research, New Delhi., Bureau of Indian Standards, New Delhi,
World Health Organization, The Royal Society for tile prevention of Accidents (ROSPA) London.,
British Standards, Institution, London., Occupational Safety and Health Administration,
Washington D.C, U.S.A., Bureau of Labor Standards, U.S.A, American Society of Safety
Engineers, Commonwealth Department of Labor and National Service, Australia. Canadian
Industrial Safety Association (CISA), Ontario, Canada, World Safety Organization (WSO), Manila,
International Occupational Safety and Health Information Center, Switzerland.
The main objectives of factory act are to provide protection to the workers employed in
factories against industrial hazards and to ensure safe and better working conditions. The
general provisions in the factory act with regard to the fencing of machinery and other safety
measures are summarized below:
Every moving part of a prime mover, fly-wheels connected to prime movers, head and
tail races of all water-wheels and turbines, any portion of bar stock that projects beyond the
head stock of lathe of in each factory shall be fenced securely by safety guards of robust
construction and these guards will always be kept in position while the part or machinery is
in operation or motion:
(i) All parts of an electric motor, generator and converter, all parts of transmission
machinery, all dangerous parts of any other machinery should be securely fenced
by means of safety guards unless they are located in such positions and/or their
construction ensures adequate safety for every person employed in the factory.
(ii) In case it becomes necessary to examine any part or parts of machinery while being
in motion only a specially trained adult worker should be deputed for the work.
(iii) Precautions against dangerous fumes.
46 Introduction to Basic Manufacturing Processes and Workshop Technology
Adequate protection should always be provided against dangerous fume. No person be
allowed to enter confined spaces, chamber, tanks etc. in which dangerous fumes are likely to
be present. If a manufacturing process is producing dust, fumes, or vapors, sufficient measures
should always be taken to prevent inhalation of the same by industrial personnel.
3.10.1 Scope of Factory Act Regulation
Every industrial establishment employing ten or more persons where manufacturing process
is carried on with the power and employing twenty or more persons where power is not used
for manufacturing process, come under the scope of this act. All types of seasonal and
perennial factories are included under this act without any distinction. The factory act has
been en-forced in all the states of India. For installing an industry licensing and registration
of the factory are also required from the government under the factory act regulation. Every
industry should be registered by sending the registration documents to the chief inspector of
factory with a written notice containing details of the factory such as the name of the factory,
name and address of the factory owner, details of power used type of production.
3.11 ELECTRICAL SAFETY MEASURES
If a person receives electric shock of mild or serious kind, directly or indirectly, the same
must be reported as electric accident. In case of stoppage of breathing after electric shock to
any victim, one should remove all sorts of obstructions from the mouth of the victim. Then
he should sit on his knees near the head of the victim and keep your both hands on his near
the collar bone, in such a way that the thumbs of both hands touch each other the fingers
remain open. He should press the back of the patient slowly and release the pressure on the
back and move up to the shoulders by sliding palms. Then the victim should be pulled upward
by holding the patient’s arm in between his elbows and shoulders. This process is repeated
until patient starts breathing himself.
Based on past experience, a number of rules and regulations have been made for handling
of electrical appliances. In industry, an inquiry is normally ordered for electrical accident.
Items carrying electricity should be properly insulated. Ageing of insulation withstand capacity
and should not be allowed to leak current. Switching contacts and point contacts should be
checked periodically to sparking and point heating. Important electric preventive measures
1. All metallic parts, externally accessible must always be earthed.
2. No inflammable materials are kept near electrical appliances, electric line wires or
electric control panels.
3. Electric safety devices like fuse, circuit breakers over-tripping must be always used
where ever required.
4. All defective and worn-out electric fittings must be replaced.
5. No untrained persons should be allowed to repair electrical faults.
6. Safety belts, helmet, rubber gloves, boots with rubber soles, and other safety items
always are used by electrician while dealing or working with high voltage. These
appliances should be provided to all electric mechanics.
7. Overloading of any electric circuit must be avoided.
8. The electric appliances when not in use must be dis-connected from main supply.
Industrial Safety 47
9. Power supply should be switched off always during maintenance work. Only
authorized person should be allowed to switch on and off’ the power supply.
10. One should avoid touching metal case of any electrical apparatus when it is in
11. Proper type of wiring should always be provided in all locations.
12. Periodical inspection should be done to detect the damages.
13. Always avoid overloading on any single point.
14. Good standards of safety items must be maintained as per norms.
3.12 FIRE PREVENTION
Accidents due to fire cause enormous damage to properties, manpower and materials. It can
be noted that the origin of fire is combustion. The main factors for combustions are presence
of oxygen, availability of combustible materials and rise of temperature to the ignition point
for the material. The cause of fire accidents may be electric-short circuit, carelessness and
ignorance, spontaneous combustion, riots and rivalry etc. Prevention of the fire involves
preventing spreading of fire by covering it with incombustible material, rescuing the affected
persons from the spot, cooling ignition point of combustible items, taking suitable precautions
and educating the all staff and workers about the possible hazards out of the consumables that
spread fires, color coding of pressure vessel containing combustible fluids, maintaining fire
extinguisher and water points in shop floor for proper precaution in case fire hazard. In case
of outbreak of fire, immediate, corrective action is very much essential in order to provide
the best possible chance of extinguishing the fire as quickly as possible, thus reducing danger
to life and other damages to the minimum possible extent. As soon as fire breaks out, the
fire alarm must be raised to alert all. All employees must be fire conscious and must know
the fire drill, position of the nearest fire point and the nearest telephone or fire alarm. Near
to equipments such as blow lamps and welding torches, which may lead to fire hazards, a
suitable fire-extinguisher should be placed well within the easy reach of every one. Fire drills
and fire orders should be displayed on all departmental notice boards and at all fire points.
All employees must make themselves familiar with these orders. Fire exits and the escape
routes should be clearly marked and kept free from all kinds of obstructions. It is also very
important to stop fighting the fire and leave the area as soon as the fire appears to be beyond
control or escape route is threatened by fire or smoke obscures or threatens to obscure the
escape route. As far as possible, fire-extinguishers should be supported by brackets firmly
fixed to the wall at a convenient height at all fire points. There should be an instruction plate
for display along each side of an extinguisher, which gives details of operation and the type
of fire for which the particular extinguisher is suitable.
The following precautions should be taken for fire prevention:
1. The maximum number of workers and officers should be trained with fire fighting
systems and equipments.
2. Keep all flammable liquids in closed containers or in safe cylinders.
3. Effective fire warning signals.
4. All doors should be opened towards outside the workroom as means of escape in
case of fire.
5. The doors and windows to be used as exit in case of fire should be easily located.
These should be marked with red letters of adequate size.
48 Introduction to Basic Manufacturing Processes and Workshop Technology
6. Always select the least flammable liquid that will serve the purpose.
7. One should provide ventilation to prevent any accumulation of vapors.
8. Always provide suitable and adequate means of fire extinguishment.
9. Every operator should be familiar with the location of fire extinguishers and their
10. Proper clearance should always be there in between the heating device and any
11. Electrical wiring should be proper.
12. Always prohibit smoking, open flames and sparks near the flammable materials.
13. A free passageways and easily open-able windows should be always provided.
14. Provide always suitable means for the safe storage and handling of all fuel used.
15. Use of flammable liquids should be minimized
16. Safe disposal for the flammable liquid wastes must be provided.
17. No one is permitted to accumulate fuels or other combustibles near the source of
open fire or spark.
3.13 TYPES OF FIRE
There are three major types of fires which are given as under.
Type 1 Fires occurring due burning of ordinary combustible materials such as wood, cloth
and paper. Pouring water is the most effective way for extinguishing this kind of
Type 2 Fires occurring due burning of flammable liquids such as oils, petrol, grease and fat.
For extinguishing, blanket or smother this kind of fire, thus excluding oxygen,
water must never be used.
Type 3 Fires in this category involve live electrical equipment. The extinguishing agent
must be non-conducting of electricity and water must not be used for extinguishing
this kind of fire.
There are five basic kinds of fire extinguishers commonly used which are discussed as
1. Dry Powder Extinguishers
These extinguishers filled with dry powder may be of the gas pressure or stored air pressure
type. They are suitable for use on both Type 2 and Type 3 fires.
2. Foam Extinguishers
These are of two main types commonly called mechanical foam and chemical foam type of fire
extinguishers. They are effective against Type 2 fires.
3. Carbon Dioxide Type Fire Extinguishers
These are filled with the carbon dioxide. It is operated by means of a plunger, lever trigger
or by opening a valve. It is fitted with a distinctively shaped discharge horn. This type of fire
extinguisher has only limited effectiveness against Type 1 kind of fires. It is suitable for
extinguishing type 2 and 3 kinds of fires.
Industrial Safety 49
4. Water Filled Fire Extinguishers
The soda acid kind is the most common kind of water extinguishers. They are most suitable
for extinguishing fire for type 1. Such fires are resulting from ordinary combustible materials
such as wood cloth and paper.
5. Vaporizing Liquid Type Fire Extinguishers
They may be filled with either carbon tetrachloride (CTC.) or chlorobromethane (CBM) where
as CTC kinds of extinguishers may be of the pump, gas cartridge or stored pressure type. And
CBM may be either gas cartridge or stored pressure. These extinguishers are most effective
against electrical kind of fire (Type 3).
6. Stored Air Pressure Type Extinguishers
In stored air pressure type extinguishers, the container is pressurized with air when the
extinguisher is filled. The extinguisher is trigger operated and operation can be stopped at
any time by releasing the trigger grip. It is suitable for type 1 kind of fire only.
7. Gas Pressure Type Extinguishers
In gas pressure type extinguishers the water is expelled under pressure provided by carbon
dioxide gas released from cartridge filled inside the container. It is suitable for Type 1 kind
3.14 FIRST AID
Even after taking all necessary safety precautions and measures, sometimes accidents may
also occur in industries. After major or minor accidents, an injured worker requires immediate
preliminary treatment in the absence of same his condition may become highly critical. To
take care of such situations, industries must employ full time, at least a medical person who
has successfully completed his Red-Cross First-Aid Course, and who can give preliminary
treatment to the injured person. The injured person may later on be shifted safely to the
nearby hospital through the ambulance or otherwise through any vehicle or by other means
as per the availability of mode of transportation. Besides the above service, a first-aid personnel
should take care of those workers or employees who come across injury by minor cuts, burns
or electric shock. The first aid provider should bring the victim in first aid room for further
treatment. In case of fatal injury first aid provider should call the doctor as soon as possible
or to arrange the ambulance for taking the victim to the hospital. He should deal the victim
with full sympathy and make early arrangement to call the family member or some responsible
member so that adequate arrangements can be made in hospital for the due care of the
victim. If breathing has stopped, he or she should be provided artificial respiration immediately.
For first aid services, a first-aid box containing the following items is always kept ready
during working hours in the shops or nearby working places where there are chances accidents
Items of a First-Aid Box
Items Name Quantity
(i) Pair of scissors 1
(ii) Large size sterilized dressings 12
50 Introduction to Basic Manufacturing Processes and Workshop Technology
(iii) Medium size sterilized dressings 12
(iv) Small sized sterilized dressings 24
(v) Large size burn dressings 12
(vi) Packets of sterilized cotton wool 2
(vii) Rolled bandages 10 cm wide 12
(viii) Rolled bandages 5 cm wide 12
(ix) Bottle (4 oz) of salvolative having the doze and made 1
of administration indicated on label
(xi) Safety pins 2 packets
(xi) Eye drops 1 small bottle
(xii) Adhesive plaster 2 roller
(xiii) 4 oz bottle containing KMnO4 crystals, etc. 2
(xiv) 4 oz bottle containting a 2% alcoholic solution 1
(xv) Betadine ointment (50mg) 1
(xvi) Saframycine ointment (50mg) 1
(xvii) Detol 1
1. What do you mean by industrial safety? What are major safety objectives?
2. What is an accident? Describe briefly the common causes and sources of accidents.
3. Explain in brief the various methods of safety adopted in plant.
4. Explain briefly the safety precautions associated with material handling in the plant.
5. Describe briefly the general provisions of factories act 1948, regarding safety.
6. Discuss various methods used for artificial respiration required for a victim.
7. How fire can be prevented in industries? Explain in brief.
8. Describe the duty of first aid personnel.
Engineering materials used to manufacture of articles or products, dictates which manufacturing
process or processes are to be used to provide it the desired shape. Sometimes, it is possible
to use more than one manufacturing processes, then the best possible process must be
utilized in manufacture of product. It is therefore important to know what materials are
available in the universe with it usual cost. What are the common characteristics of engineering
materials such as physical, chemical, mechanical, thermal, optical, electrical, and mechanical?
How they can be processed economically to get the desired product. The basic knowledge of
engineering materials and their properties is of great significance for a design and manufacturing
engineer. The elements of tools, machines and equipments should be made of such a material
which has properties suitable for the conditions of operation. In addition to this, a product
designer, tool designer and design engineer should always be familiar with various kinds of
engineering materials, their properties and applications to meet the functional requirements
of the design product. They must understand all the effects which the manufacturing processes
and heat treatment have on the properties of the engineering materials. The general classification
4.2 CLASSIFICATION OF ENGINEERING MATERIALS
A large numbers of engineering materials exists in the universe such as metals and non
metals (leather, rubber, asbestos, plastic, ceramics, organic polymers, composites and semi
conductor). Some commonly used engineering materials are broadly classified as shown in
Fig. 4.1. Leather is generally used for shoes, belt drives, packing, washers etc. It is highly
flexible and can easily withstand against considerable wear under suitable conditions. Rubber
is commonly employed as packing material, belt drive as an electric insulator. Asbestos is
basically utilized for lagging round steam pipes and steam pipe and steam boilers because it
is poor conductor of heat, so avoids loss of heat to the surroundings. Engineering materials
may also be categorized into metals and alloys, ceramic materials, organic polymers, composites
and semiconductors. The metal and alloys have tremendous applications for manufacturing
the products required by the customers.
Metals and Alloys
Metals are polycrystalline bodies consisting of a great number of fine crystals. Pure metals
possess low strength and do not have the required properties. So, alloys are produced by
52 Introduction to Basic Manufacturing Processes and Workshop Technology
melting or sintering two or more metals or metals and a non-metal, together. Alloys may
consist of two more components. Metals and alloys are further classified into two major kind
namely ferrous metals and non-ferrous metals.
(a) Ferrous metals are those which have the iron as their main constituent, such as
pig iron, cast iron, wrought iron and steels.
(b) Non-ferrous metals are those which have a metal other than iron as their main
constituent, such as copper, aluminium, brass, bronze, tin, silver zinc, invar etc.
Metallic Materials Non-metallic Materials
Ferrous Non-ferrous Organic Inorganic
Steels Cast iron
Fig. 4.1 Classification of engineering materials
4.3 FERROUS METALS
Ferrous metals are iron base metals which include all variety of pig iron, cast iron wrought
iron and steels. The ferrous metals are those which have iron as their main constituents. The
ferrous metals commonly used in engineering practice are cast iron, wrought iron, steel and
alloy steels. The basic principal raw material for all ferrous metals is pig iron which is
obtained by smelting iron ore, coke and limestone, in the blast furnace. The principal iron
ores with their metallic contents are shown in Table 4.1.
Table 4.1 Types of Iron Ore
S.No. Iron ore Color Iron %
1. Haematite (Fe3O4) Red 70%
2. Magnetite (Fe2O3) Black 72%
3. Limonite Brown 62.5%
4. Siderite Brown 48%
4.3.1 Main Types of Iron
1. Pig iron
2. Cast iron
Ferrous Materials 53
(A) White cast iron
(B) Gray cast iron
(C) Malleable cast iron
(D) Ductile cast iron
(E) Meehanite cast iron
(F) Alloy cast iron
3. Wrought iron
(A) Plain carbon steels
1. Dead Carbon steels
2. Low Carbon steels
3. Medium Carbon steels
4. High Carbon steels
(B) Alloy steels
1. High speed steel
2. Stainless steel
Some important ferrous metals, their extraction, composition, properties and their common
applications are discussed in detail as under.
4.3.2 Pig Iron
Pig iron was originated in the early days by reduction or iron ores in blast furnace and when
the total output of the blast furnace was sand cast into pigs which is a mass of iron roughly
resembling a reclining pig. It is roughly of 20" × 9" × 4" in size. It is produced in a blast
furnace and is the first product in the process of converting iron ore into useful ferrous metal.
The iron ore on initial refining and heating in blast furnace becomes pig iron when the
impurities are burnt out in a blast furnace. Pig iron acts as the raw material for production
of all kinds of cast iron and steel products. It is obtained by smelting (chemical reduction of
iron ore in the blast furnace. It is of great importance in the foundry and in steel making
processes. It is partly refined in a cupola furnace that produces various grades of cast iron.
By puddling processes, wrought iron is produced from pig iron. Steel is produced from pig iron
by various steel making processes such as bessemer, open-hearth, oxygen, electric and spray
steel making. The charge in the blast furnace for manufacturing pig iron is
(a) Ore Consisting of iron oxide or carbonate associated with earth impurities.
(b) Coke A fuel
(c) Limestone A flux
In addition to iron, pig iron contains various other constituents in varying form of
impurity such carbon, silicon, sulphur, manganese and phosphorus etc. It has the following
approximate composition which is as given as under.
Carbon — 4 to 4.5% Phosphorus — 0.1 to 2.0%
Silicon — 0.4 to 2.0% Sulphur — 0.4 to 1.0%
Manganese — 0.2 to 1.5 % Iron — Remainder
54 Introduction to Basic Manufacturing Processes and Workshop Technology
Carbon exists in iron in free form (graphite) and/or in combined form (cementite and
pearlite). Pig iron is classified on the basis of contents of free and combined carbon as follows.
These classifications are also termed as grades.
1. Grey pig iron (Grades 1, 2 and 3)
Grey pig iron contains about 3% carbon in free form (i.e., graphite form) and about 1%
carbon in combined form. This is a soft type of pig iron.
2. White pig iron (Grades 4)
White pig iron is hard and strong. It contains almost all of the carbon in the combined
3. Mottled pig iron (Grade 5)
This type of pig iron is in between the grey and white variety. It has an average hardness
and molted appearance. The free and combined forms of carbon are in almost equal proportion
in mottled pig iron.
4.3.3 Cast Iron
Cast iron is basically an alloy of iron and carbon and is obtained by re-melting pig iron with
coke, limestone and steel scrap in a furnace known as cupola. The carbon content in cast iron
varies from 1.7% to 6.67%. It also contains small amounts of silicon, manganese, phosphorus
and sulphur in form of impurities elements.
188.8.131.52 General properties of cast iron
Cast iron is very brittle and weak in tension and therefore it cannot be used for making
bolts and machine parts which are liable to tension. Since the cast iron is a brittle material
and therefore, it cannot be used in those parts of machines which are subjected to shocks.
It has low cost, good casting characteristics, high compressive strength, high wear resistance
and excellent machinability. These properties make it a valuable material for engineering
purposes. Its tensile strength varies from 100 to 200 MPa, compressive strength from 400 to
1000 MPa and shear strength is 120 MPa. The compressive strength of cast iron is much
greater than the tensile strength. The carbon in cast iron is present either of the following
1. Free carbon or graphite.
2. Combined carbon or cementite.
The cast iron is classified into seven major kinds as follows:
(a) Grey cast iron, (b) White cast iron, (c) Mottled cast iron (d) Malleable cast iron, (e)
Nodular cast iron, (f) Meehanite cast iron. (g) Alloy cast iron and The chemical composition,
extraction, properties and general applications of these types of cast iron are discussed as
184.108.40.206 Grey cast iron
Grey cast iron is grey in color which is due to the carbon being principally in the form
of graphite (C in free form in iron). It contains:
C = 2.5 to 3.8%.
Si = 1.1 to 2.8 %
Ferrous Materials 55
Mn = 0.4 to 1.0%
P = less than 0.15%
S = less than 0.1%
Fe = Remaining
It is produced in cupola furnace by refining or pig iron.
(i) When fractured it gives grey color.
(ii) It can be easily cast.
(iii) It is marked by presence of flakes of graphite in a matrix of ferrite and pearlite or
austenite; graphite flakes occupy 10% of metal volume.
(iv) It can be easily machined and possesses machinability better than steel.
(v) It possesses lowest melting of ferrous alloys.
(vi) It possesses high vibration damping capacity.
(vii) It has high resistance to wear.
(viii) It possesses high fluidity and hence can be cast into complex shapes and thin
(ix) It possesses high compressive strength.
(x) It has a low tensile strength.
(xi) It has very low ductility and low impact strength as compared with steel.
The grey iron castings are mainly used for machine tool bodies, automotive cylinder
blocks, pipes and pipe fittings and agricultural implements. The other applications involved
(i) Machine tool structures such as bed, frames, column etc.
(ii) Household appliances etc.
(iii) Gas or water pipes for under ground purposes.
(iv) Man holes covers.
(v) Piston rings.
(vi) Rolling mill and general machinery parts.
(vii) Cylinder blocks and heads for I.C. engines.
(viii) Frames of electric motor.
(ix) Ingot mould. And
(x) General machinery parts.
(xi) Sanitary wares.
(xii) Tunnel segment.
220.127.116.11 White cast iron
The white color is due to the fact that the carbon is this iron is in combined form as iron
carbide which is commonly specified as cementite. It is the hardest constituent of iron. It is
56 Introduction to Basic Manufacturing Processes and Workshop Technology
produced in cupola furnace by refining or pig iron. The white cast iron may be produced by
casting against metal chills or by regulating analysis. The chills are used when a hard and
wear resistance surface is desired for products such as for wheels, rolls crushing jaw, crusher
plates. The chemical composition of white cast iron is given as under.
C = 3.2 to 3.6%
Si = 0.4 to 1.1 %
Mg = 0.1 to 0.4%
P = less than 0.3%
S = less than 0.2%
Fe = Remaining
(i) Its name is due to the fact that its freshly broken surface shows a bright white
(ii) It is very hard due to carbon chemically bonded with iron as iron carbide (Fe3C),
which is brittle also.
(iii) It possesses excellent abrasive wear resistance.
(iv) Since it is extremely hard, therefore it is very difficult to machine.
(v) Its solidification range is 2650-2065°F.
(vi) Shrinkage is 1/8 inch per foot.
(vii) The white cast iron has a high tensile strength and a low compressive strength.
(i) For producing malleable iron castings.
(ii) For manufacturing those component or parts which require a hard, and abrasion
resistant surface such as rim of car.
(iii) Railway brake blocks.
18.104.22.168 Ductile cast iron
When small quantities of magnesium or cerium is added to cast iron, then graphite
content is converted into nodular or spheroidal form and it is well dispersed throughout the
material. The resulting structure possesses properties more like cast steel than like the other
grades of cast iron. A typical structure of spheroidal cast iron is shown in Fig. 4.2. Graphite
is in spheroidal form instead of in flaky form. Its structure may be modified by alloys or heat
treatment, as in steel to produce austenite, acicular, martensite, pearlite, and ferrite structure.
Compositions of ductile cast iron are as follows:
Carbon = 3.2 to 4.2%
Silicon = 1.0 to 4.0 %
Magnesium = 0.1 to 0.8%
Nickel = 0.0 to 3.5%
Manganese = 0.5 to 0.1%
Iron = Remaining
Ferrous Materials 57
Fig. 4.2 Typical structure of spheroidal cast iron
Silicon is also used as an alloying element since it has no effect on size and distribution
of carbon content. The magnesium controls the formation of graphite. But it has little influence
on the matrix structure. Nickel and manganese impart strength and ductility. Ductile cast
iron has high fluidity, excellent castability, strength, high toughness, excellent wear resistance,
pressure tightness, weldability and higher machinability in comparison to grey cast iron.
22.214.171.124 Malleable cast iron
The ordinary cast iron is very hard and brittle. Malleable cast iron is unsuitable for
articles which are thin, light and subjected to shock. It can be flattened under pressure by
forging and rolling. It is an alloy in which all combined carbon changed to free form by
suitable heat treatment. Graphite originally present in iron in the form of flakes which is the
source of weakness and brittleness. Carbon in this cast iron is dispersed as tiny specks instead
of being flaky or in combined form. The tiny specks have not such weakening effect and
casting would not break when dropped. The tensile strength of this cast iron is usually higher
than that of grey cast iron. It has excellent machining quality and is used for making machine
parts for which the steel forging and in which the metal should have a fair degree of
machining accuracy e.g., hubs of wagon, heels small fittings for railway rolling brake supports,
parts of agricultural machinery, pipe fittings, hinges, locks etc.
It can be obtained by annealing the castings. The cast iron castings are packed in an
oxidizing material such as iron ore or in an inert material such as ground fire clay depends
upon the process used either white heart or black heart. The packed casting is put into an
oven and is heated around 900°C temperature and is kept at that temperature for about two
days and it is then allowed to cool slowly in the furnace itself. Iron ore acting as an oxidizing
agent reacts with C and CO2 escape. Thus annealed cast product is free from carbon. If the
castings are packed in an inert material then slow cooling will separate out the combined
carbon to temper carbon. To produce malleable casting, first casting is produced which has
all combined carbon. The produced castings are then heat-treated in a special manner according
to white heart method or black heart method.
White heart malleable iron casting
The castings taken out of the mould are put into a drum having sand and powdered slag.
The drum is then closed and kept in the air furnace and it is raised to highly temperature
slowly. The temperature is raised to 920°C in two days time, kept at this temperature for
nearly up to 50 to 80 hours then the drum is allowed to cool in the furnace (generally air
furnaces) at the rate 5 to 10°C per hour till it reaches to room temperature. The whole cycle
takes about one weak. During this treatment combined carbon separates out and all the
58 Introduction to Basic Manufacturing Processes and Workshop Technology
carbon does not change into graphite state but change in other form of free carbon called
Fe3C ——→ 3Fe + C
This makes the casting less brittle and malleable. The fracture portion of such a casting
is dark grey or black in appearance. These castings are specially used in automobile industries.
Black heart malleable iron casting
The castings packed in a drum of oxidizing media which is generally powdered iron ore
or powered scale (film of Fe3O4 on surface). This close drum is kept in the furnace and heated
to 900°C. It is then maintained at this temperature to nearly 40 to 70 hours and allowed to
cool slowly in a furnace itself. The castings become malleable like white heart cast iron. The
percentage of carbon and silicon should be so selected that it can promote the development
of free carbon when these castings are annealed.
1. Malleable cast iron is like steel than cast iron.
2. It is costly than grey cast iron and cheaper than softer steel.
Malleable cast iron are generally used to form automobile parts, agriculture
implementation, hinges, door keys, spanners mountings of all sorts, seat wheels, cranks,
levers thin, waned components of sewing machines and textiles machine parts.
126.96.36.199 Meehanite cast iron
Meehanite cast iron is an inoculated iron of a specially made white cast iron. The
composition of this cast iron is graphitized in the ladle with calcium silicide. There are various
types of meehanite cast iron namely heat resisting, wear resisting and corrosion resisting
kind. These materials have high strength, toughness, ductility and good machinability. It is
highly useful for making castings requiring high temperature applications.
188.8.131.52 Alloy cast iron
The cast irons as discussed above contain small percentages of other constituents like
silicon, manganese, sulphur and phosphorus. These cast irons may be called as plain cast
irons. The alloy cast iron is produced by adding alloying elements like nickel, chromium,
molybdenum, copper and manganese in sufficient quantities in the molten metal collected in
ladles from cupola furnace. These alloying elements give more strength and result in
improvement of properties. The alloy cast iron has special properties like increased strength,
high wear resistance, corrosion resistance or heat resistance. The alloy cast irons are
extensively used for automobile parts like cylinders, pistons, piston rings, crank cases, brake
drums, parts of .crushing and grinding machinery etc.
184.108.40.206 Effect of impurities on cast iron
The cast iron contains small percentages of carbon, silicon, sulphur, manganese and
phosphorus. The affect of these impurities on the cast iron are as follows:
(1) Carbon. Carbon is one of the important elements in cast iron. It reduces melting
point of iron. Pure iron has a melting point of about 1500°C but iron with 3.50% C
has melting point of about 1350°C. When carbon is in free form i.e. as graphite form,
Ferrous Materials 59
the resulting cast iron is known grey cast iron. On the other hand, when the iron
and carbon are chemically combined form of cementite, the cast iron will be hard
and known as white cast iron.
(2) Silicon. Presence of silicon in cast iron promotes the decomposition of cementite
into graphite. It also helps to reduce the shrinkage in cast iron when carbon is
changed to graphite forms.
(3) Sulphur. It makes the cast iron hard and brittle. Since too much sulphur gives
unsound casting, therefore, it should be kept below 0.1% for most casting purposes.
It is often responsible for creating troubles to foundry men. It will make cast iron
hard thereby counteracting the softening influences of silicon. It decreases strength
and increases brittleness. It also promotes oxidation of cast iron. Hence, it is kept
as low as possible in cast iron.
(4) Manganese. It makes cast iron white and hard. It is often kept below 0.75%. It
helps to exert a controlling influence over the harmful effect of sulphur. It reduces
the harmful effects of the sulphur by forming the manganese sulphide which is not
soluble in cast iron.
(5) Phosphorus. It increases fusibility and fluidity in cast iron but induces brittleness.
It is rarely allowed to exceed 1 %. Phosphorus in irons is useful for casting of
intricate shapes and for producing very cheap and light engineering castings.
Phosphorus has no effect on the carbon as well as on shrinkage in the cast iron.
220.127.116.11 Comparison among grey, white and spherodidal cast iron
The comparison among grey, white and spherodidal cast iron is given in Table 4.2.
TABLE 4.2 Comparison among Grey, White and Spherodidal Cast Iron
S.No Grey Cast Iron White Cast Iron Spherodidal Cast Iron
1. It is an alloy of carbon and
silicon with iron having grey
color when fractured. It is
marked by the presence of
flakes of matrix of ferrite,
pearlite or austenite.
Carbon in iron exists in free
form as graphite
White cast iron has almost
all its carbon as iron carbide.
Its broken surface shows a
bright white fracture.
Graphite appears as around
Particles or spheroids.
2 It has good machinability,
high resistance to wear,
high vibration damping
capacity and high
It has poor machinability,
excellent abrasive wear
It has good machinability, good
damping, excellent castability
and sufficient wear resistance
3 It is used in machine tool
structure, Main-hole covers,
cylinder blocks, heads for
I.C. engines, gas or water
pipes for underground
purposes, frames for
electric motors, piston
rings and sanitary wares.
It is used for producing
malleable iron castings and
structural component parts
which require a hard and
abrasion resistant material.
It is used in I.C. engines, paper
Industry machinery, machinery for
farming and tractor, application,
earth moving machinery, valve
and fittings, pipes, pumps,
compressors and construction
60 Introduction to Basic Manufacturing Processes and Workshop Technology
4.3.4 Wrought Iron
Wrought iron is the assumed approximately as purest iron which possesses at least 99.5%
iron. It contains a large number of minute threads of slag lying parallel to each other, thereby
giving the metal a fibrous appearance when broken. It is said as a mechanical mixture of very
pure iron and a silicate slag. It can also be said as a ferrous material, aggregated from a
solidifying mass of pasty particles of highly refined metallic iron with which a minutely and
uniformly distributed quantity of slag is incorporated without subsequent fusion. This iron is
produced from pig iron by re-melting it in the puddling furnace or air furnace or reverberatory
furnace. The molten metal free from impurities is removed from the furnace as a pasty mass
of iron and slag. The balls of this pasty mass, each about 45 to 65 kg in weight, are formed.
These balls are then mechanically worked to squeeze out the slag and to form it into some
commercial shape. This iron contains practically no carbon and therefore can not be hardened.
A chemical composition range of typical wrought iron includes:
C = 0.02 – 0.03% P = 0.05 – 0.25% Si = 0.02 – 0.10%
S = 0.008 – 0.02% Mn = 0.0 – 0.02% Slag = 0.05 – 1.5%
Fe = remainder
The wrought iron can be easily shaped by hammering, pressing, forging, etc. It is never
cast and it can be easily bent when cold. It is tough and it has high ductility and plasticity
with which it can be forged and welded easily. Its ultimate strength can be increased considerably
by cold working followed by a period of aging. It possesses a high resistance towards corrosion.
It can accommodate sudden and excessive shocks loads without permanent injury. It has a
high resistance towards fatigue. Its ultimate tensile strength is 2,500 kg/cm2 to 5,000 kg/cm2
and the ultimate compressive strength is 3,000 kg/cm2. It can be elongated considerably by
cold working. It has high electrical conductivity. The melting point of wrought iron is about
1530°C. It has elongation 20% in 200 mm in longitudinal direction and 2–5 % in transverse
direction. Its poison’s ratio is 0.30. It can be easily formed when cold, without the outer side
cracking at the formed portion.
It is used for making chains, crane hooks, railway couplings, and water and steam pipes.
It has application in the form of plates, sheets, bars, structural works, forging blooms and
billets, rivets, and a wide range of tubular products including pipe, tubing and casing, electrical
conduit, cold drawn tubing, nipples and welding fittings, bridge railings, blast plates, drainage
lines and troughs, sewer outfall lines, weir plates, sludge tanks and lines, condenser tubes,
unfired heat exchangers, acid and alkali process lines, skimmer bars, diesel exhaust and air
brake piping, gas collection hoods, coal equipment, cooling tower and spray pond piping.
Steel is an alloy of iron and carbon with carbon content maximum up to 1.7%. The carbon
occurs in the form of iron carbide, because of its ability to increase the hardness and strength
of the steel. The effect of carbon on properties of steel is given in Fig. 4.3. Other elements
e.g. silicon, sulphur, phosphorus and manganese are also present to greater or lesser amount
to import certain desired properties to it. Most of the steel produced now-a-days is plain
Ferrous Materials 61
carbon steel. Carbon steel has its properties mainly due to carbon content and does not
contain more than 0.5% of silicon and 1.5% of manganese.
0 0.2 0.4 0.6 0.8 1.0 1.2
Fig. 4.3 Effect of carbon on properties of steel
For checking microstructure of steel, its specimen is prepared by preparing a flat mirror
surface on small piece of metal through rubbing by sand papers, polishing and buffing etc.
This surface is then followed by etching with a chemical solution. The chemical solution
reacts with various constituents in varying degree to reveal crystal structure clearly. The
revealed structure is then viewed through powerful microscope. The viewed micro structures
for different steel are depicted in Fig. 4.4.
Fig. 4.4 Micro structure of steel
18.104.22.168 Effect of impurities on steel
The effects of impurities like silicon, sulphur, manganese and phosphorus, on steel as
1. Silicon. Silicon content in the finished steel usually ranges from 0.05 to 0.30%. It
is added in low carbon steels for preventing them from becoming porous. It helps
in removing the gases and oxides. It prevents blow holes there by making steel
tougher and harder.
62 Introduction to Basic Manufacturing Processes and Workshop Technology
2. Sulphur. It renders free cutting properties in steel. It is found in steel either as
iron sulphide or manganese sulphide. Iron sulphide due to its low melting point,
produces brittleness whereas manganese sulphide does not affect so much. Therefore,
manganese sulphide is less objectionable in steel than iron sulphide.
3. Manganese. It serves as a valuable deoxidizing and purifying agent, in steel.
Manganese also combines with sulphur and thereby decreases the harmful effect of
this element remaining in the steel. It increases wear resistance, hardness and
strength and decreases machineability. When used in ordinary low carbon steels,
manganese makes the metal ductile and of good bending quantities. In high speed
steels, it is used to tougher the metal and to increase its critical temperature.
4. Phosphorus. It induces brittleness in steel. It also produces cold shortness in steel.
In low carbon steels, it raises the yield point and improves the resistance to atmospheric
corrosion. The sum of carbon and phosphorus usually does not exceed 0.25%.
To produce needed improvement in properties of plain carbon steel, certain elements in
steel are alloyed for specific purposes to increase wearing resistance, electrical and mechanical
properties which cannot be obtained in plain carbon steels.
The steel may be of various kinds and few important types are explained as under.
22.214.171.124 Plain carbon steel
Plain carbon steel is an alloy of iron and carbon. It has good machineability and malleability.
It is different from cast iron as regards the percentage of carbon. It contains carbon from 0.06
to 1.5% whereas cast iron possesses carbon from 1.8 to 4.2%. Depending upon the carbon
content, a plain carbon steels can divided to the following types:
1. Dead carbon steel — up to 0.15% carbon
2. Low carbon or mild steel — 0.15% to 0.45% carbon
3. Medium carbon steel — 0.45% to 0.8% carbon
4. High carbon steel — 0.8% to 1.5% carbon
Each type is discussed as under.
DEAD CARBON STEEL
It possesses very low percentage of carbon varying from 0.05 to 0.15%. It has a tensile
strength of 390 N/mm2 and a hardness of about 115 BHN. Steel wire, sheets, rivets, screws,
pipe, nail and chain are made from this steel. This steel is used for making camshafts, sheets
and strips for fan blades, welded tubing, forgings, chains, stamping, rivets, nails, pipes,
automobile body etc.
LOW CARBON OR MILD STEEL
Low carbon steel is sometimes known as mild steel also. It contains 0.20 to 0.30% C
which has tensile strength of 555 N/mm2 and hardness of 140 BHN. It possesses bright
fibrous structure. It is tough, malleable, ductile and more elastic than wrought iron. It can
be easily forged and welded. It can absorb shocks. It rusts easily. Its melting point is about
1410°C. It is used for making angle, channels, case hardening steel, rods, tubes, valves, gears,
crankshafts, connecting rods, railway axles, fish plates, small forgings, free cutting steel shaft
and forged components etc.
Ferrous Materials 63
1. Mild steel containing 0.15 to 0.20% carbon
It is used in structure steels, universal beams, screws, drop forgings, case hardening
steel, bars, rods, tubes, angles and channels etc.
2. Mild steel containing 0.20-0.30% carbon
It is used in making machine structure, gears, free cutting steels, shafts and forged
MEDIUM CARBON STEELS
Medium carbon steel contains carbon from 0.30 to 0.8%. It possesses having bright
fibrous structure when fractured. It is tough and more elastic in comparison to wrought iron.
It can be easily forged, welded, elongated due to ductility and beaten into sheets due to its
good malleability. It can easily absorb sudden shocks. It is usually produced as killed or semi
killed steels and is harden able by treatment. Hardenability is limited to thin sections or to
the thin outer layer on thick parts. Its tensile strength is better than cast iron and wrought
iron but compressive strength is better than wrought iron but lesser than cast iron. It rusts
readily. Its melting point is 1400°C. It can be easily hardened and it possesses good balance
of strength and ductility.
It is generally used for making railway coach axles, bolts, connecting rods, key stock,
wires and rods, shift and break levers, spring clips, gear shafts, small and medium forgings,
railway coach axles, crank pins on heavy machines, spline shafts, crankshafts, forging dies,
set screws, die blocks, self tapping screws, clutch discs, valve springs, plate punches, thrust
washers etc. The applications of different kinds of medium carbon steel are given as under.
1. Plain carbon steels having carbon % 0.30 to 0.45. Axles, special duty shafts,
connecting rods, forgings, machinery steel, spring clips, turbine, rotors, gear shafts,
key stock, forks and bolts.
2. Plain carbon steels having carbon % 0.45 to 0.60. Railway coach axles, crank
pins, crankshafts, axles, spline shafts, loco tyres.
3. Plain carbon steels having carbon % 0.60 to 0.80. Drop forging dies, die blocks,
bolt heading dies, self-tapping screws, valve spring, lock washers, hammers, cold
chisels, hacksaws, jaws for vices etc.
HIGH CARBON STEELS
High carbon steels (HCS) contain carbon from 0.8 to 1.5%. Because of their high hardness,
these are suitable for wear resistant parts. Spring steel is also high carbon steel. It is
available in annealed and pre-tempered strips and wires. High carbon steel loses their hardness
at temperature from 200°C to 250°C. They may only be used in the manufacture of cutting
tools operating at low cutting speeds. These steels are easy to forge and simple to harden.
These steels are of various types which are identified by the carbon percentage, hardness and
HCS containing 0.7 to 0.8% carbon possesses hardness of 450-500 BHN. It has application
for making cold chisels, drill bits, wrenches, wheels for railway service, jaws for vises,
structural wires, shear blades, automatic clutch discs, hacksaws etc.
64 Introduction to Basic Manufacturing Processes and Workshop Technology
Steel containing 0.8 to 0.9% C possesses hardness of 500 to 600 BHN. This steel is
used for making rock drills, punches, dies, railway rails clutch discs, circular saws, leaf
springs, machine chisels, music wires,
Steel containing 0.90 to 1.00% carbon is also known as high carbon tool steel and it
possesses hardness of 550-600 BHN. Such steel is used for making punches, dies, springs keys
and shear blades.
Steel containing 1.0 to 1.1 % C is used for making railway springs, mandrels, taps,
balls, pins, tools, thread metal dies.
Steel containing 1.1 to 1.2% C is used for making taps, twist drills, thread dies, knives.
Steel containing 1.2 to 1.3% carbon is used for making files, reamers Files, dies for
wire drawing, broaches, saws for cutting steel, tools for turning chilled iron.
Cutting tool materials imply the materials from which various lathe tools or other
cutting tools are made. The best tool material to use for a certain job is the one that will
produce the machined part at the lowest cost. To perform good during cutting, the tool
material should possess the following properties for its proper functioning.
1. A low coefficient of friction between tool material and chip material.
2. Ability to resist softening at high temperature.
3. Ability to absorb shocks without permanent deformation.
4. Sufficient toughness to resist fracture and bear cutting stresses.
5. Strength to resist disintegration of fine cutting edge and also to withstand the
stresses developed, during cutting, in the weakest part of the tool.
6. High hardness that means tool must be harder than the material being cut.
According to Indian standard IS 1570-1961, plain carbon steels are designated by the
alphabet ‘C’ followed by numerals which indicate the average percentage of carbon in it. For
example C40 means a plain carbon steel containing 0.35% to 0.45% C (0.40% on average),
although other elements like manganese may be present. In addition to the percentage of
carbon, some other specification may include e.g. C55Mn75 means the carbon content lies
between 0.50% to 0.60% and the manganese content lies between 0.60 to 0.90%. It may be
noted that only average contents are specified in such designation of steel.
126.96.36.199 Alloy steel
For improving the properties of ordinary steel, certain alloying elements are added in it
in sufficient amounts. The most common alloying elements added to steel are chromium,
nickel, manganese, silicon, vanadium, molybdenum, tungsten, phosphorus, copper, that the
titanium, zirconium, cobalt, columbium, and aluminium. Each of these elements induces
certain qualities in steels to which it is added. They may be used separately or in combination
to produce desired characteristics in the steel. The main purpose of alloying element in steel
is to improve machinability, elasticity, hardness, case hardening, cutting ability, toughness,
wear resistance, tensile strength, corrosion resistance, and ability to retain shape at high
temperature, ability to resist distortion at elevated temperature and to impart a fine grain
size to steel. Like carbon, a number of alloying elements are soluble to produce alloys with
improved strength, ductility, and toughness. Also carbon, besides forming an inter-metallic
compound with iron, combines with many alloying elements and form alloy carbides. These
alloy carbides as well as iron-alloy carbides are usually hard and lack in toughness. Some
Ferrous Materials 65
alloying elements are added to prevent or restrict grain growth. Aluminium is considered the
most effective in this respect. Others are zirconium, vanadium, chromium, and titanium. The
addition of alloying elements almost always affects the austenite-ferrite transformation
mechanism. Some alloying elements lower and some raise the critical temperature. The
compositional and structural changes produced by alloying elements change and improve the
physical, mechanical and processing properties of steel.
188.8.131.52 Effect of alloying elements in steel
The chief alloying elements used in steel are nickel, chromium, molybdenum, cobalt,
vanadium, manganese, silicon and tungsten. Each of these elements possesses certain qualities
upon the steel to which it is added. These elements may be used separately or in combination
to produce the desired characteristic in steel. Following are the effects of alloying elements
1. Nickel. Steels contain 2 to 5% nickel and from 0.1 to 0.5% carbon increase its
strength and toughness. In this range, nickel contributes great tensile strength,
yield strength, toughness and forming properties and hardness with high elastic
limit, good ductility and good resistance to corrosion. An alloy containing 25% nickel
possesses maximum toughness and offers the greatest resistance to rusting, corrosion
and burning at high temperature. It has proved beneficial in the manufacture of
boiler tubes, valves for use with superheated steam, valves for I.C. engines and
sparking plugs for petrol engines. A nickel steel alloy containing 36% of nickel is
known as invar. It has nearly zero coefficient of expansion. Therefore, it is in great
demand for making measuring instruments for everyday use.
2. Chromium. It improves corrosion resistance (about 12 to 18% addition). It increases
tensile strength, hardness, wear resistance and heat resistance. It provides stainless
property in steel. It decreases malleability of steel. It is used in steels as an alloying
element to combine hardness with high strength and high elastic limit. It also
imparts corrosion resisting properties to steel. The most common chrome steels
contain from 0.5 to 2% chromium and 0.1 to 1.5% carbon. The chrome steel is used
for balls, rollers and races for bearings. A Nickel-Chrome steel containing 3.25%
nickel, 1.5% chromium and 0.25% carbon is much used for armour plates. Chrome
nickel steel is extensively used for motor car crank shafts, axles and gears requiring
great strength and hardness.
3. Tungsten. It increases hardness, wear resistance, shocks resistance and magnetic
reluctance. It increases ability to retain hardness and toughness at high temperature.
It prohibits grain growth and increases wear resistance, shock resistance, toughness,
and the depth of hardening of quenched steel. The principal uses of tungsten steels
are for cutting tools, dies, valves, taps and permanent magnets.
4. Vanadium. It improves tensile strength, elastic limit, ductility, fatigue resistance,
shock resistance and response to heat treatment. It also acts as a degasser when
added to molten metal. It aids in obtaining a fine grain structure in tool steel. The
addition of a very small amount of vanadium (less than 0.2%) produces a marked
increase in tensile strength and elastic limit in low and medium carbon steels without
a loss of ductility.The chrome- vanadium steel containing about 0.5 to 1.5% chromium,
0.15 to 0.3% vanadium and 0.13 to 1.1% carbon have extremely good tensile strength,
elastic limit, endurance limit and ductility. These steels are frequently used for parts
such as springs, shafts, gears, pins and many drop forged parts.
66 Introduction to Basic Manufacturing Processes and Workshop Technology
5. Molybdenum. A very small quantity (0.15 to 0.30%) of molybdenum is generally
used with chromium and manganese (0.5 to 0.8%) to make molybdenum steel. It
increases hardness, wear resistance, thermal resistance. When added with nickel,
it improves corrosion resistance. It counteracts tendency towards temper brittleness.
It makes steel tough at various hardness levels. It acts as a grain growth inhibitor
when steels are heated to high temperatures. Molybdenum steels possesses hardness,
wear resistance, thermal resistance and extra tensile strength. It is used for air-
plane fuselage and automobile parts. It can replace tungsten in high speed steels.
6. Cobalt. When added to steel, it refines the graphite and pearlite and acts as a grain
refiner. It improves hardness, toughness, tensile strength and thermal resistance.
7. Titanium. It acts as a good deoxidizer and promotes grain growth. It prevents
formation of austenite in high chromium steels. It is the strongest carbide former.
It is used to fix carbon in stainless steels and thus prevents the precipitation of
8. Aluminium. It is used as a deoxidizer. If present in an amount of about 1 %, it
helps promoting nitriding.
9. Copper. It improves resistance to corrosion. It increases strength. More than 0.6
per cent copper for precipitation.
10. Silicon. It improves magnetic permeability and decreases hysteresis losses. It
decreases weldability and forgeability. It is also added as a deoxidizer during casting
of ingots. It takes care of oxygen present in steel by forming SiO2. Silicon steels
behave like nickel steels. These steels have a high elastic limit as compared to
ordinary carbon steel. Silicon steels containing from 1 to 2% silicon and 0.1 to 0.4%
carbon and other alloying elements are used for electrical machinery, valves in I.C.
engines, springs and corrosion resisting materials.
11. Manganese. It improves the strength of the steel in both the hot rolled and heat
treated condition. The manganese alloy steels containing over 1.5% manganese with
a carbon range of 0.40 to 0.55% are used extensively in gears, axles, shafts and
other parts where high strength combined with fair ductility is required. The principal
use of manganese steel is in machinery parts subjected to severe wear. These steels
are all cast and ground to finish.
12. Carbon. It increases tensile strength and hardness. It decreases ductility and
weldability. It affects the melting point.
184.108.40.206 Free cutting steel
The important features of free cutting steels are their high machinability and high
quality surface finish after finishing. These properties are due to higher sulphur and phosphorus.
Sulphur exists in the form of manganese sulphide (MnS) which forms inclusions in steel.
These inclusions promote the formation of discontinuous chips and also reduce friction on the
surface being machined so produces good surface finish easily. Phosphorus is dissolved in the
ferrite and increases hardness and brittleness. Lead up to 0.35% can be added to improve the
machinability of steel. These have high sulphur content present in form of manganese sulphide
inclusions causing the chips to break short on machining. Mn and P make steel hardened and
brittle. Lead (0.2% to 0.35%) is sometimes added to steel improving machinability properties
of steel. This consists of three Bessemer grades B1111, B1112, B1113 which differ in sulphur
content and the sulphurised steels from C1108 to C1151. The tool life achieved in machining
Ferrous Materials 67
free cutting steels is from 2 to 2.5 times higher than when carbon steels of the same carbon
content. However, it must be noted that free cutting steels have lower dynamic strength
characteristics and are more susceptible to corrosion. Free cutting steels are frequently
supplied in the cold drawn or work hardened form. These cold drawn steels have a high
tensile strength and hardness but less ductile when compared to other kind of steels.
Applications of free cutting steel
These steels are used for manufacturing axles, bolts, screws, nuts, special duty shafts,
connecting rods, small and medium forgings, cold upset wires and rods, solid turbine rotors,
rotor and gear shaft, armature, key stock, forks and anchor bolts screw stock, spring clips,
tubing, pipes, light weight rails, concrete reinforcing etc.
220.127.116.11 Nickel steel
The percentage of Nickel varies from 2 to 45 in steel. Steel having 2% Ni makes steel
more suitable for rivets, boiler plates, bolts and gears etc. Steel having Ni from 0.3 to 5%
raises elastic limit and improves toughness. Steel containing Nickel has very high tensile
strength. Steel having 25% Ni makes it stainless and might be used for I.C. engine turbine
blade etc. If Ni is present up to 27%, it makes the steel non-magnetic and non-corrodible.
Invar (Ni 36%) and super-invar (Ni 31%) are the popular materials for least coefficient of
expansion and are used for measuring instruments, surveyor tapes and clock pendulums.
Steel having 45% Ni steel possesses extension equal to that of glass, a property very import
making links between the two materials i.e. in electronic valves and bulbs.
18.104.22.168 Vanadium steel
Vanadium when added even in small proportion to an ordinary low carbon increases
significantly its elastic limit and fatigue resistance property. Vanadium makes steel strong and
tough. When vanadium is added up to 0.25%, the elastic limit of the steel is raised by 50%
can resist high alternating stresses and severe shocks.
1. It is widely used for making tools.
2. It can also be used for shafts, springs, gears, steering knuckles and drop forged
22.214.171.124 Manganese steel
Manganese when added in steel between 1.0 to 1.5% makes it stronger and tougher.
Manganese between 1.5 to 5% in steel makes it harder and more brittle. 11 to 14% manganese
in steel with carbon 0.8 to 1.5% makes it very hard, tough, non-magnetic and possesses
considerably high tensile strength. Manganese steel may be forged easily but it is difficult to
machine and hence it is usually ground. It is weldable and for welding it, a nickel manganese
welding rod is used.
1. Because of work hardening, it is suitable for jaws of stone and ore crushers, grinding
plants, tramway and railway points and crossing etc.
2. Manganese steel in the form of bars is now widely used for screening coke.
3. It is also used for helmets and shields.
4. It is used for agricultural implements such as shovels etc.
68 Introduction to Basic Manufacturing Processes and Workshop Technology
126.96.36.199 Tungsten Steel
Tungsten when added to steel improves its magnetic properties and hardenability. When
tungsten is added to an extent of 6% to high carbon steel, it retains the magnetic properties
to high degree and produce field more intense than ordinary steel. Steel having 8% tungsten
gives sufficient hardness to it to scratch even glass.
It is used for making permanent magnets and high speed cutting tools.
188.8.131.52 Silicon steel
Silicon addition improves the electrical properties of steel. It also increases fatigue
strength and ductility.
1. Steel with
Mn = 1 %, Si = 2% and C = 0.4 to 0.6%
has very high elastic limit and is used for springs.
2. Steel containing 5 to 7% silicon
retains its hardness and resistance to oxidation at high temperature. It is used for
making internal combustion engines.
3. Steel possessing 13% Si has a very high corrosion resistance and it can be used in
chemical industrial applications.
4. Steel possessing 1% Si and up to 0.95% Mn is suitable for structural purposes.
184.108.40.206 Magnetic steels
Steels having 15 to 40% Co, 0.4 to 1 % C, 1.5 to 9% Cr, 0-10% W and remaining Fe
possesses very good magnetic properties. High Cobalt steels, when correctly heat treated, are
frequently used in the making of permanent magnets for magnetos, loud speakers and other
electrical machines. An important permanent magnet alloy called Alnico contains approximately
60% Iron, 20% Nickel, 8% Cobalt and 12% Aluminium. This alloy cannot be forged and is used
as a casting hardened by precipitation heat treatment.
220.127.116.11 Heat resisting steels
Heat resisting steels are practically suitable for working at even very high temperatures.
Such steels must resist the influences which lead to failure of ordinary steels when put to
work under high temperatures. Alloy steel containing 23-30% chromium with less than 0.35%
C are mainly used to impart heat resisting service in the temperature range between 815-
1150 °C. The furnace parts and annealing boxes are generally made by this steel. These steels
are particularly suitable for working at high temperatures and are thus stable at high
temperatures. A steel containing chromium, nickel and tungsten, with the carbon content
suitably controlled provide useful combination of non-scaling and strength retaining properties
at high temperature. Such steels can work satisfactory up to 700°C and contains 0.15% C, 0.5
to 2 % Si, 0.5% Mn, 1.0 to 6%, Cr and 0.5%. Mo.
These are used in nuclear power plant, furnaces, supersonic aircrafts, missiles, annealing
Ferrous Materials 69
18.104.22.168 Spring steels
Spring steels are used for the making springs. Various types of these steel along with
their composition and uses are discussed as under.
(i) Carbon-manganese spring steels. This type of steel contains
C = 0.45 to 0.6, Si = 0.1 to 0.35% and Mn = 0.5 to 1.0%.
These steels are quenched and tempered up to 350 BHN. They are widely used for
laminated springs for railway and general purposes.
(ii) Hyper-eutectoid spring steels. This type of steel contains
C = 0.9 to 1.2%, 0.3% (max) and Mn = 0.45 to 0.70%.
These steels are oil quenched and tempered at low temperature. This type of steel
is used for volute and helical springs.
(iii) Silicon-manganese spring steels. This type of steel contains
C = 0.3 to 0.62%, Si = 1.5 to 2% and Mn = 0.6 to 1 %.
These steels are hardened and tempered. This type of steel is used for the
manufacturing of railway and road springs generally.
22.214.171.124 Structural steels
Structural steels possess high strength and toughness, resistance to softening at elevated
temperatures and enough resistance to corrosion. In addition, they should possess weldability,
workability and high hardenability. The principal alloying elements in structural steels are
chromium, nickel and manganese. These steels has various applications which are given as
They are used for structural members of bridges, buildings, rail road, cars etc. They are
also used for manufacturing components subjected to static and dynamic loads. These
components include valves, pins, studs, gears, clutches, bushes, shafts etc.
126.96.36.199 Stainless steel
Stainless steel contains chromium together with nickel as alloy and rest is iron. It has
been defined as that steel which when correctly heat treated and finished, resists oxidation
and corrosive attack from most corrosive media. Stainless steel surface is responsible for
corrosion resistance. Minimum chromium content of 12% is required for the film’s formation,
and 18% is sufficient to resist the most severe atmospheric corrosive conditions. Their principal
alloying element is chromium while some other elements like nickel, manganese etc. can also
be present in small amounts. Addition of nickel improves ductility and imparts strength.
Corrosion resistance to stainless steels increases with increase in nickel content against
neutral chloride solution and weakly oxidizing acids. Addition of molybdenum improves its
resistance to sulphuric, sulphurous and organic acids. Addition of manganese increases hot
workability of these steels.
Steels having 15 to 20% Ni and about 0.1 % carbon possesses great strength and toughness
and extremely good resistance to corrosion. Such steels are called stainless steels. Another type
of stainless steel containing 11 to 14% chromium and about 0.35% carbon is used for cutlery,
surgical and dental instruments and other purposes where hard edges are required. Maximum
resistance to corrosion is obtained when this steel is ground and polished after heat-treating.
70 Introduction to Basic Manufacturing Processes and Workshop Technology
A steel containing 18% chromium and 8% nickel is widely used and is commonly referred
to as 18/8 steel. Stainless steel is highly resistance to corrosion and oxidation. It can be classified
into three major categories according to the type of micro structures.
General Properties of Stainless Steels
It possesses wide range of strength and hardness, high ductility, formability, high corrosion
resistance, good creep resistance, good thermal conductivity, good machinability, good
weldability, high hot, cold workability, high resistance to scaling and oxidation at elevated
temperatures, excellent surface appearance and finish.
Classification of Stainless Steel
On basis of their structure, stainless steels are classified as follow:
1. Martensitic stainless steels
2. Ferritic stainless steels
3. Austenitic stainless steels.
These types of stainless steel are discussed as under.
Martensitic Stainless Steels
These steels contain 12 to 16% chromium and 0.1 to 1.2 per cent carbon. The structure
consists of hard martensite phase after hardening. The general utility chromium stainless
steel with 12% chromium and 0.15% carbon are ferromagnetic and air hardening. It is very
hard and possesses high strain and high corrosion resistance properties.
Stainless steels containing 12 to 14% chromium and 0.3% carbon are extensively used
for table cutlery, tools and equipments etc. Stainless steels containing 16-18% chromium and
0.2% carbon are used as springs, ball bearing, valves, knife blades and instruments under
high temperature and corrosive conditions. These steels are generally used for making utensils,
surgical and dental instruments, and springs of high temperature operations, ball valves and
Ferritic Stainless Steels
Ferritic stainless steels are non hardenable and contain 16 to 30% chromium and 0.08
to 0.2 per cent carbon. Structure of these steel consists of ferrite phase which cannot be
hardened by heat treatment. They have very low carbon and possess considerable ductility,
ability to be worked hot or cold, excellent corrosion resistance and are relatively in expensive.
They are always magnetic and retain their basic microstructure up to the melting point.
These are extensively used for kitchen equipment, diary machinery interior decorative
work, automobile trimmings, chemical engineering industry, stainless steel sinks, food
containers, refrigerator parts, beer barrels, automobile trimming etc. These are also used as
high temperature furnace parts when chromium content is high.
Austenitic Stainless Steel
Addition of substantial quantities of Ni to high Cr alloys gives rise to, austenitic steel.
It has good resistance to many acids (even hot or cold nitric acid). Slight amount of W and
Mo are added in such steels to increase its strength at elevated temperatures. This steel
Ferrous Materials 71
contains 16 to 24% Cr, 8 to 22% Ni and less than 0.2% C. Addition of nickel stabilizes
austenite, and hence the structure of these steels consists of austenite at room temperature.
A steel containing 18% Cr and 8% Ni is very widely used and is commonly referred to as 18/
8 stainless steel. These steels do not harden by heat treatment but can be rolled hard. These
steels possess a brilliant luster when polished. These are highly resistant to many acids even
nitric acids. The heat conductivity of steel is low, about 5% that of copper. Tungsten and
molybdenum are added to increase the strength at elevated temperatures, silicon and aluminium
to improve the resistance to scaling and selenium and sulphur are added to improve
machinability. This steel is easily weldable. After welding, it is susceptible to corrosive attack
in the area adjacent to the weld.
It is used for making heat exchangers, conveyors chains, furnaces, spokes, brewery, dairy
and chemical industrial components, cutlery parts, surgical and dental instruments, household
appliances such as kitchen utensils, sinks and saucepans. These are also used in making
components in power stations, especially in nuclear power stations, steam pipes, boiler tubes,
radiator and super heater tubes.
188.8.131.52 High speed steels
High Speed Steels (HSS) have been given this name due to the fact that these steels may
be operated as cutting tools at much higher speeds that are possible with plain carbon tool
steel. High speed steels cutting tools operate at cutting speed 2 to 3 times higher than for
High carbon steels. At higher cutting speeds, sufficient heat may be developed during the
cutting process. This heat causes the cutting edge of the tool to reach a high heat (red heat).
This heat softens the carbon tool steel and thus the tool will not work efficiently for a longer
period. These steels have the property of retaining their hardness even when heated to red
heat. High hardness at elevated temperatures is developed by addition of elements such as
tungsten, chromium vanadium to high carbon steels. These steel are generally used for
making lathe cutting tools, planner cutting tools, shaper cutting tools, slotting cutting tools,
drills, reamers, broaches, milling cutter and punches. There are four general types of high
speed steels used in machine shop.
1. High speed steel (18:4:1)
High speed steels (HSS) are most commonly operated as cutting tools at much higher
speed i.e. twice or thrice where as tool steel. It is the most common kind of cutting tool. It
contains 18% tungsten, 4% chromium and 1 % vanadium, 0.8 carbon and remaining iron. It
is considered to be one of the best of all purpose tool steels. This brand of high speed steel
is used for machining operations on steel and non-ferrous materials. This is generally used
for lathe, planer and shaper tools, drills, millings cutters, punches etc.
2. Molybdenum based high speed steel
It contains 6% Mo, 6% W, 4% Cr, 2% V, 0.8% C and remaining Fe. It has excellent
toughness and cutting ability. Molybdenum high speed steels are cheaper than other types of
steels and are particularly used for drilling and tapping tools. These steels are also used for
making rough cutting tools, lathe tools and various kinds of milling cutters.
3. Cobalt based high speed steel
It contains 1 to 12% Co, 20% W, 4% Cr, 2% V, 0.8 carbon and remaining iron. This is
also known as super high speed steel, because cutting tool made of this steel can be operated
72 Introduction to Basic Manufacturing Processes and Workshop Technology
at much higher speeds in comparison to high speed steel of 18:4:1 kind. In this steel, cobalt
is added from 2 to 15 per cent in order to increase the cutting efficiency especially at high
temperature. Cobalt high speed steel generally contains 20% W, 4% Cr, 2% V and 12% Co and
remaining Fe. Since the cost of this steel is more, therefore, it is principally used for making
cutting tools for heavy operations which impose high pressure and temperature on the tool.
It is extensively used for making high production tools of heavy work for high production
lathe, planer, shaper, milling and boring machine.
4. Vanadium High Speed Steel
Generally, this steel contains more than 1% V and 0.70% C. This steel possesses better
abrasive resistance in comparison to normal HSS type steel. It is preferred for machining
materials which are highly difficult to machine by conventional means. These steels cutting
tools are close competitors of carbides cutting tools such as drills, reamers, milling cutters
etc. In addition to having heat resistance properties of high speed steels possesses desirable
properties of high hardness, high compressive strength and outstanding wear resistance.
184.108.40.206 Availability of steel in market
Steel are available in market in various rolled forms like sheets, plates, strips, rods,
beams, channels, angles, tees etc. The common structural shapes for market form of supply
are reflected in Fig. 4.5. Steels are generally identified, coded and designated according to
suitable standards by a group of symbols indicating the important characteristics.
Flange Flange Flange
D D D
L L L
Channel T-Section T-Section
Fig. 4.5 Market forms of steel structure shapes
220.127.116.11 Designation of steels
Bureau of Indian Standards (BIS) designates the various grades of steels by a system of
codification which bears direct relationship with the important characteristics of steel such as
Ferrous Materials 73
tensile strength, chemical composition. physical and surface conditions. According to this
method a particular grade designation would be applicable to certain steel only. Hence steel
may be designated by a group of symbols indicating the important characteristics.
(i) 1025. Indicates C-25 which is plain carbon steel,
(ii) 1112. It is a free cutting steel having percentage
C = 0.13 Max.
Mn = 0.7 – 1.0 %
P = 0.07 – 0.12 %
S = 0.16 – 0.23%
(iii) 4145. It is Cr-Mo – steel having percentage
C = 0.33 – 0.38%
Mn = 0.7 – 0.9%
P or S = 3.025%
Si = 0.2 – 0.35%
Cr = 0.81 – 1.1 %
Mo = 0.18 – 0.25%
(iv) 8650. It is Ni-Cr-Mo alloy steel having percentages
Ni = 0.4 – 0.7%
Cr = 0.4 – 0.6%
Mo = 0.15 – 0.25%
(v) 3145. It is a Ni-Cr steel having
Ni = 0.3 – 0.35%
Cr = 0.4 – 0.5%
(vi) 2330. It is a Ni-steel having percentages
C = 0.28 – 0.33%
S = 0.04%
Mn = 0.5%
Si = 0.02 – 0.35 %
Ni = 3.25 – 3.75%
(vii) 5150 It is a Cr-Steel
Following symbol recommended to be used to indicate heat treatment given to steel and
is to be suffixed at the end of normal symbol of steel.
(1) Annealed and softened a
(2) Case carburized c
(3) Hard, drawn, cold reduced d
(4) Hot rolled h
(5) Normalized n
(6) Spherodised 0
74 Introduction to Basic Manufacturing Processes and Workshop Technology
(7) Patented p
(8) Hardened and Tempered q
(9) Stress relieved s
(10) Tempered t
Following symbols should be recommended to be suffixed with the normal steel symbol
to indicate the steel quality
(1) Non-ageing quality A
(2) Stabilizing against stress corrosion and inter-annular attack E
(3) Control cooled ensure freedom from flakes L
(4) Fully-killed (deoxidized) D
(5) Semi-killed D2
(6) Rimming quality R
(7) Grain size controlled G
(8) Hardenability controlled H
(9) Inclusion controlled I
(10) Structural homogeneity guaranteed by macro- structure test M
Carbon Tool Steel (Annealed)
Carbon tool steel in annealed condition is explained as below with designation and uses.
C-60 Spindles for machine tools, coupling, crank shaft axles and pinions.
C-65 Small washers and thin stamped parts.
C- 70 Buffer spring shock absorbers.
C- 75 Light flat, springs formed from annealed stock.
C-75-C-85 Flat and coils springs for automobiles and railway vehicles.
C-50 to C-113 Springs made from small flat section.
Plain Carbon Structural Steel
Designation and Uses
St-42 For bridge and building construction, railway rolling stock, screw
spikes and oil well castings.
St-44 Pressure vessels, fasteners, value fittings for compressed gas cylinders
and railway rolling stock.
St-47 For railway rolling stock, pressure parts of marine and land boilers
and rivets for air receivers.
St-50 For mines, forgings of marine and engine parts.
St-52-54 For railway wheels, electric tramways cars.
Ferrous Materials 75
1. How are engineering materials classified?
2. How ferrous metals differ from non-ferrous metals?
3. State the name of important iron ores.
4. How cast iron differs from steel?
5. Write short notes on :
(i) Pig iron
(ii) Grey cast iron
(iii) White cast iron
(iv) Ductile cast iron
(v) Malleable cast iron.
6. Discuss in brief the effect of impurities in cast iron.
7. What is wrought iron? Discuss in brief its chemical composition, properties and applications.
8. What are plain carbon steels? Discuss in brief the classification of plain carbon steels and
also state few applications of different plain carbon steels.
9. What are alloy steels? Discuss in brief the effects of alloying elements on steel.
10. How are alloy steels classified?
11. Write short notes on:
(i) Stainless steel
(ii) High speed steel
(iii) Designation of steels.
Non-Ferrous Materials 77
impurities are oxide, silica, clay and titanium oxide. It is found in India in the states of Bihar
and Madhya Pradesh.
The bauxite is purified and then dissolved in fused cryolite (double fluoride of aluminium
and sodium). The aluminium is then separated from this solution by electrolysis at about
Pure aluminium has silvery color and lusture. It is ductile, malleable and very good
conductor of heat and electricity. It has a very high resistance to corrosion than the ordinary
steel. Its specific gravity is 2.7 and melting point is 658°C. Its tensile strength varies from
95 to 157 MN/m2. In proportion to its weight it is quite strong. In its pure state the metal
would be weak and soft for most purposes, but when mixed with small amounts of other
alloys, it becomes hard and rigid. It may be blanked, formed, drawn, turned, cast, forged and
die cast. Its good electrical conductivity is an important property and is broadly used for
overhead cables. It forms useful alloys with iron, copper, zinc and other metals.
It is mainly used in aircraft and automobile parts where saving of weight is an advantage.
The high resistance to corrosion and its non-toxicity make it a useful metal for cooking
utensils under ordinary conditions. Aluminium metal of high purity has got high reflecting
power in the form of sheets and is, therefore, widely used for reflectors, mirrors and telescopes.
It is used in making furniture, doors and window components, rail road, trolley cars, automobile
bodies and pistons, electrical cables, rivets, kitchen utensils and collapsible tubes for pastes.
Aluminium foil is used as silver paper for food packing etc. In a finely divided flake form,
aluminium is employed as a pigment in paint. It is a cheap and very important non ferrous
metal used for making cooking utensils.
5.2.1 Aluminium alloys
The aluminium may be easily alloyed with other elements like copper, magnesium, zinc,
manganese, silicon and nickel to improve various properties. The addition of small quantities
of alloying elements into other metals helps to converts the soft and weak metal into hard
and strong metal, while still retaining its light weight. Various aluminium alloys are
3. Magnalium and
These alloys are discussed as below:
It is an important wrought alloy. Its composition contains following chemical contents.
Copper = 3.5-4.5%
Manganese = 0.4-0.7%
Magnesium = 0.4-0.7%
Aluminium = 94%
78 Introduction to Basic Manufacturing Processes and Workshop Technology
Duralumin can be very easily forged, casted and worked because it possesses low melting
point. It has high tensile strength, comparable with mild steel combined with the characteristics
lightness of Al. It however possesses low corrosion resistance and high electrical conductivity.
This alloy possesses higher strength after heat treatment and age hardening. After working,
if this alloy is age hardened for 3 or 4 days. This phenomenon is known as age hardening.
It hardens spontaneously when exposed to room temperature. This alloy is soft enough for
a workable period after it has been quenched. It is light in weight as compared to its strength
in comparison to other metals. It can be easily hot worked at a temperature of 500°C.
However after forging and annealing, it can also be cold worked.
Duralumin is used in the wrought conditions for forging, stamping, bars, sheets, tubes,
bolts, and rivets. Due to its higher strength and lighter weight, this alloy is widely used in
automobile and aircraft components. To improve the strength of duralumin sheet, a thin film
of Al is rolled along with this sheet. Such combined sheets are widely used in air-craft
industries. It is also employed in surgical and orthopedic work, non-magnetic work and
measuring instrument parts constructing work.
5.2.3 Y -alloy
Y-Alloy is also called copper-aluminium alloy. The addition of copper to pure aluminium
increases its strength and machinability. Its composition contains following chemical contents.
Copper = 3.5-4.5%
Manganese = 1.2-1.7%
Nickel = 1.8-2.3%
Silicon, magnesium, iron = 0.6% each
Aluminium = 92.5%.
The addition of copper in aluminium increases its strength and machinability. Y-alloy can
be easily cast and hot worked. Like duralumin, this alloy is heat treated and age hardened.
The age-hardening process of Y-alloy is carried out at room temperature for about five days.
Y-Alloy is mainly used for cast purposes, but it can also be used for forged components
like duralumin. Since Y -alloy has better strength than duralumin at high temperatures,
therefore it is much used in aircraft engines for cylinder heads, pistons, cylinder heads, crank
cases of internal combustion engines die casting, pump rods etc.
Magnalium is an alloy of aluminium, magnesium, copper, nickel and tin etc. It contains
Al = 85 to 95%, Cu = 0 to 25%, Mg = 1 to 5%,
Ni = 0 to 1.2%, Sn = 0 to 3%, Fe = 0 to 0.9%,
Mn = 0 to 0.03%, Si = 0.2 to 0.6%.
Non-Ferrous Materials 79
It is made by melting the aluminium with 2-10% magnesium in a vacuum and then
cooling it in a vacuum or under a pressure of 100 to 200 atmospheres.
Magnalium is light in weight and brittle. This alloy possesses poor castability and good
machinability. It can be easily welded.
Due to its light weight and good mechanical properties, it is mainly used for making
aircraft and automobile components.
Hindalium is a common trade name of aluminium alloy. It is an alloy of aluminium, magnesium,
manganese, chromium and silicon etc. In India, it is produced by Hindustan Aluminium
Corporation Ltd., Renukoot (U.P.). Hindalium is commonly produced as a rolled product in 16
gauges. Utensils manufactured by this alloys are strong and hard, easily cleaned, low cost
than stainless steels, having fine finish, having good scratch resistance, do not absorb much
Hindalium is mainly used for manufacturing anodized utensil. Utensils manufactured by
this alloys are strong and hard, easily cleaned, low cost than stainless steels, having fine
finish, having good scratch resistance, do not absorb much heat etc.
Copper is one of the most widely used non-ferrous metals in industry. It is extracted from ores
of copper such as copper glance, copper pyrites, melachite and azurite. Copper ores are found
in the state of Sikkim and Bihar of India and Bharma.
Copper ore is first ground and then smelted in a reverberatory or small blast furnace for
producing an impure alloy. Then the air is blown through the molten metal to remove
sulphur and iron contamination to obtain blister copper in the converter. Copper is then
refined further using electrolysis processes.
Pure copper is soft, malleable and ductile metal with a reddish-brown appearance. It is
a good conductor of electricity. It is non-corrosive under ordinary conditions and resists
weather very effectively. Its tensile strength varies from 300 to 470 MN/m2 and melting point
is 1084°C. It is one of the best conductors of heat and it is highly resistant to corrosion. This
non ferrous metal can withstand severe bending and forging without failure. It does not cast
well. If copper is heated to red heat and cooled slowly it becomes brittle, but if cooled rapidly
it becomes soft, malleable and ductile. It can be welded at red heat.
Copper is mainly used in making electric cables and wires for electric machinery, motor
winding, electric conducting appliances, and electroplating etc. It can be easily forged, casted,
rolled and drawn into wires. Copper in the form of tubes is used widely in heat transfer work
80 Introduction to Basic Manufacturing Processes and Workshop Technology
mechanical engineering field. It is used for household utensils. It is also used in production
of boilers, condensers, roofing etc. It is used for making useful alloys with tin, zinc, nickel
and aluminium. It is used to form alloys like brass, bronze and gun metal. Alloys of copper
are made by alloying it with zinc, tin, and lead and these find wide range of applications.
Brass, which is an alloy of copper and zinc, finds applications in utensils, household fittings,
decorative objects, etc. Bronze is an alloy of copper and tin and possesses very good corrosion
resistance. It is used in making valves and bearings. Brass and bronze can be machined at
high speeds to fine surface finish.
The following copper alloys are important
1. Copper-zinc alloys (Brasses)
2. Copper-tin alloys (Bronzes)
Brasses are widely used alloy of copper (main constituent) and zinc. They also contain small
amounts of lead or tin or aluminium. The most commonly used copper-zinc alloy is brass.
There are various types of brasses, depending upon the proportion of copper and zinc. The
fundamental a binary alloy comprises 50% copper and 50% zinc. By adding small quantities
of other elements, properties of brass may be greatly changed. For example addition of lead
(1 to 2%) improves the machining quality of brass. It has a greater-strength than that of
copper, but has a lower thermal and electrical conductivity. Brasses alloys are very resistant
to atmospheric corrosion and can be easily soldered. They can be easily fabricated by processes
like spinning and can also be electroplated with metals like nickel and chromium. Some of
common phases of brass are discussed as under.
If the copper crystal structure is face centered cubic (FCC), there will be up to 36% of
zinc. This solid solution is known as alpha brass. It has good mechanical properties, good
corrosion resistance but it possesses lower electrical conductivity than copper.
If the amount of zinc increases beyond 36%, beta brass will appear in the microstructure
of the slowly cooled brass. This has body centered cubic structure (BCC). This phase is hard
but quite tough at room temperature.
When zinc content is increased in brass beyond 45%, then gamma phase is appeared in
its structure. This structure is extremely brittle, rendering an alloy which makes it unsuitable
for general engineering purposes. The various types of brasses are discussed as under.
18.104.22.168 Red Brass
Red brass is an important material used for heat conducting purposes. Itcontains
Cu = 85%
Zn = 15%.
Red brass is having excellent corrosion resistance and workability. It possesses tensile
strength ranging from 27-31 kg/mm 2. Percentage elongation of this brass is 42-48.
Non-Ferrous Materials 81
Red brass is mainly utilized for making, heat exchanger tubes, condenser, radiator cores,
plumbing pipes, sockets, hardware, etc.
22.214.171.124 Yellow Brass or Muntz Metal
Yellow brass is also known as muntz metal. It contains
Cu = 60%
Zn = 40%
Muntz metal is having high strength and high hot workability. It is having tensile
strength 38 Kg/mm2 (approximately). The percentage elongation of this brass is 45%.
Yellow brass or muntz metal is suitable for hot working by rolling, extrusion and stamping.
It is utilized for making small various components of machine and electrical equipment such
as bolts, rods, tubes, valves and fuses. This metal is utilized for making for pump parts, valves,
taps, condenser tubes, sheet form for ship sheathing (because of excellent corrosion resistance).
126.96.36.199 Cartridge Brass
It contains 70% Cu and 30% Zn. It is having good combination of strength and ductility.
It is having tensile strength between 31-37 kg/mm2. Percentage elongation of this brass is
55-66%. It is generally processed into rolled sheets. The metal alloy can be easily cold worked
using cold working processes such as wire drawing, deep drawing and pressing.
It is utilized for making for making tubes, automotive radiator cores, hardware fasteners,
rivets, springs, plumber accessories and in tube manufacture.
188.8.131.52 Admiralty Brass
Cu = 71%
Zn = 29%
Sn = 1%
1. Admiralty brass is highly resistant to corrosion.
2. It is highly resistant to impingement attack of sea water.
3. It is having tensile strength 30 kg/mm2 (approx.).
4. It can be cold worked
5. It possesses good corrosion resistance to sea water corrosion.
6. The percentage elongation of admiralty brass is 65%.
Admiralty brass is utilized for making condenser tubes in marine and other installations.
It is used for making plates used for ship building. It is utilized also for making bolts, nuts,
washers, condenser plant and ship fittings parts, etc.
82 Introduction to Basic Manufacturing Processes and Workshop Technology
184.108.40.206 Naval Brass
Navel brass is commonly used for making marine components. It contains
Cu = 59%
Zn = 40%
Sn = 1%
Properties of naval brass are similar to muntz metal. As 1% zinc is replaced by 1% tin
in Muntz metal to make navel brass, corrosion resistance of this material to sea water is
significantly improved. The percentage elongation of navel brass is 47% and its tensile strength
is 38 kg/mm2 (approx.).
Navel brass is commonly utilized for making marine hardware casting, piston rods,
propeller shafts, welding rods etc.
220.127.116.11 Manganese Brass
Manganese brass is sometimes also called manganese bronze. It contains
Cu = 60%
Zn = 38%
Mn = 0.5%
Fe = 1.0%
Sn = 0.5%
Manganese brass possesses sufficient toughness and good corrosion resistance. It is very
active in reducing the oxides of other metals.
Manganese brass is utilized for making hydraulic rams, valves and cylinders, tubes,
pump rods, propellers, bolts, nuts etc.
18.104.22.168 Iron Brass or Delta Metal
Iron brass or delta brass contains
Cu = 60%
Zn = 37%
Fe = 3%
Iron brass or delta metal is hard, strong, tough, and having good corrosion resistance.
It can be casted easily.
If corrosion is to be resisted in mild steel, then some amount of iron brass or delta metal
is added in mild steel.
Non-Ferrous Materials 83
22.214.171.124 Gilding Brass
Gilding brass is a very cheap metal for making jewellery, decorative and ornamental
products. It generally contains
Cu = 85%
Zn = 15%
Because of better appearance this metal is commonly used for jewellery, decorative and
126.96.36.199 Free Cutting Brass
Free cutting brass contains
Cu = 57.5%
Zn = 40%
Pb = 2.5%
Free cutting brass is highly machinable and it does not allow bending.
Free cutting brass is used for making cast, forged or stamped blanks to be used for
further machining such as high speed turning and screwing.
188.8.131.52 Lead Brass
Lead brass is also known as cloak brass which contains
Cu = 65%
Zn = 34%
Pb = 1%
Lead brass or cloak brass is used in making small gears and pinions for clock work.
Bronze is a common alloy of copper and tin. The alloys of copper and tin are generally termed
as bronzes. The wide range of composition of these alloys comprise of 75 to 95% copper and
5 to 25% tin.
Properties of bronzes
Bronze has higher strength, better corrosion resistance than brasses. It is comparatively
hard and resists surface wear and can be shaped or rolled into wire, rods and sheets very
easily. It has antifriction or bearing properties. Bronze is costlier than brass. The tensile
strength of bronze increases gradually with the amount of tin, reaching a maximum when tin
is about 20%. However the percentage of tin content if increases beyond this amount, the
tensile strength decreases very rapidly. Bronze is most ductile when it contains about 5% of
tin. As the amount of tin increases about 5%, the ductility gradually decreases and practically
disappears with about 20% of tin. Whereas presence of zinc in the bronze increases fluidity
of molten metal, strength and ductility.
Some of the common types of bronzes are discussed as under:
84 Introduction to Basic Manufacturing Processes and Workshop Technology
184.108.40.206 Phosphor Bronze
When bronze contains phosphorus in very small amount, then phosphor bronze is produced.
A common type of phosphor bronze has the following composition.
Cu = 89 to 94%
Sn = 6 to 10%
P = 0.1 to 0.3%
Tensile strength, ductility, elasticity, soundness of castings, good wearing quality and
resistance to fatigue of phosphor bronze increases with increase of phosphorus in bronze. This
material possesses good corrosion resistance especially for sea water, so that it is much used
for propeller blades. Phosphor bronze of proper composition can be easily casted, forged,
drawn, and cold rolled.
Phosphorus bronze is used making for bolts, electric contact springs, bearings, bushes,
gears, ship sheathing, valve parts, propeller blades, worm wheels, gears, nuts for machine
lead screws, pump parts, linings and for many other purposes. It is also suitable for making
springs and corrosion resistance mine cables.
220.127.116.11 Silicon bronze
Silicon bronze contains
Cu = 96%
Si = 3%
Mn or Zn = 1%
Silicon bronze has good general corrosion resistance of copper combined with higher
strength. It can be cast, rolled, stamped, forged and pressed either hot or cold and it can be
welded by all the usual methods.
Silicon bronze is widely used for making boilers, tanks, stoves or where high strength and
good corrosion resistance is required. It is used also for making screws, tubing’s, pumps etc.
18.104.22.168 Beryllium bronze
Beryllium bronze is a copper base alloy contains
Cu = 97.5%
Br = 2.5%
Beryllium bronze possesses higher tensile strength than other bronzes. It possesses
excellent corrosion resistance. It is having high yield point and high fatigue limit. It is having
good hot and cold resistance. This can be heat treated by precipitation hardening. It possesses
excellent formability in soft condition, and high fatigue and creep resistance in hardened
condition. However it involves high cost.
Beryllium bronze is particularly suitable material for making springs, tubes, diaphragms
and electrical contacts, heavy duty electrical switches, cams and bushings. This is used for
Non-Ferrous Materials 85
springs, heavy duty electrical switches, cams and bushings. Having non-sparking characteristics,
it is used for making chisels and hammers using for such conditions where spark might cause
explosion. It has a film forming and a soft lubricating property, which makes it more suitable
as a bearing metal. Since the wear resistance of beryllium copper is five times that of
phosphorous bronze, therefore it is used as a bearing metal in place of phosphor bronze.
22.214.171.124 Manganese bronze
Manganese bronze is an alloy of copper, zinc and little percentage of manganese. The
usual composition of this bronze is
Copper = 60%
Zinc = 35%
Manganese = 5%
Manganese bronze is highly resistant to corrosion. It is stronger and harder than phosphor
Manganese bronze is mainly used for bushes, plungers, feed pumps, rods etc. Worm
gears are frequently made from this bronze.
126.96.36.199 Aluminium Bronze
Aluminium bronze possesses
Cu = 85 to 88%
Al = 8 to 11%
Fe = 3%
Sn = 0.5%
The aluminium bronze with 8% aluminium possesses very good cold working properties.
When iron is added to this metal, its mechanical properties are greatly improved by refining
the grain size and improving the ductility. The maximum tensile strength of this alloy is 450
MPa with 11 % aluminium. This material possesses good resistance to corrosion and it is
somewhat difficult to cast due to oxidation problem.
Aluminium bronze is generally used for making fluid connection fittings, gears, propellers,
air pumps, bushings, tubes, slide and valves etc. Cams and rollers are commonly produced
using this alloy.
188.8.131.52 Bell Metal
Bell metal generally contains
Cu = 66.7%
Sn = 33.3%
Bell metal is very strong. It possesses resistance to corrosion water and atmosphere. It
is used to make bells.
86 Introduction to Basic Manufacturing Processes and Workshop Technology
The composition of constantan is
Cu = 55%
Ni = 45%
(i) Constantan is high specific resistance
(ii) Specific resistance is unaffected by temperature variation.
Constantan is used for accurate resistors like thermo-couples,
(i) Wheet-stone bridge,
(ii) Low temperature heaters and
5.4 NICKELAND ITSALLOY
Nickel and its alloys are discussed as under.
Nickel is a silvery shining white metal having extremely good response to polish. The most
important nickel’s ore is iron sulphides which contain about 3% of nickel. About 90% of the
total production of nickel is obtained by this source. This ore is mainly found in Canada and
The ore of Nickel is initially roasted to reduce the sulphur content and then smelted to
separate the gangue from it. Matte (impure product of the smelting of sulphide ore especially
those of nickel or copper, is known as matte) delivered by the smelting furnace is then put
in a Bessemer converter to oxidize the iron. The iron oxide thus combines with a limestone
and quartz and form the slag. The Bessemer’s matte consists chiefly of copper and nickel
Nickel is as hard as steel. It possesses good heat resistance. It is tough and having good
corrosion resistance. Its melting point is 1452°C and specific gravity is 0.85. At normal
temperature, nickel is paramagnetic. Nickel alloys are sometimes used for their high potential
field strengths, some for their permeability and some for their high coercive force. When it
contains small amount of carbon, it is quite malleable. It is somewhat less ductile than soft
steel, but small amount of magnesium improves ductility considerably.
Nickel is used in kitchen utensils and appliances, and in laundry and dairy machinery.
It is extensively useful for electroplating plating work for protecting surfaces of iron and brass
from corrosion. It is also utilized as an important alloying element in some type of cast iron
and steel. It is helpful for making stainless steel. Its alloys are discussed as under.
Non-Ferrous Materials 87
5.4.2 Nickel Alloys
The important nickel alloys are haste alloy, Monel metal, inconel, nomonic and ni-chrome.
184.108.40.206 Haste Alloy or high Temprature Alloy
Haste alloy or high temperature alloy is mainly a nickel base alloy. It contains
Ni = 45%,
Cr = 22%,
Mo = 9%,
Co = 1.5%,
W = 0.5%,
C = 0.15% and
Fe = Remaining
(i) It can be hot and easily cold worked, casted and welded.
(ii) It has high resistance corrosion especially to acids and salts except nitric acid
(iii) It can be machined also.
(iv) This alloy is used where the resistance to corrosion is of consideration.
The high temperature alloys are those alloys which can withstand high temperatures
about 1100°C. These alloys are used in components of nuclear plants, jet and rocket
220.127.116.11 Monel Metal
Monel metal is an important alloy of nickel and copper. It contains 68% Ni, 30% Cu, 1%
Fe and small amount of other constituents like iron, manganese, silicon and carbon.
Monel metal is superior to brass or bronze in resisting corrosion and in retaining its
strength at high temperature. It is magnetic at ordinary temperatures. Its mechanical properties
are improved by cold working. It can be cast, cold and hot worked, forged and welded. It
resembles nickel in appearance and is strong, ductile and tough. It has good mechanical
properties and can retain them even at elevated temperatures. It has high excellent corrosion
Monel metal is also used for pump fittings, condenser tubes, sea water exposed parts etc.
It is widely used for making turbine blades, containers, parts for chemical plants, food handling
machinery parts, marine parts, pump impellers, propellers, evaporators and heat exchangers
in chemical works.
88 Introduction to Basic Manufacturing Processes and Workshop Technology
Ni = 80%
Cr = 14%
Fe = 6%
Inconel has high resistance to corrosion and oxidation at elevated temperatures. It can be
readily cold-worked and hot-worked, but does not respond to heat treatment. It contains high
mechanical properties coupled corrosion and heat resisting properties. It can be cast, forged,
rolled and cold drawn. Its specific gravity is 8.55 and melting point is 1395°C. Its Brinell
Hardness is about 160BHN. It can be soft soldered or can be welded by oxyacetylene welding.
Inconel is used for making springs, exhaust manifold of aircraft engines, machinery for
food processing industries, especially milk and milk products. It is widely used for processing
uranium and for sheathing for high temperature heating elements.
18.104.22.168 Nomonic alloy
The composition of nomonic alloy is given as under.
Cr = 15 to 18%
Co = 15 to 18%
Ti = l.2 to 4.0%
Al = l.5%
Ni = Remaining
(i) Nomonic is a special type of nickel alloy having good strength
(ii) It can be easily heat treated to attain excellent properties for very high temperature
Nomonic is widely used for making gas turbine engines
Ni = 60%
Cr = 15%
Fe = 20%
Ni-chrome is non-corrosive. It can easily withstand high temperatures without oxidation.
Ni-chrome is commonly used for making electrical resistance wire for electric furnaces
and heating elements.
Non-Ferrous Materials 89
Lead is a bluish grey metal with a high metallic lusture when freshly cut. It is a very durable
and versatile material. The heavy metal obtained from the bottom of the furnace is further
oxidized in Bessemer’s converter to remove most of the impurities.
Lead has properties of high density and easy workability. It has very good resistance to
corrosion and many acids have no chemical action on it. Its melting point is 327°C and specific
gravity is 11.35. It is the softest and heaviest of all the common metals. It is very malleable
and may be readily formed into foil. It can readily be scratched with fingernail when pure.
The lead pipes installed by the Romans in the public baths in Bath, England, nearly 2000
years ago are still in use. Lead is used in safety plug in boilers, fire door releases and fuses.
It is also used in various alloys such as brass and bronze. It finds extensive applications as
sheaths for electric cables, both overhead and underground. Its sheets are used for making
roofs, gutters etc. It is employed for chemical laboratory and plant drains. In the soldering
process, an alloy of lead and tin is most widely utilized as a solder material for joining metals
in joining processes.
Zinc is bluish grey in color and is obtained from common ores of zinc are zinc blende (ZnS),
zincite (ZnO), calamine (ZnCO3). These ores are commonly available in Burma. The oxide is
heated in an electric furnace where the zinc is liberated as vapor. The vapors are then cooled
in condensers to get metallic zinc.
Zinc possesses specific gravity is 6.2 and low melting point of 480°C. Its tensile strength
is 19 to 25 MPa. It becomes brittle at 200°C and can be powdered at this temperature. It
possesses high resistance to corrosion. It can be readily worked and rolled into thin sheets
or drawn into wires by heating it to 100-150°C.
With regards to industrial applications, zinc is the fourth most utilized metal after iron,
aluminium, and copper. Zinc is commonly used as a protective coating on iron and steel in
the form of a galvanized or sprayed surface. It is used for generating electric cells and making
brass and other alloys. The oxide of zinc is used as pigment in paints. Parts manufactured
by zinc alloys include carburetors, fuel pumps, automobile parts, and so on.
Tin is recognized as brightly shining white metal. It does not corrode in wet and dry conditions.
Therefore, it is commonly used as a protective coating material for iron and steel. The main
source of tin is tinstone. Large deposits of tinstone occur in Tairy (Burma) and small quantities
in Hazaribagh in Bihar of India
To obtain crude tin, the ores of tins are crushed, calcined, washed and then smelted in
a furnace using anthracite coal and sand. The crude tin is then refined in a reverberatory
90 Introduction to Basic Manufacturing Processes and Workshop Technology
furnace to get commercially pure tin. Chemically pure tin is made by electrolytic deposition
from commercial tin.
Tin is considered as a soft and ductile material. It possesses very good malleability. Its
melting point is 232°C and specific gravity is 7.3. It is malleable and hence can be hammered
into thin foils
Tin-base white metals are commonly used to make bearings that are subjected to high
pressure and load. Tin is used as coating on other metals and alloys owing to its resistance
to corrosion. It is employed in low melting point alloys as a substitute for Bismuth. It is
generally preferred as moisture proof packing material. Because of its high malleability, it
finds application in tin cans for storing food and food items.
5.7.1 Tin Base Alloy
Tin base alloy is also known as Babbitt metal which contains
Sn = 88%
Sb = 8%
Cu = 4%
Babbit metal possesses excellent antifriction properties and sufficient mechanical strength.
It can be easily casted. It is expensive because of high tin content.
Because of the above properties, Babbit metal is the most common bearing metal used
with cast iron boxes where the bearings are subjected to high pressure and load applications.
5.8. BEARING OR ANTIFRICTION ALLOYS
A bearing alloy or antifriction alloy commonly possesses good wearing quality, low co-efficient
of friction, high thermal conductivity, good casting qualities, non-corrosive properties, ability
to withstand high pressure and impact, low shrinkage after coating and less cost. Various
Bearing Metals are:
5.8.1 Admiralty Gun Metal
The composition of admiralty gun metal generally contains
Cu = 88%
Sn = 10%
Pb = 2%
Admiralty gun metal is having tensile strength of the order of 270 MN/m2. It possesses
elongation of about 20% and Brinell Hardness of 65 BHN.
Non-Ferrous Materials 91
Admiralty gun metal is generally utilized where lubrication is needed and oiling is
5.8.2 Lead Bronze
Lead bronze generally contains
Cu = 80%
Sn = 10%
Pb = 10%
Lead bronze possesses tensile strength of 230 MN/m2 , Brinell Hardness of 65 BHN and
elongation of about 15%.
Lead bronze possesses has antifriction properties and hence is generally utilized where
lubrication is doubtful.
5.8.3 Hard Bearing Bronze
Hard bearing bronze basically contains
Cu = 85%
Sn = 15%
Hard bearing bronze generally possesses tensile strength of 220 MN/m2, 100 BHN and
percentage elongation of 2%.
Hard bearing bronze is commonly used for high compressive loads such as locomotive
slide valves etc.
5.9 CUTTING TOOL MATERIAL
Few material for cutting tools are generally used which are as follows.
(i) High Speed Steel
These have superior hot hardness and it can retain the hardness up to 900°C. In
it tungsten produces martensite structure with other elements. It is three types
18-4-1 High Speed Steel.
It has 18% tungsten, 4% chromium, 1% vanadium and 0.7% carbon: This is used for
machining or metal cutting speed above 50 m/min. But for higher cutting speed
vanadium is increased.
Molybdenum high Speed Steel
It has 6% Molybdenum, 4% chromium and 2% vanadium.
92 Introduction to Basic Manufacturing Processes and Workshop Technology
Cobalt High Speed Steel
It is also known as super high speed steel. It has 1-12% cobalt, 20% tungsten, 4%
chromium and 2% vanadium. It is very good for high cutting speed.
(ii) Cemented Carbides
The use of tungsten as an alloying elements gives steel the properly of retaining
hardness at high temperature up to 900°C to 1000°C. Carbide is made by mixing
tungsten metal powder with carbon and heating the mixture to the about 1600°C in
the atmosphere of hydrogen until the two substance have under gone the chemical
reaction to produce tungsten carbides. Cemented carbide is a powder metallurgical
product. The powder of several carbide compounds are pressed and bonded together
in a matrix to from a cemented material. Today, the following three groups of
cemented carbides are extensively applied for cutting elements of tools.
(a) WC + Co + (WC-TiC-TaC-NiC) for use in the machining of steels.
(b) WC + Co for use in the machining of cast irons and non ferrous metals.
(c) TiC + Ni + Mo for use in the machining of high temperature high strength metals.
Cemented carbides have a very high hardness (second only to diamond) and high wear
resistance to abrasion. They do not loose their cutting properties i.e., hardness over
a wide range of temperature up to 900-1000°C. Therefore tools tipped with cemented
carbides are capable of efficiently machining the hardest metals, including hardened
steels at high cutting speeds. Such tools can operate at cutting speeds from 16 to 25
folds those permitted for tools made of carbon tool steels. One drawback of cemented
carbides is their brittleness. Very high stiffness (Young’s modulus is about three times
that of steel) of the cemented carbides requires that they are well supported on a
shank of sufficient thickness, for even a small amount of bonding deformation in a
material of this stiffness may induce very high tensile stresses. Cemented carbides
are weak in tension than in compression. They have a strong tendency to form
pressure welds at low cutting speeds. In view of this they should be operated at speeds
considerably in excess of those used with high speed steel tools. This caused for
machine tools of increased power. Carbides that obtain high cobalt percentage are
tougher and stronger than that contain low cobalt. Hence they are used for rough
cutting, interrupted cuts and for milling. The low cobalt variety is used for finished
operations such as turning with a smooth chip cross-section and a continuous cut. It
is recommended to keep the braze metal as thin as possible.
(iii) Ceramics Tool
The latest development in the metal cutting tools uses Aluminium oxide, generally
referred as ceramics. These tools are made by compacting Al2O3 powder in a mould
at about 280 kg/cm2 or more. The part is then sintered at 2200°C. This method is
also known cold pressing ceramic tool. Hot pressed ceramic tool materials are
expensive owing to their higher mould costs. These are made in form of tips that
are clamped to metal shanks. These tools have very low heat conductivity and
possess extremely high compressive strength. However they are quite brittle. The
have low bending strength. They can with stand temperatures up to 1200°C and can
be used at cutting speeds 10 times that of high speed cutting tools and 4 times that
of cemented carbides. They are chiefly used for single point cutting tools for semi-
finish and turning of cast iron, plastics and other work. Heat conductivity of ceramics
is very low and hence these tools are generally used without a coolant.
Non-Ferrous Materials 93
(iv) Carbides tool
It may be produced from carbides of tungsten, titanium and tantanum with same
percentage, of cobalt. The product is obtained by a special technique known as
powder metallurgy. Usually it contains 82% tungsten, 8% cobalt and l0% titanium
and the product is obtained by a special technique known as power metallurgy.
Cobalt acts as a binder and others are very hard substance. This tool contains high
degree of hardness and resistance. It is able to retain hardness at elevated
temperatures up to l000°C. It can be operated at speeds 5 to 6 times or (more)
higher than those with high speed steel.
It is a noble material which is so costly that its application becomes limited. It is
a hardest material. It can be used for cutting at a speed 50 times greater than
H.S.S. tools. It can retain its hardness even at a temperature of 1650. It has low
coefficient of friction and high heat conductivity. Diamond tools are used to produce
good surface finish.
5.10 COMPOSTION AND APPLICATIONS OF FEW TYPICAL MATERIALS
The composition and applications of few typical materials is given in Table 5.1.
Table 5.1 Composition and Applications of Few Typical Materials
S. No Alloy Composition Uses
1 Duralmin, 95% Aluminium + 4% Copper+ Light structures, extruded
0.5% Manganese + 0.5% Magnesium sections and sheet
2 Gun metal 90% copper + 10% zinc Small valves, fittings for
3 Monel 67% Ni + 28% Copper + remaining Valve parts for superheated
carbon, iron and Manganese steam turbine blades
4 Phosphor bronze 90% Copper + 9.7% Tin + 0.3% Bearings, worm wheels,
Phosphorus rods sheets
5 High carbon steel 0.8% to 1.5% Carbon + Files, dies for wire drawing,
remaining iron clutch disc
6 Spheroidal CI 3.2%-4.5% carbon 1-4% Si 0.1-8% Mn For high wear resistance
0.1% P 0-3.5% Ni 0.05-0.1% Mn
7 Wrought iron 99% Pig Iron + 0.12% Carbon + Chains, crane hooks,
0.25% Phosphorus + 0.05 % Sulphur railway couplings
5.11 CERAMICS MATERIALS
Ceramic materials are non-metallic solids made of inorganic compounds such as oxides,
nitrides, borides and carbides. Theses materials are fabricated by first shaping the powder
with or without the application of pressure into a compact form and after that it is subjected
to high temperature. Ceramics possesses electrical, magnetic, chemical and thermal properties
which are exceptionally good.
Examples: MgO, CdS, SiC, Al2O3, glass, cement, garnets, ferrites, concrete etc.
94 Introduction to Basic Manufacturing Processes and Workshop Technology
Ceramic materials are utilized for making electronic control devices, computers, structures,
components of nuclear engineering and aerospace field.
Composites are mixture of materials such as metal and alloys and ceramics, metals and
organic polymers, ceramics and organic polymers.
Examples: Vinyl coated steels, steel reinforced concrete, fiber reinforced plastics, carbon
reinforced rubber etc.
These materials are used for making sports items, structures, and electrical devices.
Semiconductors are solid materials, either non-metallic elements or compounds which allow
electrons to pass through them. These materials occupy intermediate position between
conductors and insulators. Semiconductors usually have high resistivity, negative temperature
coefficient of resistance and are generally hard and brittle.
Examples: Germanium (Ge), Arsenic (As), Silicon (Si), Boron (B), Sulphur (S), Selenium
Semiconductors are utilized in making devices used in areas of telecommunication and
radio communication, electronics and power engineering, photocells, rectifiers etc.
5.14 ORGANIC POLYMERS
Polymers consist of carbon chemically combined with usually with hydrogen, oxygen or other
non- metallic substances. They are formed by polymerization reaction in which simple molecules
are chemically combined into long chain molecules.
Examples: Nylon, Teflon, Polyethylene, PVC, Terylene, Cotton etc.
Polymers are used in making packings, pipes, covers and insulating materials etc.
Plastics are commonly known as synthetic resins or polymers. In Greek terminology, the
term polymer comprises ‘poly’ means ‘many’ and ‘mers’ means ‘parts’. Thus, the term, polymer
represents a substance built up of several repeating units, each unit being known as a
monomer. Thousands of such units or monomers join together in a polymerization reaction
to form a ‘polymer’. Some natural polymers like starch, resins, shellac, cellulose, proteins,
etc are vary common in today’s use. Synthetic polymers possess a number of large applications
in engineering work. Therefore plastic materials are fairly hard and rigid and can be readily
molded into different shapes by heating or pressure or both. Various useful articles can be
produced from them rapidly, accurately and with very good surface quality. They can be easily
Non-Ferrous Materials 95
produced in different colors or as transparent. They are recognized by their extreme lightness,
good corrosion resistance and high dielectric strength. Plastics are synthetic resins characterized
as a group by plastic deformation under stress. These materials generally are organic high
polymers (i.e. consisting of large chain like molecules containing carbon) which are formed
in a plastic state either during or after their transition from a low molecular weight chemical
to a high molecular weight solid material. These materials are very attractive organic
engineering materials and find extensive applications in industrial and commercial work such
as electrical appliances, automotive parts, communication products bodies (Telephone, Radio,
TV), and those making household goods. They possess a combination of properties which
make them preferable to other materials existing in universe.
Properties of plastics
The properties of plastics are given as under.
1. Plastics are light in weight and at the same time they possess good toughness
strength and rigidity.
2. They are less brittle than glass, yet they can be made equally transparent and
3. Their high dielectric strength makes them suitable for electric insulation.
4. They resist corrosion and the action of chemicals.
5. The ease with which they can be mass-produced contributes greatly to their popularity
as wrappers and bags.
6. They possess the property of low moisture absorption.
7. They can be easily molded to desired shapes.
8. They can easily be made colored.
9. They are bad conductance of heat.
10. They are hard, rigid and heat resistance.
11. They possesses good deformability, good resiatance against weather conditions, good
colorability, good damping characteristics and good resistance to peeling.
Plastics are broadly classified into thermo plastics and thermo-setting plastics.
5.15.1 Thermo Plastics
Those plastics which can be easily softened again and again by heating are called thermoplastic.
They can be reprocessed safely. They retain their plasticity at high temperature, i.e. they
preserve an ability to be repeatedly formed by heat and pressure. Therefore, they can be
heated and reshaped by pressing many times. On cooling they become hard. They are some
times also called as cold-setting plastics. They can be very easily shaped into tubes, sheets,
films, and many other shapes as per the need.
Types of Thermo Plastics
96 Introduction to Basic Manufacturing Processes and Workshop Technology
4 P.V.C (Polyvinyl chloride)
6 Auorinated polymers,
7 Polycarbonate etc.
The reason for the re-softening of thermoplastic resins with heat is that they are composed
of linear or long chain molecules. Application of heat weakens the intermolecular bonds by
increasing thermal agitation of the molecules, and the material softens and thus plastic can
be easily molded and remolded without damage
5.15.2 Thermo-Setting Plastics
Those plastics which are hardened by heat, effecting a non-reversible chemical change, are
called thermo-setting. Alternatively these plastics materials acquire a permanent shape when
heated and pressed and thus cannot be easily softened by reheating. They are commonly
known as heat-setting or thermosets.
(i) Phenol-formaldehyde resins
(ii) Urea-formaldehyde resins
(iii) Melamine-formaldehyde resins
(iv) Polyester resins
(v) Epoxy resins
(vi) Silicone resins
Other thermosetting compounds are phenol furfural, polysters, alkyds, and polyurethanes.
The most common thermosetting compound is phenol formaldehyde which is discussed as
Phenol formaldehyde is called as bakelite due to the name of its inventor Bakelite. It is
the most commonly and widely used plastic. It is made by the reaction of phenol with
formaldehyde. It has high strength, hardness, stability, rigidity and can be easily casted or
laminated. It is highly resistant to heat, electricity and water. It is made in dark color shades.
Its general uses are in making articles such as stereo cabinets, radio cabinets, plugs, knobs,
dials, bottle cap, pulleys, wheels, telephones, switches and handles.
Thermosetting resins, when subjected (once only) to the heat and pressure required for
forming, change into a hard and rigid substance. Once done so, they cannot be softened again
by the application of heat. The reason for the above phenomenon is that the thermosetting
plastics consist of linear, relatively low molecular weight thermoplastic polymer chains with
cross-links which bond the chains together with primary valence bonds. Such three-dimensional
Non-Ferrous Materials 97
polymers, once cross-linked, will not soften when heated (but may decompose disintegrate at
higher temperatures) because this process is an irreversible chemical reaction and the entire
structure becomes essentially a single molecule. In contrast the thermoplastic resins can be
re-softened and remolded by application of heat and pressure. They retain their plasticity at
high temperature, i.e. they preserve an ability to be repeatedly formed by heat and pressure.
5.15.3 Comparison Between Thermo Plastic and Thermosetting Plastic
Thermoplastic are those which are obtained from the substituted derivatives of ethylene
which can be made to polymerize under the influence of heat and catalyst. These materials
are softened by heat and affected by certain solvent. A notable feature of these resins is the
ability of their scrap or rejects to be reworked along with the new material. Cellulose nitrate
(celluloid) and polythene are the example of these materials. Where as thermosetting are
those which are formed into shape under heat and pressure and results in a permanently
hard product. The heat first softens the material, but as additional heat and pressure is
applied, it becomes hard phenol formaldehyde (bakelite). Phenol furfural (Durite) is the example
of thermosetting plastics. The comparison between thermo plastic and thermosetting plastic
is given in Table 5.2.
Table 5.2 Comparison between Thermo Plastic and Thermosetting Plastic
S.No Thermo Plastic Thermosetting Plastic
1 They can be repeatedly softened by heat Once hardened and set, they do not soften with
and hardened by cooling. the application of heat.
2 They are comparatively softer and less They are more stronger and harder than
strong. thermoplastic resins
3 Objects made by thermoplastic resins Objects made by thermosetting resins can be
can not be used at comparatively higher used at comparatively higher temperature
temperature as they will tend to soften without damage
4 They are usually supplied as granular They are usually supplied in monomeric or
material partially polymerized material form in which
they are either liquids or partially thermoplastic
5 Applications. Toys, combs, toilet goods, Applications. Telephone receivers, electric plugs,
photographic films, insulating tapes, radio and T.V. cabinets, camera bodies,
hoses, electric insulation, etc. automobile parts, tapes, hoses, circuit breaker
switch panels, etc.
5.15.4 Fabricating of Plastics
(a) Themo-plastics can be formed by
(i) Injection molding.
(iii) Blow molding.
98 Introduction to Basic Manufacturing Processes and Workshop Technology
(b) Thermosetting plastics can be formed by
(i) Compression or transfer molding.
Thermoplastics can be joined with the help of
(i) Solvent cements.
(ii) Adhesive bonding
(iv) Mechanical fasteners
Thermosetting plastics can be joined with the help of
(i) Adhesive bonding
(ii) Mechanical fasteners.
5.15.5 Additions in Polymer
To make polymer more for further processing of products, plastics, and some other material
are added to the polymers before or during polymerization. These materials are
They are also known accelerator or hardener. They act as catalysts to accelerate the
chemical reactions during polymerization of plastics.
Fillers are added to synthetic resins for increasing strength, stiffness and thermal
resistance of the plastics. These are clay, talc, alumina, carbon black, calcium carbonate, wood
flour, mica, quartz, asbestos, glass fibres etc.
Modifiers are added to plastics for improving mechanical properties
Plasticizers are fluids of high molecular weight. They are added for softening the resins
at forming temperature and to improve their toughness at the finished stage and to impart
flexibility to their finished products.
The additions of stabilizers to plastics help in preventing deterioration due to the action
of heat and light.
Initiators help in starting the reaction i.e. polymerization.
Dyes and pigments
Dyes and pigments are the coloring agents, added to impart different colors and shades
to plastic materials.
5.16 MATERIALS FOR NUCLEAR ENGINEERING PURPOSES
The various metals for producing nuclear energy are used as main materials namely
moderators, reflectors, fuel elements, fuel canning materials, control elements, and pressure
Non-Ferrous Materials 99
vessel materials. Uranium, thorium, plutonium, zirconium, beryllium, niobium and their
alloys are primarily used for nuclear engineering applications.
Most important metal found in nature and used for nuclear energy is uranium. It is used as
a nuclear fuel and is radioactive, easily oxidized mat and exists in three allotropic forms. It
has a poor resistance to corrosion and needs to be protected for use as fuel elements by roll
cladding a thin aluminium or zirconium jacket. Therefore it is strengthened by a thin film
of aluminium or zirconium through a rolling process known as cladding. This metal in the
pure condition is weak and is susceptible to severe irradiation damage and growth in the
reactor environments. Addition of some alloying elements such as chromium, molybdenum,
plutonium and zirconium are added to make great use of this material for generating nuclear
power. Uranium compounds have been found to give better service. Uranium oxide is re
highly refractory, shows no phase change in an inert atmosphere, possesses a good strength
and a high corrosion resistance. But it has a low thermal shock resistance, poor thermal
conductivity and a high coefficient of in expansion. The melting point of uranium is 1850°C.
Thorium is another possible fuel and is also a radioactive metal like uranium. It is a nuclear
fuel and is free from phase changes below 1480°C. It can be converted into uranium by beta
decay. It can be converted into uranium by beta decay. In its pure form it is weak and soft,
but its mechanical properties are improved by adding small amount of other elements e.g.,
only 0.2% of carbon addition raises its tensile strength from. Its mechanical properties change
drastically by small addition of impurities. Small additions of titanium, zirconium, and niobium
decrease the strength and hardness of the metal. Uranium addition increases the strength
of thorium. Thorium like uranium is an emitter of alpha rays and releases considerable
quantity of the radioactive products during processing, but this being a cubic metal is less
susceptible to irradiation damage. The melting point of thorium is 1845°C.
Plutonium is not a natural element but synthetic. It is produced through the absorption of
neutrons by uranium 238 and subsequent beta decays. It is a concentrated type of fuel used
in a fast reactor without a moderator. It is identified as highly toxic and chemically very
reactive material. It has a poor resistance to corrosion. This material can be easily oxidized.
It is frequently used for production of atomic weapons and it possesses tremendous applications
in breeder reactors.
The natural form of zirconium contains 0.5 to 2% halfnium which is a strong absorber of
neutrons and must therefore be removed. It possesses excellent corrosion resistance against
most of the acids and having good strength, good weldability and fatigue resistance. It has a poor
resistance to CO2 at elevated temperatures and that can be further improved by adding 0.5%
Cu and 0.5% Mo. It is specifically used in gas cooled reactors and cladding of fuel elements.
Beryllium is specially used as a moderator, reflector and neutron source in nuclear reactors.
It is a coarse grained light and brittle metal which possesses highly developed texture. During
100 Introduction to Basic Manufacturing Processes and Workshop Technology
melting, vacuum or inert gas is necessary because it is very reactive and forms compounds
with the furnace atmosphere and refractory materials. In order to fabricate components from
beryllium, powder metallurgy techniques are used.
Niobium possesses good corrosion resistance, strength and ductility. It has a high melting
point of 2470°C. Its oxidation resistance above 400°C is indifferent, but can be greatly improved
by alloying elements. It is added to many base metals to produce heat resisting alloys but this
material is quite expensive.
5.17 MATERIAL SELECTION PROCEDURE FOR COMPONENTS
For selection a material for a particular application, one has to take into consideration
various physical and mechanical properties of the material. Selection of material for a
manufacturing process is an important decision. In many instances, the selection of a specific
material can even dictate the manufacturing process to be used. The selection of material also
has an influence on the final cost of the product. It is important to note that the material
cost accounts to approximately 50% of the manufacturing cost. Hence, selection of manufacturing
process for a material must be made with the due care. The stepwise approach for material
selection is as follows:
1 Initially material requirement is identified by keeping in view overall objectives of
the part for which the selection of material is made. These objectives can be
referred with reference to cost, durability, life, etc.
2 The material requirements are identified through a number of materials. For example,
low specific weight requirement is met by aluminium and also by nylon. Make a list
of all such materials that meet all or most of the, requirements.
3 In case when more than one material appears to be suitable, the final choice should
be determined by considering influencing factors and restrictions like availability of
raw material, cost, inhibitions of aesthetics, and so on. For example, when we want
to select a material for manufacturing coins, the requirements are: the material
should possess good ductility, hardness, corrosion resistance, high plasticity, and
should be light in weight. The list of materials that satisfy these requirements is
large including gold, silver, copper, and their alloys. Final selection may be made
taking into consideration cost and availability. As another example, one uses stainless
steel for manufacturing shaving razor blades because the material selected should
have good malleability (ability to be hammered into thin sheets), corrosion resistance,
more abrasive resistance, and economical. The edge may be alloyed to make it hard
and retain sharpness.
The material selection procedure for the following products is given as under.
Rock crusher jaw
The function of crusher jaws is to crush. The crusher jaws should be hard, shock
absorbing and require good compressive strength. For such properties we choose cast-iron
because it has good castability, fluidity and good damping capacity. Its castings are made by
dry sand casting process.
Non-Ferrous Materials 101
It is made by plastic materials containing cellulose acetate (Thermo plastics), polystyrene
(thermoplastics) phenol formaldehyde (thermo setting plastics) because these materials have
high mechanical strength, impact resistance, transparency, colorability, fabricating quality,
versatility, molding ability, high dielectric strength and high refractive index.
Diesel Engine Piston
As the function of piston to reciprocate in the cylinder, it will require good wear and
corrosion resistance and ability to with stand at high temperature. Therefore material like
cast iron, bronze and aluminium alloy etc are preferred because of the requirements of
lightness with sufficient strength, refractoriness stress relieving, hardening, and tempering,
Lifting hook of crane
The purpose hook in crane is to lift load and it will require bearing sudden and excessive
heavy shock-loads without permanent injury. For such purposes wrought iron will prove
better and it is not heat-treated.
Bed of high precision lathe
Bed of high precision lathe needs high compressive strength, better shock absorbing
capacity, good damping capacity, corrosion resistance and good wear resistance, hardness and
reduced effect of residual stresses for better functional requirements. Grey cast iron because
its good lubricating properties due to presence of graphite will be suitable to meet the
functional requirements. However for increasing its usefulness alloying elements such as Ni,
Cr and Mo etc can also be alloyed in grey cast iron.
1. How do you classify non-ferrous metals?
2. Discuss the properties and uses of the following non-ferrous metals:
(i) Copper (ii) Zinc (iii) Aluminium (iv) Magnesium
(v) Lead (vi) Tin (vii) Nickel. (viii) Plutonium
3. What is brass? Describe the composition, properties and uses of important types of brasses?
4. What is bronze? Describe the composition, properties and uses of different types of bronzes?
5. Explain the various types of aluminium alloys giving their composition, properties and uses?
6. Discuss the various types of nickel alloys?
7. Which are the main metals used in nuclear energy? Describe them in brief.
8. How will you select the suitable engineering materials for a particular application?
102 Introduction to Basic Manufacturing Processes and Workshop Technology
Before pouring into the mold, the metal to be casted has to be in the molten or liquid state.
Furnace is used for carrying out not only the basic ore refining process but mainly utilized
to melt the metal also. A blast furnace performs basic melting (of iron ore) operation to get
pig iron, cupola furnace is used for getting cast iron and an electric arc furnace is used for
re-melting steel. Different furnaces are employed for melting and re-melting ferrous and non-
ferrous materials. The following are the factors which are responsible for the selection of
(i) Considerations of initial cost and cost of its operation.
(ii) Relative average cost of repair and maintenance.
(iii) Availability and relative cost of various fuels in the particular locality.
(iv) Melting efficiency, in particular speed of melting.
(v) Composition and melting temperature of the metal.
(vi) Degree of quality control required in respect of metal purification of refining,
(vii) Cleanliness and noise level in operation.
(viii) Personnel choice or sales influence.
Heat in a melting furnace is created by combustion of fuel, electric arc, electric resistance,
etc. A furnace contains a high temperature zone or region surrounded by a refractory wall
structure which withstands high temperatures and being insulating minimizes heat losses to
the surroundings. For refining and melting the ferrous and non ferrous materials, various
furnaces are used.
6.2 FURNACES FOR MELTING DIFFERENT MATERIALS
1. Grey Cast Iron
(b) Air furnace (or Reverberatory Furnace)
(c) Rotary furnace
(d) Electric arc furnace
Melting Furnaces 103
(a) Electric furnaces
(b) Open hearth furnace
3. Non-ferrous Metals
(a) Reverberatory furnaces (fuel fired) (Al, Cu)
(b) Rotary furnaces
(i) Fuel fired
(ii) Electrically heated
(c) Induction furnaces (Cu, Al)
(i) Low frequency
(ii) High frequency.
(d) Electric Arc furnaces (Cu)
(e) Crucible furnaces (AI, Cu)
(i) Pit type
(ii) Tilting type
(iii) Non-tilting or bale-out type
(iv) Electric resistance type (Cu)
(f) Pot furnaces (fuel fired) (Mg and AI)
Some of the commonly used furnaces in foundries are discussed as under.
6.3 BLAST FURNACE
After mining, various kinds of iron ores are brought to the blast furnace which is the starting
process for refining iron ores or mined ores and for the poduction of pig iron. Blast furnace
was invented in 14th century. A typical blast furnace along with its various parts is shown
in Fig. 6.1. It is large steel shell about 9 mt. in diameter which is lined with heat resistant
bricks. It is set on the top of brick foundation. There are four major parts of blast furnace
from bottom to top hearth, bosh, stack and top. The hearth acts as a storage region for
molten metal and molten slag. The charge of blast furnace possesses successive layers of iron
ore, scrap, coke, and limestone and some steel scrap which is fed from the top of the furnace.
Iron ore exists as an aggregate of iron-bearing minerals. These mineral aggregates are oxides
of iron called hematite, limonite, and magnetite. They all contribute to the smelting process.
Hematite is a red ore and contains about 70% iron. Limonite is a hydrated oxide and contains
about 60% iron. Magnetite is a magnetic oxide and contains about 72% iron. It takes about
1.6 tons of iron ore, 0.65 ton of coke, 0.2 ton of lime-stone and about 0.05 ton of scrap iron
and steel to produce 1 ton of pig iron. For burning this charge, about 4 tons of air is required.
The impurities or other minerals are present in the ore. These impurities may be silicon,
104 Introduction to Basic Manufacturing Processes and Workshop Technology
Fig. 6.1 Typical blast furnace
sulfur, phosphorus, manganese, calcium, titanium, aluminum, and magnesium. The amounts
of silicon, phosphorus, and sulfur present will determine the purification process used in the
manufacture of the steel. The output from the furnace in form of pig iron is collected in large
ladles from the tap hole existing at lower portion of furnace. As the coke burns, aided by the
air forced into the furnace, the ore melts and collects in the hearth. As the melting process
proceeds, the entire mass settles and thus makes room for the addition of charges at the top.
While the melting is going on, the limestone forms a slag with the impurities. The second
component which makes up the charge is the coke which is made from coal. Coke must be
dust proof, not too combustible, and strong, since it must support the charge. It supplies the
heat which reduces the ore and melts the iron. The iron picks up carbon from the coke and
impurities from the ore. The amount of carbon picked up by the iron is more than is needed
in the production of steel. The carbon becomes part of the pig iron used in the making of
steel. The control of this carbon during the subsequent processes determines the properties
of the steel. The manufacture of coke from bituminous coal is a distillation process. The
impurities are driven off leaving coke.
The pig iron is then processed for purification work for production of various kinds of
iron and steel in form of ingots (large sections) using different furnaces. Fig 6.2 shows a flow
chart for production of different kinds of iron and steel. The steel ingots can be further
processed in rolling mill or blooming mill to produce different structural shapes and sections
of steel. Fig 6.3 represents the entire process for production of market form of steel supply
of different shapes or sections.
Melting Furnaces 105
Slag and cinders
Fig. 6.2 Flow chart for converting pig iron into useful iron and steel
6.4 CUPOLA FURNACE
Cupola furnace is employed for melting scrap metal or pig iron for production of various cast
irons. It is also used for production of nodular and malleable cast iron. It is available in good
varying sizes. Fig. 6.4 shows the various parts and zones of cupola furnace. The main
considerations in selection of cupolas are melting capacity, diameter of shell without lining
or with lining, spark arrester.
Limestone Slag Iron
106 Introduction to Basic Manufacturing Processes and Workshop Technology
Fig. 6.3 Production process of market form of steel supply of different shapes or sections
Furnacl Charging door
Air blast inlet
Fig. 6.4 Cupola furnace
6.4.1 Various Zones of Cupola Furnace
Various numbers of chemical reactions take place in different zones of cupola. The construction
and different zones of cupola are discussed as under.
Melting Furnaces 107
The space between the bottom of the tuyeres and the sand bed inside the cylindrical shell
of the cupola is called as well of the cupola. As the melting occurs, the molten metal is get
collected in this portion before tapping out.
2. Combustion zone
The combustion zone of Cupola is also called as oxidizing zone. It is located between
the upper of the tuyeres and a theoretical level above it. The total height of this zone is
normally from 15 cm. to 30 cm. The combustion actually takes place in this zone by consuming
the free oxygen completely from the air blast and generating tremendous heat. The heat
generated in this zone is sufficient enough to meet the requirements of other zones of cupola.
The heat is further evolved also due to oxidation of silicon and manganese. A temperature
of about 1540°C to 1870°C is achieved in this zone. Few exothermic reactions takes place in
this zone these are represented as :
C + O2 ——→→→→→ CO2 + Heat
Si + O2 ——→→→→→ SiO2 + Heat
2Mn + O2 ——→→→→→ 2MnO + Heat
3. Reducing zone
Reducing zone of Cupola is also known as the protective zone which is located between
the upper level of the combustion zone and the upper level of the coke bed. In this zone, CO2
is changed to CO through an endothermic reaction, as a result of which the temperature falls
from combustion zone temperature to about 1200°C at the top of this zone. The important
chemical reaction takes place in this zone which is given as under.
CO2 + C (coke) ——→→→→→ 2CO + Heat
Nitrogen does not participate in the chemical reaction occurring in his zone as it is also
the other main constituent of the upward moving hot gases. Because of the reducing atmosphere
in this zone, the charge is protected against oxidation.
4. Melting zone
The lower layer of metal charge above the lower layer of coke bed is termed as melting
zone of Cupola. The metal charge starts melting in this zone and trickles down through coke
bed and gets collected in the well. Sufficient carbon content picked by the molten metal in
this zone is represented by the chemical reaction given as under.
3Fe + 2CO ——→→→→→ Fe3C + CO2
5. Preheating zone
Preheating zone starts from the upper end of the melting zone and continues up to the
bottom level of the charging door. This zone contains a number of alternate layers of coke bed,
flux and metal charge. The main objective of this zone is to preheat the charges from room
temperature to about 1090°C before entering the metal charge to the melting zone. The
preheating takes place in this zone due to the upward movement of hot gases. During the
preheating process, the metal charge in solid form picks up some sulphur content in this zone.
The empty portion of cupola above the preheating zone is called as stack. It provides the
passage to hot gases to go to atmosphere from the cupola furnace.
108 Introduction to Basic Manufacturing Processes and Workshop Technology
6.4.2 Charging of Cupola Furnace
Before the blower is started, the furnace is uniformly pre-heated and the metal and coke
charges, lying in alternate layers, are sufficiently heated up. The cover plates are positioned
suitably and the blower is started. The molten metal starts trickling down and collecting in
the well. The height of coke charge in the cupola in each layer varies generally from 10 to
15 cms. The requirement of flux to the metal charge depends upon the quality of the charged
metal and scarp, the composition of the coke and the amount of ash content present in the
coke. Generally about 40 kg to 50 kg of limestone, in form of flux, per metric ton of the metal
is used. The amount of this flux to be charged should be properly determined. The excess
amount of flux affects the acid lining of cupola. Lesser amount of the flux than required will
result in the loss of molten metal. First charge received of the molten metal is either allowed
to drain out or used for rough castings. For having desired composition of the casting, it is
essential to control the proportions of its various constituents at the stage of raw material
requirement for melting. It is also necessary due to number of losses and gains of different
constituents take place inside the cupola during the process of melting. These losses and
gains in composition are identified for compensating purposes. The losses or gains of different
constituents during melting as identified are given as under:
1. Iron – Loss of about 4%
2. Carbon – Gain of about 0.1 to 0.15%.
3. Silicon – Loss of about 10%
4. Manganese – Loss of about 15 to 20%.
5. Phosphorus – Practically no change.
6. Sulphur – Gain of about 0.03 to 0.05%.
6.4.3 Working of Cupola Furnace
Initially the furnace prop is opened to drop the existing earlier charge residue. The furnace
is then repaired using rich refractory lining. After setting the prop in position, the fire is
ignited using firewood and then small amount of coke is used to pick fire. The little oxygen
is then supplied for combustion. Lime, coke, and metal in balanced proportions are charged
through the charging door upon the coke bed and at proper time on starting the blower. Air
is forced from wind box through tuyers into furnace. The forced air rise upward rough the
stack furnaces for combustion of coke. Besides being fuel, the coke supports the charge until
melting occurs. On increase of temperature, the lime stone melts and forms a flux which
protects the metal against from excessive oxidation. Lime also fuses and agglomerates the
coke ash. The melting occurs and proceeds and molten metal is collected at the bottom.
Molten metal may be tapped at intervals before each skimming, or the tap-hole may be left
open with metal flowing constantly. In most cupolas slag is drained from the slag hole at the
back of furnace. When metal is melted completely the bottom bar is pulled sharply under the
plates and bottom is dropped. All remaining slag, un-burned coke or molten metal drops from
the furnace. When the melt charge has cooled on closing furnace, it is patched and made
ready for the next heat.
Applications of Cupola
Cupola is most widely used for melting practices for production of grey cast iron, nodular
cast iron, malleable cast iron and alloy cast iron. It can be used for melting some copper-base
alloys, and in duplexing and triplexing operations for making of steel, malleable cast iron and
ductile cast iron. Steel can be also prepared in cupola by employing duplexing and triplexing
Melting Furnaces 109
operations. In duplexing melting operation two furnaces are used, and triplexing operations,
three furnaces are employed
6.4.4 Jamming of Cupola Furnace
Jamming of cupola furnace is a very common problem for which sufficient care should be
taken to prevent it. It occurs frequently due to the negligence of the furnace operator. The
cupola furnace may be either jammed temporarily or permanently and the same are discussed
6.4.5 Temporary Jamming of Cupola Furnace
Temporary jamming of cupola furnace means the temporary suspension of air supply in
the tuyere zone due to choking of the tuyere mouths. This is caused mainly due to the low
temperatures at the tuyere openings resulting in the solidification of iron and slag around
these openings. The air passage is hence chocked and the supply of air is temporarily stopped.
It results in incomplete combustion of the coke/fuel inside the furnace and hence leads to
rapid reduction of the temperature in the furnace. Therefore this temporary jamming must
be prevented by frequent poking of this solidified material by means of a poking bar through
the tuyeres. The operator of cupola should always keep himself alert enough for not allowing
such solidification for continue melting in furnace for a longer period.
6.4.6 Permanent Jamming of Cupola Furnace
Permanent jamming of cupola furnace means a complete cut-off of the air supply to the cupola
due to the permanent choking of the air passage. This occurs on account of the overflow of
the slag into the wind chamber. As the metal melts and starts collecting in the well of the
furnace, its level rises gradually and the slag being lighter, always floats on the top surface
of the molten metal. If, the molten metal is not tapped out in time due to the negligence of
the operator, the level of molten metal in furnace will start rising in the well and a stage will
come when this level approaches to the tuyere level. Any slightest delay further, in tapping
by the cupola operator will cause the slag to flow through the tuyere openings into the wind
belt. Since the slag comes in contact with the air at low temperature it quickly solidifies in
the wind belt as well as in the tuyers and therefore chock the passages of air flow permanently
in the furnace. Hence the cupola furnace reaches in such undesirable condition on account
of the above occurrence. Therefore, to avoid such undesired situation, the operator of cupola
furnace should always be vigilant enough to tap the molten metal out from well of the cupola
furnace before the level of molten metal rises up to the tuyere level. Hence the cupola
furnace may continue melting for longer period.
6.4.7 Thermal Efficiency of Cupola Furnace
Thermal efficiency of cupola furnace is the ratio of heat actually utilized in melting and
superheating the metal to the heat evolved in it through various means. The total heat
evolved involves the heat due burning of coke, heat evolved due to oxidation of iron, Si and
Mn and heat supplied by the air blast. During melting it is observed that approximately 48-
70 % of the evolved heat is going as waste.
6.4.8 Precautions for Safety of Cupola Furnace
For operating the cupola successfully, the following safety precautions must always be kept
110 Introduction to Basic Manufacturing Processes and Workshop Technology
1. For safety of Cupola, better quality refractory lining must be used for preparing or
repairing furnace so that it can withstand high temperature as produced inside the
furnace during melting, otherwise it will fuse and mix with molten metal to form
2. The furnace operator during firing the furnace should always make an effort to
place the metal charge in the centre. He must ensure that the coke charge is well
distributed all around and towards the firebrick lining to ensure uniform and thorough
melting of the metal.
3. As the air passes through the tuyeres, the temperature near the tuyere openings
will therefore be comparatively lower and consequently the molten iron and slag
will have a tendency to solidify near these openings and block them. This should
be prevented by frequent poking and removal of these materials by means of a
poking rod through the tuyeres.
4 Amount of air supply should be properly controlled. An excess amount of air will
always result in waste of fuel and lowering of temperature inside and a lesser
amount, than required, will cause incomplete combustion of fuel which is undesirable.
5. Tap hole must be properly closed by means of a well suitable plugging means. Clay
mixed with an equal amount of coal dust forms a very suitable mixture for plugging
up the tap hole.
6 In closing the tap-hole, precaution must be taken to press the plug downwards in
the hole so that the splash of the molten metal, during plugging does not fall on
the hands of the furnace operator.
7 Molten metal should always be tapped out well in time before its level rises too high
in the well of the cupola furnace. Any delay of tapping molten metal, the slag
floating on the surface of the molten metal, will start flowing into the wind belt
through the tuyeres and air passage will be choked and it will result in severe
problem of the jamming of cupola furnace.
6.5 OPEN HEARTH FURNACE
In open hearth furnace, pig iron, steel scrap etc. are melted to obtain steel. This furnace is
widely used in American foundries for steel production. The hearth is surrounded by roof and
walls of refractory bricks as shown in Fig. 6.5. The charge is fed through a charging door and
is heated to 1650°C mainly by radiation of heat from the burning of gaseous fuels above it. This
heat is obtained by the burning of sufficiently pre-heated air and gas. Such pre-heated air of gas
is obtained by passing them though arc shaped hot regenerators at a lower level. This contains
fire bricks which are arranged to extract heat from exhaust gases. In the furnace air and fuel
are passed through a honeycomb of hot firebrick, called checkers. It preheats the air and fuel
so that they are ready for combustion when they enter the hearth. The products of combustion
at the same time pass through the checkers at the other end of the furnace. The hot gases heat
the checkers. The process then reverses itself, and the newly heated checkers now are used to
heat the air and the fuel. It is said as a regenerative process. The products of combustion after
giving up their heat to the checkers pass up through the stack. On firing of coke, the charge
is heated. Part of the heat necessary, results from radiation from the low hot roof of the
chamber. The furnace is raised bricked in with the charging platform, at the rear, also raised
so that the charge may be put into the furnace. The melt is tapped off the front into large ladles.
Melting Furnaces 111
The chemical composition of the end product depends upon the lining, the charge, and the
control impurities added during the melt after the melt has been tapped off into the ladle. The
lining plays a major roll in the control of impurities. For magnesite lined furnace, the charge
consists of pig iron, limestone, and scrap iron. The limestone forms a slag. This slag and the
oxygen in the air combine to remove impurities. The slag reacts with the sulfur and the
1. Walls of refractory bricks, 2. Roof, 3. Melting chamber,
4. Air and gas ducts, 5. Charging doors, 6. Checkerwork
Fig. 6.5 Open hearth furnace
phosphorus in the metal, while the bubbling air causes oxidation of the carbon and silicon. If
too much carbon is present in the melt, iron ore is added. The oxygen from the iron oxide burns
out the excess carbon. If the carbon content is too low, pig iron is added. This replenishes the
carbon. Other alloying elements like Cr, Ni. Co, W, Mo, V etc. are added as needed.
Ferromanganese may be added to the crucible after tapping. For acid lining furnace, the charge
should be scrap iron and low-phosphorus pig iron. Limestone is required to keep the slag fluid.
As described above, the basic lining burns phosphorus, silicon, and carbon. The slag is tapped
off by the molten metals being allowed to overflow the sides of the crucible into a slag pot.
Oxygen is one of the most important elements used in the reduction of the molten metal. Rust,
scale, slag, and limestone are some of the sources of oxygen. Oxygen is introduced into the
furnace with oxygen lances through the roof of the furnace. Twice the oxygen input will double
the carbon reduction. This increases the steel production of the furnace.
6.6 PIT FURNACE
Pit furnace is a type of a furnace bath which is installed in the form of a pit and is used for
melting small quantities of ferrous and non ferrous metals for production of castings. It is
provided with refractory inside and chimney at the top. Generally coke is used as fuel. It is
provided with refractory lining inside and chimney at the top. Natural and artificial draught
can be used for increasing the capability towards smooth operation of the furnace. Fig. 6.6
shows the typical pit furnace.
112 Introduction to Basic Manufacturing Processes and Workshop Technology
Fig. 6.6 Pit furnace
6.7 CORELESS TYPE INDUCTION FURNACE
It is also called high frequency induction furnace. It consists of refractory crucible placed
centrally inside a water cooled copper coil. Fig. 6.7 represent the construction and working
of this type of furnace.
Molten Metal Crucible
Transite or tilting shell
of Copper Tubing
on Molten Metal
Fig. 6.7 Coreless type induction furnace
6.8 AIR FURNACE
This furnace is also known as puddling or reverbratory furnace. It is used for making
wrought iron. Fig 6.8 shows the construction of this type of furnace.
Melting Furnaces 113
Fire Bridge Skimming
TAP Hole Molten Iron Hearth
Fig. 6.8 Air furnace
6.9 METHODS OF MEASURING TEMPERATURE
Furnace temperature is measured by following methods namely (i) Electrical pyrometers (2)
Thermo electric pyrometers (3) Radiation pyrometers (4) Optical pyrometers and (5) Photo-
An important radiation pyrometer is discussed as under.
Crucible Teapot Pouring
(a) (b) (c)
Fig. 6.9 Pouring practices
6.9.1 Radiation Pyrometer
Radiation pyrometer is a temperature device by which the temperature of hot body is measured
by measuring the intensity of total heat and light radiation emitted by a hot body. A radiation
pyrometer works on the principle of focusing the energy from all wave lengths of radiation
upon a sensitive element thus causing a force to be developed in the element which may be
114 Introduction to Basic Manufacturing Processes and Workshop Technology
a resistance pyrometer or a thermo couple. All the radiations are concentrated by concave
mirror upon the hot junction of a thermo couple. Mirror placed in inclined position is used
to indicate whether correct focus can be obtained.
6.10 POURING PRACTICES
Molten metal is collected in ladles from furnaces and skimmed properly before pouring into
the mould. Some of the pouring practices are shown in Fig 6.9.
1 What are the general principles of the melting practice?
2 What important factors are considered during melting?
3 What are the factors which govern the selection of a suitable type of furnace for melting a
4 What characteristics a refractory material should possess to make it suitable for use in
furnaces? How many types of refractory are there?
5 Sketch a blast furnace. Describe its construction and working.
6 Make a neat sketch of a cupola, indicating its various zones and describe the following:
(ii) Preparation before operations
(iii) Charging method
(iv) Different zones and their functions
(vii) Limitations and
7 What do you mean by basic and acid cupolas? Where each type is preferred and why?
8 How is air requirement for cupola calculated
9 Why is the flux used during melting of metals in cupola?
10 How do you determine the thermal efficiency of a cupola furnace?
11 How will you specify a cupola furnace?
12 What necessary precautions are required in operating the cupola?
13 What are the expected gains in or losses of the various constituents of metal charge during
melting and how are these constituents controlled?
14 Why does a cupola sometimes get jammed up? How can it be prevented?
15 Explain with the help of neat sketches the construction and working of the following types
of crucible furnaces: (a) A coal fired pit furnace, (b) An oil fired tilting furnace, and (c) A gas
fired crucible furnace
16 What are crucible furnaces? Where are they preferred and why?
17 What are the different types of electric furnaces? Describe anyone of them.
18 Describe crucible furnaces.
19 Write short notes on the following:
(a) Open-hearth furnace and (b) Resistance furnace.
Melting Furnaces 115
20 What is refining?
21 What are the different types of pouring ladles?
22 Describe the construction working and uses of core less type induction furnace.
23 What do you understand by fluxing?
24 Name the different types of fluxes, arid describe anyone of them.
25 Describe the purpose for using the pyrometers in melting practice.
116 Introduction to Basic Manufacturing Processes and Workshop Technology
PROPERTIES AND TESTING OF METALS
7.1 PROPERTIES OF METALS
The important properties of an engineering material determine the utility of the material
which influences quantitatively or qualitatively the response of a given material to imposed
stimuli and constraints. The various engineering material properties are given as under.
1. Physical properties
2. Chemical properties
3. Thermal properties
4. Electrical properties
5. Magnetic properties
6. Optical properties, and
7. Mechanical properties
These properties of the material are discussed as under.
7.1.1 Physical Properties
The important physical properties of the metals are density, color, size and shape (dimensions),
specific gravity, porosity, luster etc. Some of them are defined as under.
Mass per unit volume is called as density. In metric system its unit is kg/mm3. Because of
very low density, aluminium and magnesium are preferred in aeronautic and transportation
It deals the quality of light reflected from the surface of metal.
3. Size and shape
Dimensions of any metal reflect the size and shape of the material. Length, width,
height, depth, curvature diameter etc. determines the size. Shape specifies the rectangular,
square, circular or any other section.
Porperties and Testing of Metals 117
4. Specific Gravity
Specific gravity of any metal is the ratio of the mass of a given volume of the metal to
the mass of the same volume of water at a specified temperature.
A material is called as porous or permeable if it has pores within it.
7.1.2 Chemical Properties
The study of chemical properties of materials is necessary because most of the engineering
materials, when they come in contact with other substances with which they can react, suffer
from chemical deterioration of the surface of the metal. Some of the chemical properties of
the metals are corrosion resistance, chemical composition and acidity or alkalinity. Corrosion
is the gradual deterioration of material by chemical reaction with its environment.
7.1.3 Thermal Properties
The study of thermal properties is essential in order to know the response of metal to
thermal changes i.e. lowering or raising of temperature. Different thermal properties are
thermal conductivity, thermal expansion, specific heat, melting point, thermal diffusivity.
Some important properties are defined as under.
Melting point is the temperature at which a pure metal or compound changes its shape
from solid to liquid. It is called as the temperature at which the liquid and solid are in
equilibrium. It can also be said as the transition point between solid and liquid phases.
Melting temperature depends on the nature of inter-atomic and intermolecular bonds. Therefore
higher melting point is exhibited by those materials possessing stronger bonds. Covalent,
ionic, metallic and molecular types of solids have decreasing order of bonding strength and
melting point. Melting point of mild steel is 1500°C, of copper is 1080°C and of Aluminium is
7.1.4 Electrical Properties
The various electrical properties of materials are conductivity, temperature coefficient of
resistance, dielectric strength, resistivity, and thermoelectricity. These properties are defined
Conductivity is defined as the ability of the material to pass electric current through it
easily i.e. the material which is conductive will provide an easy path for the flow of electricity
2. Temperature Coefficient of Resistance
It is generally termed as to specify the variation of resistivity with temperature.
3. Dielectric Strength
It means insulating capacity of material at high voltage. A material having high dielectric
strength can withstand for longer time for high voltage across it before it conducts the
current through it.
118 Introduction to Basic Manufacturing Processes and Workshop Technology
It is the property of a material by which it resists the flow of electricity through it.
If two dissimilar metals are joined and then this junction is heated, a small voltage (in
the milli-volt range) is produced, and this is known as thermoelectric effect. It is the base of
the thermocouple. Thermo -couples are prepared using the properties of metals.
7.1.5 Magnetic Properties
Magnetic properties of materials arise from the spin of the electrons and the orbital motion
of electrons around the atomic nuclei. In certain atoms, the opposite spins neutralize one
another, but when there is an excess of electrons spinning in one direction, magnetic field
is produced. Many materials except ferromagnetic material which can form permanent magnet,
exhibit magnetic affects only when subjected to an external electro-magnetic field. Magnetic
properties of materials specify many aspects of the structure and behavior of the matter.
Various magnetic properties of the materials are magnetic hysteresis, coercive force and
absolute permeability which are defined as under.
1. Magnetic Hysteresis
Hysteresis is defined as the lagging of magnetization or induction flux density behind the
magnetizing force or it is that quality of a magnetic substance due to energy is dissipated in
it on reversal of its magnetism. Below Curie temperature, magnetic hysteresis is the rising
temperature at which the given material ceases to be ferromagnetic, or the falling temperature
at which it becomes magnetic. Almost all magnetic materials exhibit the phenomenon called
2. Coercive Force
It is defined as the magnetizing force which is essential to neutralize completely the
magnetism in an electromagnet after the value of magnetizing force becomes zero.
3. Absolute Permeability
It is defined as the ratio of the flux density in a material to the magnetizing force
producing that flux density. Paramagnetic materials possess permeability greater than one
whereas di-magnetic materials have permeability less than one.
7.1.6 Optical Properties
The main optical properties of engineering materials are refractive index, absorptivity,
absorption co-efficient, reflectivity and transmissivity. Refractive index is an important optical
property of metal which is defined as under.
It is defined as the ratio of velocity of light in vacuum to the velocity of a material. It
can also be termed as the ratio of sine of angle of incidence to the sine of refraction.
7.1.7 Mechanical Properties
Under the action of various kinds of forces, the behavior of the material is studied that
measures the strength and lasting characteristic of a material in service. The mechanical
properties of materials are of great industrial importance in the design of tools, machines and
Porperties and Testing of Metals 119
structures. Theses properties are structure sensitive in the sense that they depend upon the
crystal structure and its bonding forces, and especially upon the nature and behavior of the
imperfections which- exist within the crystal itself or at the grain boundaries. The mechanical
properties of the metals are those which are associated with the ability of the material to resist
mechanical forces and load. The main mechanical properties of the metal are strength, stiffness,
and weldability. These properties can be well understood with help of tensile test and stress
strain diagram. The few important and useful mechanical properties are explained below.
It is defined as the property of a material to regain its original shape after deformation
when the external forces are removed. It can also be referred as the power of material to
come back to its original position after deformation when the stress or load is removed. It
is also called as the tensile property of the material.
2. Proportional limit
It is defined as the maximum stress under which a material will maintain a perfectly
uniform rate of strain to stress. Though its value is difficult to measure, yet it can be used
as the important applications for building precision instruments, springs, etc.
3. Elastic limit
Many metals can be put under stress slightly above the proportional limit without
taking a permanent set. The greatest stress that a material can endure without taking up
some permanent set is called elastic limit. Beyond this limit, the metal does not regain its
original form and permanent set will occurs.
4. Yield point
At a specific stress, ductile metals particularly ceases, offering resistance to tensile
forces. This means, the metals flow and a relatively large permanent set takes place without
a noticeable increase in load. This point is called yield point. Certain metals such as mild steel
exhibit a definite yield point, in which case the yield stress is simply the stress at this point.
Strength is defined as the ability of a material to resist the externally applied forces with
breakdown or yielding. The internal resistance offered by a material to an externally applied
force is called stress. The capacity of bearing load by metal and to withstand destruction
under the action of external loads is known as strength. The stronger the material the
greater the load it can withstand. This property of material therefore determines the ability
to withstand stress without failure. Strength varies according to the type of loading. It is
always possible to assess tensile, compressive, shearing and torsional strengths. The maximum
stress that any material can withstand before destruction is called its ultimate strength. The
tenacity of the material is its ultimate strength in tension.
It is defined as the ability of a material to resist deformation under stress. The resistance
of a material to elastic deformation or deflection is called stiffness or rigidity. A material that
suffers slight or very less deformation under load has a high degree of stiffness or rigidity.
For instance suspended beams of steel and aluminium may both be strong enough to carry
the required load but the aluminium beam will “sag” or deflect further. That means, the steel
120 Introduction to Basic Manufacturing Processes and Workshop Technology
beam is stiffer or more rigid than aluminium beam. If the material behaves elastically with
linear stress-strain relationship under Hooks law, its stiffness is measured by the Young’s
modulus of elasticity (E). The higher is the value of the Young’s modulus, the stiffer is the
material. In tensile and compressive stress, it is called modulus of stiffness or “modulus of
elasticity”; in shear, the modulus of rigidity, and this is usually 40% of the value of Young’s
modulus for commonly used materials; in volumetric distortion, the bulk modulus.
Plasticity is defined the mechanical property of a material which retains the deformation
produced under load permanently. This property of the material is required in forging, in
stamping images on coins and in ornamental work. It is the ability or tendency of material
to undergo some degree of permanent deformation without its rupture or its failure. Plastic
deformation takes place only after the elastic range of material has been exceeded. Such
property of material is important in forming, shaping, extruding and many other hot or cold
working processes. Materials such as clay, lead, etc. are plastic at room temperature and steel
is plastic at forging temperature. This property generally increases with increase in temperature
Ductility is termed as the property of a material enabling it to be drawn into wire with
the application of tensile load. A ductile material must be strong and plastic. The ductility is
usually measured by the terms, percentage elongation and percent reduction in area which
is often used as empirical measures of ductility. The materials those possess more than 5%
elongation are called as ductile materials. The ductile material commonly used in engineering
practice in order of diminishing ductility are mild steel, copper, aluminium, nickel, zinc, tin
Malleability is the ability of the material to be flattened into thin sheets under applications
of heavy compressive forces without cracking by hot or cold working means. It is a special
case of ductility which permits materials to be rolled or hammered into thin sheets. A
malleable material should be plastic but it is not essential to be so strong. The malleable
materials commonly used in engineering practice in order of diminishing malleability are
lead, soft steel, wrought iron, copper and aluminium. Aluminium, copper, tin, lead, steel, etc.
are recognized as highly malleable metals.
Hardness is defined as the ability of a metal to cut another metal. A harder metal can
always cut or put impression to the softer metals by virtue of its hardness. It is a very
important property of the metals and has a wide variety of meanings. It embraces many
different properties such as resistance to wear, scratching, deformation and machinability etc.
Brittleness is the property of a material opposite to ductility. It is the property of
breaking of a material with little permanent distortion. The materials having less than 5%
elongation under loading behavior are said to be brittle materials. Brittle materials when
subjected to tensile loads, snap off without giving any sensible elongation. Glass, cast iron,
brass and ceramics are considered as brittle material.
Porperties and Testing of Metals 121
When a metal part when is subjected to a high constant stress at high temperature for
a longer period of time, it will undergo a slow and permanent deformation (in form of a crack
which may further propagate further towards creep failure) called creep.
It is the property of metals which denotes the ease in its forming in to various shapes
and sizes. The different factors that affect the formability are crystal structure of metal, grain
size of metal hot and cold working, alloying element present in the parent metal. Metals with
smal1 grain size are suitable for shallow forming while metal with size are suitable for heavy
forming. Hot working increases formability. Low carbon steel possesses good formability.
Castability is defined as the property of metal, which indicates the ease with it can be
casted into different shapes and sizes. Cast iron, aluminium and brass are possessing good
Weldability is defined as the property of a metal which indicates the two similar or
dissimilar metals are joined by fusion with or without the application of pressure and with
or without the use of filler metal (welding) efficiently. Metals having weldability in the
descending order are iron, steel, cast steels and stainless steels.
7.2 RECOVERY,RECRYSTALLISATIONAND GRAIN GROWTH
When metal is subjected to hot working and cold working processes, plastic deformation
occurs which is an important phenomenon. Plastic deformation of metal distorts the crystal
lattice. It breaks up the blocks of initial equiaxed grains to produce fibrous structure and
increases the energy level of metal. Deformed metal, during comparison with its un-deformed
state, is in non-equilibrium, thermodynamically unstable state. Therefore, spontaneous
processes occur in strain-hardened metal, even at room temperature that brings it into a
more stable condition. When the temperature of metal is increased, the metal attempts to
approach equilibrium through three processes: (i) recovery, (ii) recrystallisation, and (iii) grain
growth. Fig.7.1 reflects the recovery, recrystallisation and grain growth and the main property
changes in each region.
When a strain-hardened metal is heated to a low temperature, the elastic distortions of the
crystal lattice are reduced due to the increase in amplitude of thermal oscillation of the
atoms. This heating will decrease the strength of the strain-hardened metal but there is an
increase in the elastic limit and ductility of metal, though they will not react the values
possessed by the initial material before strain-hardening. No changes in microstructure of
metal are observed in this period. The partial restoration of the original characteristics,
produced by reducing the distortion of the crystal lattice without remarkable changes in
microstructure, is called recovery. At the initial state, the rate of the recovery is fastest and
it drops off at longer times at given temperature. Hence the amount of recovery that occurs
in a practical time increases with increasing temperature. The individual characteristic recover
at different rates and gain various degrees of completion in a given cold worked metal.
122 Introduction to Basic Manufacturing Processes and Workshop Technology
Formation of new equiaxed grains in the heating process of metal, instead of the oriented
fibrous structure of the deformed metal, is called recrystallisation. The process of
recrystallisation is illustrated through Fig. 7.1. The first effect of heating of metal is to form
new minute grains and these rapidly enlarge until further growth is restricted by grain
meeting another. The original system of grains go out of the picture and the new crystallized
structure is formed in the metal. Recrystallisation does not produce new structures however
it produces new grains or crystals of the same structure in the metal. It consists in having
the atoms of the deformed metal overcome the bonds of the distorted lattice, the formation
of nuclei of equiaxed grains and subsequent growth of these grains due to transfer of atoms
from deformed to un-deformed crystallites. Finer grains get refined and acquire a shape
resembling fibres. The temperature at which crystallization starts, that is new grains are
formed, is called recrystallisation temperature. Recrystallisation temperature is also
defined as that temperature at which half of the cold worked material will recrystallise in 60
Cold worked and reworked
Recrystallization Grain growth
Fig. 7.1 Recovery, recrystalisation and grain growth
7.2.3 Grain Growth
On recrystallisation of metal, the grains are smaller and somewhat regular in shape. The
grains in metal will grow if the temperature is high enough or if the temperature is allowed
to exceed the minimum required for recrystallisation and this growth of grain is the result
of a tendency to return to more stable and larger state. It appears to depend primarily on
the shape of the grain. For any temperature above the recrystallization temperature, normally
there is practical maximum size at which the grains will reach equilibrium and cease to grow
significantly. However, there are certain kinds of abnormal grains growth in metal that occur
as a result of applied or residual gradients of strain due to non-uniform impurity distribution,
and which permits growing very large single grain in metal.
7.3 TESTING OF METALS
Metal testing is accomplished for the purpose of for estimating the behavior of metal under
loading (tensile, compressive, shear, tortion and impact, cyclic loading etc.) of metal and for
Porperties and Testing of Metals 123
providing necessary data for the product designers, equipment designers, tool and die designers
and system designers. The material behavior data under loading is used by designers for
design calculations and determining weather a metal can meet the desired functional
requirements of the designed product or part. Also, it is very important that the material
shall be tested so that their mechanical properties especially their strength can be assessed
and compared. Therefore the test procedure for developing standard specification of materials
has to be evolved. This necessitates both destructive and non-destructive testing of materials.
Destructive tests of metal include various mechanical tests such as tensile, compressive,
hardness, impact, fatigue and creep testing. A standard test specimen for tensile test is
shown in Fig. 7.2. Non-destructive testing includes visual examination, radiographic tests,
ultrasound test, liquid penetrating test and magnetic particle testing.
R = Fillet Radius
D = Diameter
Fig. 7.2 Tensile test specimen
7.3.1 Tensile test
A tensile test is carried out on standard tensile test specimen in universal testing machine.
Fig. 7.3 shows a schematic set up of universal testing machine reflecting the test
specimen griped between two cross heads. Fig. 7.4 shows the stress strain curve for
ductile material. Fig. 7.5 shows the properties of a ductile material. Fig. 7.6 shows the
stress strain curves for wrought iron and steels. Fig. 7.7 shows the stress strain curve
for non ferrous material.
Operating Hand Wheel
Strain Gauge or
A – Limit of proportionality
B – Elastic limit
C – Yield point
D – Maximum stress point
E – Breaking of fracture point
Fig. 7.3 Schematic universal testing machine Fig. 7.4 Stress strain curve for ductile material
124 Introduction to Basic Manufacturing Processes and Workshop Technology
Fig. 7.5 Properties of a ductile material
Rolled Annealed Copper
Fig. 7.6 Stress strain curves for wrought Fig. 7.7 Stress strain curves for non-ferrous material
iron and steel
7.3.2 Compression Test
Compression test is reverse of tensile test. This test can also be performed on a universal
testing machine. In case of compression test, the specimen is placed bottom crossheads. After
that, compressive load is applied on to the test specimen. This test is generally performed for
testing brittle material such as cast iron and ceramics etc. Fig. 7.8 shows the schematic
compression test set up on a universal testing machine. The following terms have been
deduced using figures pertaining to tensile and compressive tests of standard test specimen.
Hook’s law states that when a material is loaded within elastic limit (up to proportional
limit), stress is proportional to strain.
Strain is the ratio of change in dimension to the original dimension.
Porperties and Testing of Metals 125
Fig. 7.8 Schematic compression test set up on a universal testing machine
The ratio of increase in length to the original length is known as tensile strain.
The ratio of decrease in length to the original length is known as compressive strain.
Modulus of Elasticity
The ratio of tensile stress to tensile strain or compressive stress to compressive strain is
called modulus of elasticity. It is denoted by E. It is also called as Young’s modulus of elasticity.
E = Tensile Stress/Tensile Strain
Modulus of Rigidity
The ratio of sheer stress to shear strain is called modulus of rigidity. It is denoted by G.
G = Shear Stress/Shear Strain
The ratio of direct stress to the volumetric strain (ratio of change in volume to the
original volume is known as volumetric strain) is called Bulk modulus (denoted by K).
K = Direct stress/volumetric strain
Linear and Lateral Strain
When a body is subjected to tensile force its length increases and the diameter decreases.
So when a test specimen of metal is stressed, one deformation is in the direction of force
which is called linear strain and other deformation is perpendicular to the force called lateral
126 Introduction to Basic Manufacturing Processes and Workshop Technology
The ratio of lateral strain to linear strain in metal is called poisson’s ratio. Its value is
constant for a particular material but varies for different materials.
The maximum amount of energy which can be stored in an elastic limit is known as
Modulus of Resilience
The proof resilience per unit volume of a material is modulus of resilience or elastic toughness.
7.3.3 Testing of Hardness
It is a very important property of the metals and has a wide variety of meanings. It embraces
many different properties such as resistance to wear, scratching, deformation and machinability
etc. It also means the ability of a metal to cut another metal. The hardness of a metal may
be determined by the following tests.
(a) Brinell hardness test
(b) Rockwell hardness test
(c) Vickers hardness (also called Diamond Pyramid) test
(d) Shore scleroscope
Fig. 7.9 shows Rockwell hardness testing machine.
2. Indentor holder.
5. Screw wheel.
Fig. 7.9 Rockwell hardness testing machine
7.3.4 Testing of Impact Strength
When metal is subjected to suddenly applied load or stress, it may fail. In order to assess the
capacity of metal to stand sudden impacts, the impact test is employed. The impact test
measures the energy necessary to fracture a standard notched bar by an impulse load and
as such is an indication of the notch toughness of the material under shock loading. Izod test
and the Charpy test are commonly performed for determining impact strength of materials.
These methods employ same machine and yield a quantitative value of the energy required
to fracture a special V notch shape metal. The most common kinds of impact test use notched
specimens loaded as beams. V notch is generally used and it is get machined to standard
specifications with a special milling cutter on milling machine in machine shop. The beams
may be simply loaded (Charpy test) or loaded as cantilevers (Izod test). The function of the
Porperties and Testing of Metals 127
V notch in metal is to ensure that the specimen will break as a
result of the impact load to which it is subjected. Without the
notch, many alloys would simply bend without breaking, and it
would therefore be impossible to determine their ability to absorb
energy. It is therefore important to observe that the blow in Charpy
test is delivered at a point directly behind the notch and in the
Izod test the blow is struck on the same side of the notch towards
the end of the cantilever. Fig. 7.10 shows the impact testing set
up arrangement for charpy test. The specimen is held in a rigid
vice or support and is struck a blow by a traveling pendulum that
fractures or severely deforms the notched specimen. The energy
input in this case is a function of the height of fall and the weight
of the pendulum used in the test setup. The energy remaining
after fracture is determined from the height of rise of the pendulum
due to inertia and its weight. The difference between the energy
input and the energy remaining represents the energy absorbed by
the standard metal specimen. Advance testing setups of carrying out
such experiments are generally equipped with scales and pendulum-
actuated pointers, which provide direct readings of energy absorption.
7.3.5 Testing of Fatique
Material subjected to static and cyclic loading, yield strength is the main criterion for product
design. However for dynamic loading conditions, the fatigue strength or endurance limit of
a material is used in main criteria used for designing of parts subjected to repeated alternating
stresses over an extended period of time. Fig 7.11 shows a fatigue test set up determining
the fatigue strength of material. The fatigue test determines the stresses which a sample of
material of standard dimensions can safely endure for a given number of cycles. It is performed
on a test specimen of standard metal having a round cross-section, loaded at two points as
a rotating simple beam, and supported at its ends. The upper surface of such a standard test
specimen is always in compression and the lower surface is always in tension. The maximum
stress in metal always occurs at the surface, halfway along the length of the standard test
specimen, where the cross section is minimum. For every full rotation of the specimen, a
point in the surface originally at the top centre goes alternately from a maximum in compression
to a maximum in tension and then back to the same maximum in compression. Standard test
specimens are tested to failure using different loads, and the number of cycles before failure
is noted for each load. The results of such tests are recorded on graphs of applied stress
against the logarithm of the number of cycles to failure. The curve is known as S-N curve.
Shut Off Switch
Flexible Coupling Revolution
Fig. 7.11 Schematic fatigue test setup
Fig. 7.10 Schematic impact
testing machine setup
128 Introduction to Basic Manufacturing Processes and Workshop Technology
7.3.6 Testing of Creep
Metal part when is subjected to a high
constant stress at high temperature for
a longer period of time, it will undergo
a slow and permanent deformation (in
form of a crack which may further
propagate further towards creep failure)
called creep. Creep is time dependent
phenomena of metal failure at high
constant stress and at high temperature
such subjecting of at steam turbine
blade. A schematic creep testing setup
is shown in Fig. 7.12. Test is carried
out up to the failure of the test specimen.
A creep curve for high temperature and
long time creep is shown in Fig. 7.13.
The curve shows different portions of
the primary secondary and tertiary
creep which ends at fracture in metals.
Fig. 7.13 Creep curve for a high temperature and long time creep test
7.4 CHOICE OF MATERIALS FOR THE ENGINEERING APPLICATONS
The choice of materials for the engineering purposes depends upon the following factors:
1 Availability of the materials,
2 Properties needed for meeting the functional requirements,
3 Suitability of the materials for the working conditions in service, and
4 The cost of the materials.
7. Instrument for
Fig. 7.12 Schematic creep testing setup
Porperties and Testing of Metals 129
1 Classify the various properties of engineering materials.
2 Explain various physical properties of engineering materials.
3 Explain briefly thermal conductivity and thermal expansion.
4 Explain various mechanical properties of engineering materials.
5 Define various chemical properties of engineering materials.
6 Explain various electrical properties of engineering materials.
7 Define various optical properties of engineering materials.
8 Explain various magnetic, chemical and optical properties of engineering materials.
9 Write short notes on the following:
(a) Elasticity (b) Plasticity (c) Fatigue (d) Creep (e) Toughness.
10 Write short notes on the following:
(a) Malleability, (b) Brittleness, (c) Yield point, (d) Ductility, (e) Wear resistance and
11 Write short notes on the following:
(a) Machinability, (b) Hardness, (c) Stiffness, (d) Weldabilty, (e) Formability, (f) Ductility and
130 Introduction to Basic Manufacturing Processes and Workshop Technology
Heat treatment is a heating and cooling process of a metal or an alloy in the solid state with
the purpose of changing their properties. It can also be said as a process of heating and
cooling of ferrous metals especially various kinds of steels in which some special properties
like softness, hardness, tensile-strength, toughness etc, are induced in these metals for
achieving the special function objective. It consists of three main phases namely (i) heating
of the metal (ii) soaking of the metal and (iii) cooling of the metal. The theory of heat
treatment is based on the fact that a change takes place in the internal structure of metal
by heating and cooling which induces desired properties in it. The rate of cooling is the major
controlling factor. Rapid cooling the metal from above the critical range, results in hard
structure. Whereas very slow cooling produces the opposite affect i.e. soft structure. In any
heat treatment operation, the rate of heating and cooling is important. A hard material is
difficult to shape by cutting, forming, etc. During machining in machine shop, one requires
machineable properties in job piece hence the properties of the job piece may requires heat
treatment such as annealing for inducing softness and machineability property in workpiece.
Many types of furnaces are used for heating heat treatment purposes. The classification of
such heat treatment furnaces is given as under.
8.2 HEAT TREATMENT FURNACES
8.2.1 Hearth Furnaces
These furnaces are heated by fuel which may be coke, coal, gas (town, blast or natural) and
fuel oil. They can also be operated electrically. They are generally of two types.
(a) Stationary type
It consists of four types
(1) Direct fuel fired furnace
(2) Indirect fuel fired furnace
(3) Multiple furnace
(4) Re-circulation furnace
Heat Treatment 131
(b) Movable type
It consists of two types
(1) The car bottom type
(2) The rotary type
8.2.2 Bath Furnaces
In bath type furnaces, heating may be done using by gas, oil or electricity. These furnaces
are further classified as:
(1) Liquid bath type
(2) Salt bath type
(3) Lead bath type
(4) Oil bath type
8.3 CONSTITUENTS OF IRON AND STEEL
Fig. 8.1 shows micro structure of mild steel (0.2-0.3% C). White constituent in this figure is very
pure iron or having very low free carbon in iron in form of ferrite and dark patches contain
carbon in iron is chemically combined form known as carbide (Cementite). Cementite is very
hard and brittle. Now if the dark patches of the above figure are further observed, a substance
built up of alternate layer of light and dark patches is reflected in Fig. 8.2. These layers are
alternatively of ferrite and cementite. This substance is called as pearlite and is made up of 87%
ferrite and 13% cementite. But with increase of carbon content in steel portion of pearlite
increases up to 0.8% C. The structure of steel at 0.8% C is entirely of pearlite. However if carbon
content in steel is further increased as free constituent up to 1.5% C, such steel will be called
as high carbon steel. The micro structure of high carbon steel is depicted in Fig. 8.3.
Fig. 8.1 Micro structure of mild steel Fig. 8.2 Micro structure of Fig. 8.3 Micro structure of
pearlitic eutectoid steel of high carbon steel
8.4 ALLOTROPY OF IRON
In actual practice it is very difficult to trace the cooling of iron from 1600°C to ambient
temperature because particular cooling rate is not known. Particular curve can be traced
from temperature, time and transformation (TTT) curve. However allotropic changes observed
during cooling of pure iron are depicted in Fig. 8.4. When iron is cooled from molten condition
up to the solid state, the major allotropic changing occurs which are:
1539-1600°C Molten-Fe (Liquid state of iron)
1400-1539°C Delta-Fe (Body centered)
132 Introduction to Basic Manufacturing Processes and Workshop Technology
910-1400°C Gamma-Fe (FCC atomic arrangement and austenite structure)
770- 910°C Beta-Fe (Body centered-nonmagnetic)
Up to 770°C Alpha-Fe (BCC atomic arrangement and ferrite structure)
Fig. 8.4 Allotroic changes during cooling of pure iron
(i) First changing occurs at l539°C at which formation of delta iron starts.
(ii) Second changing takes place at 1404°C and where delta iron starts changes into
gamma iron or austenite (FCC structure).
(iii) Third changing occurs at 910°C and where gamma iron (FCC structure) starts
changes into beta iron (BCC structure) in form of ferrite, leadaburite and austenite.
(iv) Fourth changing takes place at 768°C and where beta iron (BCC structure) starts
changes into alpha iron in form of ferrite, pearlite and cementite.
Therefore, the temperature points at which such changing takes place into allotropic
forms are called critical points. The critical points obtained during cooling are slightly lower
than those obtained in heating. The most marked of these range commonly called the point
of recalescence and point of decalescence.
8.5 TRANSFORMATION DURING HEATING AND COOLING OF STEEL
When a steel specimen is heated, its temperature rises unless there is change of state or a
change in structure. Fig. 8.5 shows heating and cooling curve of steel bearing different
structures. Similarly, if heat is extracted, the temperature falls unless there is change in state
or a change in structure. This change of structure does not occur at a constant temperature.
It takes a sufficient time a range of temperature is required for the transformation. This
range is known as transformation range. For example, the portion between the lower critical
temperature line and the upper critical temperature line with hypo and hyper eutectoid
Heat Treatment 133
steels, in iron carbon equilibrium diagram. This range is also known as critical range. Over
heating for too long at a high temperature may lead to excessive oxidation or decarburization
of the surface. Oxidation may manifest itself in the form of piece of scale which may be driven
into the surface at the work piece if it is going to be forged. If steel is heated, well above the
upper critical temperature, large austenite grains form. In other words steel develops
undesirable coarse grains structure if cooled slowly to room temperature and it lacks both in
ductility and resistance to shock.
Austenite 0.5% C
Fig. 8.5 Heating and cooling curve of steel
8.6 IRON-CARBON EQUILIBRIUM DIAGRAM
Fig. 8.6 shows, the Fe-C equilibrium diagram in which various structure (obtained during
heating and cooling), phases and microscopic constituents of various kinds of steel and cast
iron are depicted. The main structures, significance of various lines and critical points are
discussed as under.
8.6.1 Structures in Fe-C-diagram
The main microscopic constituents of iron and steel are as follows:
134 Introduction to Basic Manufacturing Processes and Workshop Technology
1 2 3 4 4.3 5 6 6.7
( + )α γG
δ Fe + liquid
δ iron A
γ Solid Solution
Fig. 8.6 Fe-C equilibrium diagram
Austenite is a solid solution of free carbon (ferrite) and iron in gamma iron. On heating
the steel, after upper critical temperature, the formation of structure completes into austenite
which is hard, ductile and non-magnetic. It is able to dissolve large amount of carbon. It is
in between the critical or transfer ranges during heating and cooling of steel. It is formed
when steel contains carbon up to 1.8% at 1130°C. On cooling below 723°C, it starts transforming
into pearlite and ferrite. Austenitic steels cannot be hardened by usual heat treatment methods
and are non-magnetic.
Heat Treatment 135
Ferrite contains very little or no carbon in iron. It is the name given to pure iron crystals
which are soft and ductile. The slow cooling of low carbon steel below the critical temperature
produces ferrite structure. Ferrite does not harden when cooled rapidly. It is very soft and
Cementite is a chemical compound of carbon with iron and is known as iron carbide
(Fe3C). Cast iron having 6.67% carbon is possessing complete structure of cementite. Free
cementite is found in all steel containing more than 0.83% carbon. It increases with increase
in carbon % as reflected in Fe-C Equilibrium diagram. It is extremely hard. The hardness
and brittleness of cast iron is believed to be due to the presence of the cementite. It
decreases tensile strength. This is formed when the carbon forms definite combinations
with iron in form of iron carbides which are extremely hard in nature. The brittleness and
hardness of cast iron is mainly controlled by the presence of cementite in it. It is magnetic
Pearlite is a eutectoid alloy of ferrite and cementite. It occurs particularly in medium and
low carbon steels in the form of mechanical mixture of ferrite and cementite in the ratio of
87:13. Its hardness increases with the proportional of pearlite in ferrous material. Pearlite is
relatively strong, hard and ductile, whilst ferrite is weak, soft and ductile. It is built up of
alternate light and dark plates. These layers are alternately ferrite and cementite. When seen
with the help of a microscope, the surface has appearance like pearl, hence it is called
pearlite. Hard steels are mixtures of pearlite and cementite while soft steels are mixtures of
ferrite and pearlite.
As the carbon content increases beyond 0.2% in the temperature at which the ferrite is
first rejected from austenite drop until, at or above 0.8% carbon, no free ferrite is rejected
from the austenite. This steel is called eutectoid steel, and it is the pearlite structure in
As iron having various % of carbon (up to 6%) is heated and cooled, the following phases
representing the lines will tell the about the structure of iron, how it charges.
8.6.2 Significance of Transformations Lines
The line ABCD tells that above this line melting has been completed during heating the
iron. The molten metal is purely in the liquidus form. Below this line and above line AHJECF
the metal is partially solid and partially liquid. The solid metal is known as austenite. Thus
the line ABCD represents temperatures at which melting is considered as completed. Beyond
this line metal is totally in molten state. It is not a horizontal line the melting temperature
will vary with carbon content.
This line tells us that metal starts melting at this temperature. This line is not horizontal
and hence the melting temperatures will change with carbon content. Below this line and
above line GSEC, the metal is in solid form and having austenite structure.
136 Introduction to Basic Manufacturing Processes and Workshop Technology
This line occurs near 723°C and is a horizontal line and is known as lower critical
temperature line because transformation of steels starts at, this line. Carbon % has not effect
on it that means steel having different % of carbon will transforms at the same temperature.
The range above the line up to GSE is known as transformation range. This line tells us the
steel having carbon up to 0.8% up to 0.8% will starts transforming from ferrite and pearlite
to austenite during heating.
It is a line at temperature 1130°C which tells that for cast iron having % of C from 2%
to 4.3%. Below this line and above line SK, Cast iron will have austenite + ledeburite and
cementite + ledeburite.
8.6.3 Critical Temperatures
The temperatures at which changes in structure takes place is known as critical temperatures,
these are as follows:
1. The temperature along GSE is known as upper critical temperature. The
temperature along GS during heating as (upper critical temperature) where austenite
+ alpha iron changes into austenite and vice versa.
2. The temperature along GS during cooling as A3 where austenite changes into
austenite + alpha iron and vice versa during heating.
3. The temperature along line SE during heating as Acm changes into austenite from
austenite + cementite and vice versa.
4. The temperature along PSK is known as lower critical temperature when
pearlite changes into austenite on heating as denoted, by A1.
8.6.2 Objectives of Heat Treatment
The major objectives of heat treatment are given as under
1. It relieves internal stresses induced during hot or cold working.
2. It changes or refines grain size.
3. It increases resistance to heat and corrosion.
4. It improves mechanical properties such as ductility, strength, hardness, toughness,
5. It helps to improve machinability.
6. It increases wear resistance
7. It removes gases.
8. It improves electrical and magnetic properties.
9. It changes the chemical composition.
10. It helps to improve shock resistance.
11. It improves weldability.
The above objectives of heat treatment may be served by one or more of the following
heat treatment processes:
Heat Treatment 137
2. Anne aling.
5. Case hardening
6. Surface hardening
(a) Induction hardening,
(b) Flame hardening.
Fig. 8.7 shows the heating temperature ranges for various heat treatment processes.
A Lower critical
Austenite ( -Fe)γ
A Upper critical range
Ferrite + Pearlite
0.2 0.4 0.6 0.8 1.0 1.5 2.0
Pearlite + Cementite
Fig. 8.7 Heating temperature ranges for various heat treatment processes
Normalizing is a defined as softening process in which iron base alloys are heated 40 to 50°C
above the upper-critical limit for both hypo and hyper eutectoid steels and held there for a
specified period and followed by cooling in still air up to room temperature. Fig 8.7 shows the
138 Introduction to Basic Manufacturing Processes and Workshop Technology
heating temperature ranges for normalizing process of both hypo and hyper carbon steel.
Fig. 8.8 shows the structure obtained after normalizing of medium carbon steel.
1. To soften metals
2. Refine grain structure
3. Improve machinability after forging and rolling
4. improve grain size
5. Improve structure of weld
6. Prepare steel for sub heat treatment
It is a softening process in which iron base alloys are heated above the transformation range
held there for proper time and then cool slowly (at the of rate of 30 to 150°C per hour) below
the transformation range in the furnace itself. Heating is carried out 20°C above upper critical
temperature point of steel in case of hypo eutectoid steel and the same degree above the
lower critical temperature point in case of type eutectoid steel. Fig 8.7 shows the heating
temperature ranges for annealing or softening process of both hypo and hyper carbon steel.
Fig. 8.9 shows the structure obtained after annealing of medium carbon steel. The structure
of steel on slow cooling changes into ferrite and pearlite for hypo eutectoid steel, pearlite for
eutectoid steel and pearlite and cementite for hyper eutectoid steel. The time for holding the
article in furnace is ½ to 1 hour. As ferrous metals are heated above the transformation
range, austenite structure will be attained at this temperature.
For a particular type of structure specific cooling rate is required to have good annealing
properties for free machining. As metal is slowly cooled after heating and holding in and with
the furnace and buried in non conducting media such sand, lime or ashes, carbon steels are
cooled down at particular rate normally 150-200°C per hour while alloy steel in which austenite
is very stable and should be cooled much lower (30°C to 100°C per hour). Very slow cooling
is required in annealing to enable austenite to decompose at two degrees of super cooling so
as to form a pearlite and ferrite structure in hypo-eutectoid steel, a pearlite structure in
eutectoid steel and pearlite and cementite structure in hyper eutectoid steel. In successfully
annealed steel, the grains of ferrite are large and regular while pearlite consists of cementite
and ferrite. Hypo-eutectoid hot worked steel may under go full annealing to obtain coarse
grain structure for free machining. When steel is cold worked the hardness (Brinell hard)
considerably increases and ductility decreases slightly. The ductility of steel may be then
restored by so called recrystallisation or process annealing.
8.9.1 Objectives of Annealing
The purpose of annealing is to achieve the following
1. Soften the steel.
2. Relieve internal stresses
3. Reduce or eliminate structural in-homogeneity.
4. Refine grain size.
5. Improve machinability.
6. Increase or restore ductility and toughness.
Heat Treatment 139
Annealing is of two types
(a) Process annealing
(b) Full annealing.
In process annealing, ductility is increased with somewhat decrease in internal stresses.
In this, metal is heated to temperature some below or close to the lower critical temperature
generally it is heated 550°C to 650°C holding at this temperature and it is slowly cooled. This
causes completely recrystallisation in steel.
The main purpose of full annealing of steel is to soften it and to refine its grain
structure. In this, the hypo-eutectoid steel is heated to a temperature approximately 20°
to 30°C above the higher critical temperature and for hypereutectoid steel and tool steel
is heated to a temperature 20 to 30°C above the lower critical temperature and this
temperature is maintained for a definite time and then slowly cooed very slow1y in the
It is lowest temperature range of annealing process in which iron base alloys are heated 20
to 40°C below the lower critical temperature, held therefore a considerable period of time e.g.
for 2.5 cm diameter piece the time recommended is four-hours. It is then allowed to cool very
slowly at room temperature in the furnace itself. Fig 8.7 shows the heating temperature
ranges for spheroidizing process of carbon steel. Fig. 8.9 shows the structure obtained after
annealing of carbon steel. During this process, the cementite of steel which is in the combined
form of carbon becomes globular or spheroidal leaving ferrite in matrix, thus imparting
softness to steel. After normalizing of steels, the hardness of the order of 229 BHN and as
such machining becomes difficult and hence to improve machining, these are spheroidised
first and then machined. This treatment is carried out on steels having 0.6 to 1.4% carbon.
The objectives of spheroidising are given as under.
Fig. 8.8 Structure of normalized Fig. 8.9 Structure of annealed
medium carbon steel medium carbon steel
1. To reduce tensile strength
2. To increase ductility
3. To ease machining
4. To impart structure for subsequent hardening process
8.11 COMPARISON BETWEEN ANNEALING AND NORMALISING
The comparison between annealing and normalizing is given as under in Table 8.1.
140 Introduction to Basic Manufacturing Processes and Workshop Technology
Table 8.1 Comparison between Annealing and Normalising
S.No. Annealing Normalising
1 In this hypo-eutectoid steel is heated to a In this metal is heated 30 to 50°C above
temperature approximately 20 to 30°C above higher critical temperature.
temperature the higher critical temperature
and for hypereutectoid steel is heated 20 to
30°C above the lower c